393 91 17MB
English Pages 544 Year 2009
This book provides students of civil engineering and architecture with a grounding in the fundamentals of structures, an
411 101 3MB Read more
This practical step-by-step guide - designed for use at your computer - gives clear, compact instructions and self-test
441 29 163KB Read more
344 42 2MB Read more
This volume combines the chemistry and materials science of nanomaterials and biomolecules with their detection strategi
334 85 5MB Read more
Semiconductors play a major role in modern microtechnology, especially in microelectronics. Since the dimensions of new
301 45 8MB Read more
Seismic Design for Architects shows how structural requirements for seismic resistance can become an integral part of th
605 46 7MB Read more
Nanomaterials Design for Sensing Applications examines chemosensors, beginning with molecules that are able to respond t
334 32 53MB Read more
Whether a website, marketing campaign, museum exhibit, a video game or a complex control system, the design we see is th
359 54 10MB Read more
Following an overview of nanotechnologies for diagnostic purposes, this book goes on to look at nanoparticle-based magne
375 107 7MB Read more
Butterworth-Heinemann is an imprint of Elsevier 30 Corporate Drive, Suite 400, Burlington, MA 01803, USA Linacre House, Jordan Hill, Oxford OX2 8DP, UK Copyright © 2009, Elsevier Ltd. All rights reserved. No part of this publication may be reproduced, stored in a retrieval system, or transmitted in any form or by any means, electronic, mechanical, photocopying, recording, or otherwise, without the prior written permission of the publisher. Permissions may be sought directly from Elsevier’s Science & Technology Rights Department in Oxford, UK: phone: (+44) 1865 843830, fax: (+44) 1865 853333, E-mail: [email protected] You may also complete your request online via the Elsevier homepage (http://elsevier.com), by selecting “Support & Contact” then “Copyright and Permission” and then “Obtaining Permissions.” Library of Congress Cataloging-in-Publication Data Application submitted British Library Cataloguing-in-Publication Data A catalogue record for this book is available from the British Library. ISBN: 978-0-7506-8149-0 For information on all Butterworth–Heinemann publications visit our Web site at www.elsevierdirect.com Printed in China 09 10 11 12 13
10 9 8 7 6 5 4 3 2 1
Working together to grow libraries in developing countries www.elsevier.com | www.bookaid.org | www.sabre.org
There is currently an extraordinary amount of interest in nanomaterials and nanotechnologies, terms now familiar not only to scientists, engineers, architects, and product designers but also to the general public. Nanomaterials and nanotechnologies have been developed as a consequence of truly significant recent advances in the material science community. Their use, in turn, is expected to have enormous consequences on the design and engineering of everything from common consumer products and buildings all the way through sophisticated systems that support a wealth of applications in the automotive, aerospace, and other industries. Hopes exist for being able to make things smaller, lighter, or work better than is possible with conventional materials. Serious problems facing society might also be positively addressed via the use of nanomaterials and nanotechnologies. In the energy domain, for example, nano-based fuel cells or photovoltaics can potentially offer greater efficiencies than are possible with conventional materials. Developments in nanomaterials and nanotechnologies have consequently aroused the interest of many individuals involved in engineering, architecture, and product design, whether in the automotive, building, or even the fashion industries. In the excitement surrounding these new materials and technologies, however, their potential can, and has been, frequently overhyped. A mystique surrounds these words that can cloud understanding of what nanomaterials and nanotechnologies really are and what they can deliver. One of the purposes of this book is to demystify the subject and distinguish what is real from what is not. Though there is a need to better understand what benefits and costs might be associated with using nanomaterials, in the design fields little true understanding exists about what these new materials and technologies actually are and how they might be used effectively. In the science and engineering domain the situation is often the converse. The fundamental science-based knowledge is
there, but not necessarily an understanding of how these materials and technologies might be used to address real societal needs or, more simply, to provide a basis for useful applications—a situation often best described by the classic phrase “a technology looking for an application.” Relatively few applications in architecture and product design exist at this point, so there are few role models or case studies to explore. Still, the core belief reflected in this book is that nanomaterials and nanotechnologies do offer new ways of addressing many current needs as well as providing the basis for a positive vision for future developments. The book explores these kinds of forward-looking potential applications. The field is clearly in an emerging state, but its potential is evident. The question is one of how to move forward. The position reflected in this book is that this can only be accomplished by designers, engineers, and material scientists working together. Yet simply suggesting that these groups “collaborate” is usually ineffective. There needs to be a common basis for communication and idea exchange. The language of understanding spoken by one group can be foreign to the other. Within this context, a primary goal of this book is to provide both a common ground and a common language for better understanding how to use nanomaterials and nanotechnologies effectively. It seeks to convey the necessary technical understanding of the essential ideas underlying these new materials and technologies to designers so that they might better be able to understand how to exploit their characteristics effectively within a design context. At the same time it seeks to introduce material scientists and engineers knowledgeable about nanomaterials to design issues and design processes. What design problems need to be solved, and how do designers think about solving them? Only with this mutual understanding can they effectively become engaged in developing meaningful applications. To meet these aspirations, the scope of the book is inherently large, seeking to explore what nanomaterials and nanotechnologies are and how they might be applied in diverse industries. However, though the scope is large, the approach followed in this book is based on the well-explored premise that most effective design applications occur when there is a true in-depth understanding of the materials or technologies involved and not when an overly simplified approach is taken wherein discussions of technological issues are reduced to an almost meaningless state. The book has many unique features. It summarizes discussions of many different ideas and technologies normally found distributed
all across the literature. A case in point occurs in Chapter 8 of this book, which presents coverage of the many different synthesis processes used for making nanomaterials. There are many indepth discussions throughout the literature of specific synthesis methods, such as soft lithography or sol-gel deposition methods, but these same discussions do not comprehensively cover other techniques. The approach here is to explore all primary methods of nanosynthesis and the mechanical, thermal, optical, and electrical properties they create—a comprehensive view that will be welcomed by teachers of engineering and material scientists. A broad knowledge of resulting properties is important, too, for any designer or engineer trying to use nanomaterials. It can be difficult to locate real values for properties of nanomaterials; a mechanical property may be reported in one source, a thermal property in another. In writing this book, considerable effort was put into sifting through the literature to identify credible values for primary properties. Even once some of these properties are known, experience in the design world suggests that these values have to be placed in comparison to more traditional materials before they will be used, particularly given the higher costs of nano-based materials. A good way to explore materials and to select them to meet specific design objectives is to present their properties as “material property charts.” These charts give a graphical overview of material attributes and allow comparisons to be made between them, as well as serving as a basis for more advanced material selection and related design techniques. Critical properties of various nanomaterials have now been incorporated into these kinds of charts, facilitating an understanding of where and how to effectively use nanomaterials within a design context. In a broader sense, another unique feature of the book is the overall orientation to applications. Discussions are focused around thinking about products and buildings via the nature of the involved physical environments, systems, and assemblies. Environments may alternatively be considered either as an integral part of a design, such spaces as within a building, or as defining the context within which a product operates or is reflective of its salient mode of operation. Systems are generally defined as physical components or parts that work interactively to provide some particular type of function. In both products and buildings, broad considerations of thermal, sound, lighting, and mechanical environments and their related functional systems are invariably important and invariably influence the definition of needed material properties; consequently
they influence the role that nanomaterials and nanotechnologies might or might not effectively play. This kind of perspective reflects the way designers think about how and where to introduce new materials or technologies—a perspective that would be well worth scientists and engineers interested in applications of nanomaterials knowing something about. The book is organized in a direct way and makes extensive use of illustrations. The first two chapters are self-contained nontechnical overviews of the general characteristics of nanomaterials and provide examples of ways in which nanomaterials can be found in both nature and in an historical context. Chapter 3 sets the broad design context and explores fundamental design processes. Chapter 4 then reviews basic technical properties of materials as a prelude for focusing on nanomaterials. This is followed in Chapter 5 by an introduction to material property charts, material indices, and their use for optimized material selection. Formal material screening and selection procedures are also presented, providing a methodology for comparing the benefits of using nanomaterials to other kinds of more traditional high-performance materials. This introduction leads into an in-depth treatment of nanomaterials that begins in Chapter 6. A major contribution here is that of clarifying ways that various nanomaterial types can be formally classified. Size effects and other defining characteristics of nanomaterials are explored. Specific mechanical, thermal, and electrical properties of common nanomaterial types are detailed in Chapter 7. Processes for synthesizing and characterizing nanomaterials are next described and illustrated in Chapter 8. Several material property charts illustrating various properties of nanomaterials are included. The book then turns to design or application-oriented considerations. A discussion of specific applications in common design environments—thermal, mechanical, electrical, and optical—follows in Chapter 9. These sections broadly explore a range of nanomaterial and nanotechnology applications as they relate to these different design environments. Chapter 10 looks at applications from specific product or industry perspectives—nanotextiles, nanopaints, nanosealants, nanotechnologies for self-cleaning, antimicrobial or self-healing, and others. Chapter 11 briefly examines nanomaterials in relation to health and the environment. Chapter 12 concludes with a whirlwind tour of the driving forces underlying nanomaterial and nanotechnology developments in several industries.
The target audience for this book includes students in engineering and architecture, professional engineers, architects, and product designers who are interested in exploring how these new materials and technologies might result in better products or buildings. Firms and industry groups who are planning to be intimately involved in the nanotechnology field will find the broad perspective interesting. Obviously, individuals in these fields have quite different backgrounds, interests, and understanding of materials and their properties as well as technologies. Having a single book address these multiple audiences is inherently difficult. Designers have primary goals of making products and buildings interesting, efficient, and useful, with materials being an important enabling design component. Their interests revolve more around final design qualities and applications than on achieving a quantitative understanding of materials and their properties. Many designoriented engineers have similar interests but are more focused on the way material properties affect design, and they employ quantitative methods to achieve these ends. Material engineers and scientists are clearly interested in fundamental properties and how to create new materials for broad usage. Therefore, depending on the reader’s background, the following two paragraphs suggest general guidelines on how to read this book. In the field of engineering, second- or third-year undergraduate students and first-year graduate students will find the book useful as supplementary reading. These students should find familiar ground in the more technically oriented discussions of basic material properties in Chapter 4, as will engineers in firms. Chapter 5 on material selection processes based on material attribute charts will be of great interest to any who have never been exposed to this approach before and will provide a concise review for those who have already used them. Chapters 6, 7, and 8 provide a good introduction to classification systems, basic fundamentals, synthesis, characterization methods, and properties of nanomaterials—information that is currently scattered among many sources and difficult to find in one place. Obviously, whole in-depth courses could be built around many of the topics succinctly addressed in these chapters. The intent, however, is to provide a solid conceptual understanding of these topics, not to go into depth. Individuals interested in further depth should refer to the entries described in “Further Readings.” The application-oriented sections in Chapters 9, 10, 11, and 12 provide overviews of ways that nanomaterials and nanotechnologies are either used or poised to be used in practice. Engineers and material scientists not actively engaged in design practices
will benefit from reviewing these chapters as a way of understanding what material characteristics are needed and considered useful by the design community. Some of the basic ways designers conceptualize the use of materials in products and buildings are also introduced in Chapter 3, which is useful reading for anyone who does not have a design background. Architects and product designers range widely in their interests and need to understand material properties in depth. For typical architects in firms or students who have had basic courses in materials and who have a general curiosity about nanomaterials and how they might ultimately impact design, quantitative treatments are rarely needed. Chapters 1, 2, and 3 provide an insight into what nanomaterials are all about and are useful here. Chapter 5 on material selection processes is highly relevant to designers. Chapters 9, 10, 11, and 12 contain discussions on nanomaterials that are particularly appropriate for the design community. These chapters contain only qualitative technical descriptions and should be generally accessible to all interested readers. Many designers, however, are indeed quite technically inclined and have focused interests on materials and on technologically based innovations and are willing to put in the time necessary to understand them in some depth. This group would indeed find it useful to review the chapters on basic nanomaterial types and processing methods mentioned previously. Indeed, it is to this group that the design focus in this book is largely oriented, not to the casual reader. We hope that you enjoy the book! Mike Ashby Engineering Design Centre Engineering Department Cambridge University Paulo Ferreira Materials Science and Engineering Program University of Texas at Austin Daniel Schodek Graduate School of Design Harvard University
The authors would like to thank students Mr. Joshua Sahoo for his dedicated work in collecting and analyzing the data required to build the chart diagrams containing nanomaterials; and Alda Black, Elizabeth Bacon, Nathan Fash, Ben Schodek, Xue Zhou and others who helped draw many of the figures. For some of the transmission electron microscopy images, the authors would like to acknowledge the use of the Microscopy Facilities at the High Temperature Materials Laboratory (HTML) at Oak Ridge National Laboratory. The research was sponsored by the Assistant Secretary for Energy Efficiency and Renewable Energy, Office of FreedomCAR and Vehicle Technologies, as part of the High Temperature Materials Laboratory User Program, Oak Ridge National Laboratory, managed by UT-Batelle, LLC, for the U.S Department of Energy under contract number DE-AC05OO0R22725.
CH A PTER 1
Nanomaterials and Nanotechnologies: An Overview
Imagine dissociating a human body into its most fundamental building blocks. We would collect a considerable portion of gases, namely hydrogen, oxygen, and nitrogen; sizable amounts of carbon and calcium; small fractions of several metals such as iron, magnesium, and zinc; and tiny levels of many other chemical elements (see Table 1.1). The total cost of these materials would be less than the cost of a good pair of shoes. Are we humans worth so little? Obviously not, mainly because it is the arrangement of these elements and the way they are assembled that allow human beings to eat, talk, think, and reproduce. In this context, we could ask ourselves: What if we could follow nature and build whatever we want, atom by atom and/or molecule by molecule? In 1959, Physics Nobel Laureate Richard Feynman gave a talk at Caltech on the occasion of the American Physical Society meeting. The talk was entitled, “There’s Plenty of Room at the Bottom.” In this lecture, Feynman said: What I want to talk about is the problem of manipulating and controlling things on a small scale … What are the limitations as to how small a thing has to be before you can no longer mold it? How many times when you are working on something frustratingly tiny like your wife’s wrist watch have you said to yourself, “If I could only train an ant to do this!” What I would like to suggest is the possibility of training an ant to train a mite to do this … A friend of mine (Albert R. Hibbs) suggests a very interesting possibility for relatively small machines. He says that, although it is a very wild idea, it would be interesting in surgery if you Nanomaterials, Nanotechnologies and Design Copyright 2009 Elsevier Ltd. All rights of reproduction in any form reserved.
2 CHAPTER 1
Nanomaterials and Nanotechnologies: An Overview
Approximate Chemical Composition of a 70 Kg Human Body
Number of Atoms
Number of Atoms
4.22 × 1027
3 × 1020
1.61 × 1027
2 × 1020
8.03 × 1026
1 × 1020
3.9 × 1025
1 × 1020
1.6 × 1025
1 × 1020
9.6 × 1024
8 × 1019
2.6 × 1024
5 × 1019
2.5 × 1024
4 × 1019
2.2 × 1024
2 × 1019
1.6 × 1024
2 × 1019
4.7 × 1023
2 × 1019
3.9 × 1023
7 × 1018
8.3 × 1022
6 × 1018
4.5 × 1022
6 × 1018
2.1 × 1022
6 × 1018
2.2 × 1021
3 × 1018
2.2 × 1021
3 × 1018
2 × 1021
3 × 1018
1 × 1021
8 × 1017
7 × 1020
2 × 1017
3 × 1020
8 × 1010 Total = 6.71 × 1027
Adapted from R. Freitas Jr., in Nanomedicine, Volume I: Basic Capabilities, Landes Bioscience, 1999, http://www.nanomedicine.com/NMI. htm.
could swallow the surgeon. You put the mechanical surgeon inside the blood vessel and it goes into the heart and “looks” around. It finds out which valve is the faulty one and takes a little knife and slices it out.
Although Feynman could not predict it, this lecture was to become a central point in the field of nanotechnology, long before anything related with the word nano had emerged. Feynman’s vision was amazing, particularly if we consider that a broad spectrum of
Why Nanomaterials? 3
FIGURE 1.1 Sequence of images showing the various levels of scale. (Adapted from Interagency Working Group on Nanoscience, Engineering and Technology, National Science and Technology Council Committee on Technology, “Nanotechnology: Shaping the World Atom by Atom.” Sept.1999.)
Increasing size Nanomaterial range
Individual atoms, < 1nm
DNA, 2.5 nm
Biological, > 1000 nm
Pinhead, 1,000,000 nm
Human, 2,000,000,000 nm
currently mature scientific and engineering areas are based on concepts described in Feynman’s lecture 50 years ago. The term nanotechnology was first used in 1974 by Norio Taniguchi to refer to the precise and accurate tolerances required for machining and finishing materials. In 1981, K. E. Drexler, now at the Foresight Nanotech Institute for Molecular Manufacturing, described a new “bottom-up” approach, instead of the top-down approach discussed earlier by Feynman and Taniguchi. The bottom-up approach involved molecular manipulation and molecular engineering to build molecular machines and molecular devices with atomic precision. In 1986, Drexler published a book, Engines of Creation, which finally popularized the term nanotechnology. The term nano derives from the Greek word for dwarf. It is used as a prefix for any unit such as a second or a meter, and it means a billionth of that unit. Hence, a nanometer (nm) is a billionth of a meter, or 10−9 meters. To get a perspective of the scale of a nanometer, observe the sequence of images shown in Figure 1.1. Despite the wide use of the word nanotechnology, the term has been misleading in many instances. This is because some of the technology deals with systems on the micrometer range and not on the nanometer range (1–100 nm). Furthermore, the research frequently involves basic and applied science of nanostructures and not basic or applied technology. Nanomaterials are also not undiscovered materials, but nanoscale forms of well-known materials such as gold, silver, platinum, iron and others. Finally, it is important to keep in mind that some past technology such as, for example, nanoparticles of carbon used to reinforce tires as well as nature’s photosynthesis would currently be considered a form of nanotechnology. Photosynthesis is in fact an excellent example of the role of nanostructures in the world’s daily life. Leaves contain millions of chloroplasts, which
4 CHAPTER 1
Nanomaterials and Nanotechnologies: An Overview
make a green plant green (see Figure 1.2). Inside each chloroplast, hundreds of thylakoids contain light-sensitive pigments. These pigments are molecules with nanoscale dimensions that capture light (photons) and direct them to the photo reaction centers. At every reaction center, there are light-sensitive pigments that execute the actual photon absorption. When this happens, electrons become excited, which triggers a chain reaction in which water and carbon dioxide are turned into oxygen and sugar.
FIGURE 1.2 A green leaf is composed of chloroplasts inside which photosynthesis occurs.
What is so special about nanotechnology? First, it is an incredibly broad, interdisciplinary field. It requires expertise in physics, chemistry, materials science, biology, mechanical and electrical engineering, medicine, and their collective knowledge. Second, it is the boundary between atoms and molecules and the macro world, where ultimately the properties are dictated by the fundamental behavior of atoms. Third, it is one of the final great challenges for humans, in which the control of materials at the atomic level is possible. So, are nanoscience and nanotechnology real, are they still fiction? During the 1990s Drexler’s book Engines of Creation inspired many science fiction writers to think about the prospects of nanotechnology. For example, in the episode “Evolution” of Star Trek, a boy releases “nanites,” which are robots at the nanoscale fabricated to work in living cells. These machines end up evolving into intelligent beings that gain control the starship Enterprise. In the book Queen of Angels, humans with psychological problems can be treated by an injection of nanodevices. These fictional ideas could become reality if in the future we become able to control matter at the atomic or molecular level. Yet, some skeptical questions may arise, such as: ■
Are molecular entities stable?
Are quantum effects an obstacle to atomic manipulation?
Is Brownian motion a significant effect in nanocomponents?
Are friction and wear relevant for nanocomponents?
The answer to the first question is yes. The human population is the best living example. Each human being contains approximately 1027 atoms that are reasonably stable, and due to cellular multiplication, the human body is able to build itself using molecular mechanisms. With respect to the quantum effects, the uncertain atomic position (∆x) can be estimated from classical vibrational frequency calculations. As discussed by R. Freitas in his book Nanomedicine, for a carbon atom in a single C-C bond, ∆x is approximately 5% of the electron cloud diameter. Hence, the manipulation of nano-
Why Nanomaterials? 5
structures should not be affected by quantum effects. In terms of Brownian motion, we should consider the nanocomponents as harmonic oscillators. In this context, molecular collisions are as likely to absorb energy as to release it, and thus no net effect is expected. Finally, in regard to friction and wear effects at the nanoscale, the repulsive fields between the molecules should provide the necessary lubrication. Products such as oil should be avoided because they cause contamination. For example, a molecular bearing of 2 nm rotating at 1 MHz dissipates about 10−6 picowatts due to friction, whereas a micron-size mechanical component dissipates 1–1000 picowatts (R. Freitas, Nanomedicine). In general, the skeptical questions we’ve posed can be disqualified because so far, nanotechnology does not seem to violate any physical law. What are the possible approaches to making nanomaterials and nanotechnologies? There are basically two routes: a top-down approach and a bottom-up approach. The idea behind the topdown approach is the following: An operator first designs and controls a macroscale machine shop to produce an exact copy of itself, but smaller in size. Subsequently, this downscaled machine shop will make a replica of itself, but also a few times smaller in size. This process of reducing the scale of the machine shop continues until a nanosize machine shop is produced and is capable of manipulating nanostructures. One of the emerging fields based on this top-down approach is the field of nano- and micro-electromechanical systems (NEMS and MEMS, respectively). MEMS research has already produced various micromechanical devices, smaller than 1 mm2, which are able to incorporate microsensors, cantilevers, microvalves, and micropumps. An interesting example is the microcar fabricated by Nippondenso Co. (see Figure 1.3). The car is 4800 µm long, 1800 µm wide, and 1800 µm high. Each tire is 690 µm diameter and 170 µm wide, whereas the license plate is 10 µm thick. The car has 24 components, including tires, wheels, axles, bumpers, all parts assembled by a micromechanical manipulator. Which technologies can be used to produce nanostructures using a top-down approach? At the moment, the most used is photolithography. It has been used for a while to manufacture computer chips and produce structures smaller than 100 nm. This process is discussed extensively in Chapter 8. Typically, an oxidized silicon (Si) wafer is coated with a 1µm thick photoresist layer. After exposure to ultraviolet (UV) light, the photoresist undergoes a photochemical reaction, which breaks down the polymer by rupturing the polymer chains. Subsequently, when the wafer is rinsed in a developing solution, the exposed areas are removed. In this fashion, a pattern
FIGURE 1.3 Microcar produced by Nippondenso Co. The latest model has a micromotor 1 mm in diameter. With power supplied by a 25 micron copper wire, the car runs smoothly at a speed of about 1 cm/s with 3 V voltage and 20 mA current. (Courtesy of Nippondenso.)
6 CHAPTER 1
Nanomaterials and Nanotechnologies: An Overview
is produced on the wafer surface. The system is then placed in an acidic solution, which attacks the silica but not the photoresist and the silicon. Once the silica has been removed, the photoresist can be etched away in a different acidic solution. Though the concept of photolithography is simple, the actual implementation is very complex and expensive. This is because (1) nanostructures significantly smaller than 100 nm are difficult to produce due to diffraction effects, (2) masks need to be perfectly aligned with the pattern on the wafer, (3) the density of defects needs to be carefully controlled, and (4) photolithographic tools are very costly, ranging in price from tens to hundreds of millions of dollars. As a response to these difficulties, electron-beam lithography and X-ray lithography techniques have been developed as alternatives to photolithography. In the case of electron beam lithography, the pattern is written in a polymer film with a beam of electrons. Since diffraction effects are largely reduced due to the wavelength of electrons, there is no blurring of features, and thus the resolution is greatly improved. However, the electron beam technique is very expensive and very slow. In the case of X-ray lithography, diffraction effects are also minimized due to the short wavelength of X-rays, but conventional lenses are not capable of focusing X-rays and the radiation damages most of the materials used for masks and lenses. Due to these limitations, the most recent lithography methods, such as printing, stamping, and molding, use mechanical processes instead of photons or electrons. These methods are normally called soft lithography methods because they involve the use of polymers. They are discussed in Chapter 8. The process starts with the fabrication of a mold by photolithograpy or e-beam lithography. Subsequently, a chemical precursor to polydimethylfiloxane (PDMS) is applied over the mold and cured. As a result, a solid PDMS stamp that matches the pattern of the mold is produced. The stamp can then be used in several ways to make structures at the nanoscale. For example, in the case of microcontact printing the stamp is coated with a solution consisting of organic molecules (thiol ink) and compressed into a thin film of gold (Au) deposited on a silicon (Si) wafer. In this fashion the thiol ink is transferred from the stamp to the gold surface, reproducing the original pattern of the stamp. In the case of micromolding, the PDMS stamp sits on a flat, hard surface and a liquid polymer is injected into any available cavity between the stamp and the surface. Subsequently, the polymer cures into the patterns provided by the cavities. The advantages of using soft lithography methods are (1) no special equipment is required, and (2) versatility in the range of materials
Why Nanomaterials? 7
and geometries produced. As for disadvantages, due to the inherent presence of polymers, soft lithography processes often exhibit significant strains that are not ideal for certain applications, such as nanoelectronics. From the discussion so far, it is obvious that the top-down approach is not a friendly, inexpensive, and rapid way of producing nanostructures. Therefore, a bottom-up approach needs to be considered. The concept of the bottom-up approach is that one starts with atoms or molecules, which build up to form larger structures. In this context, there are three important enabling bottom-up technologies, namely (1) supramolecular and molecular chemistry, (2) scanning probes, and (3) biotechnology. The supramolecular and molecular chemistry route is based on the concept of selfassembly. This is a strategy for nanofabrication that involves designing molecules so that they aggregate into desired structures. The advantages of self-assembly are that (1) it solves the most difficult steps in nanofabrication, which involve creating small structures; (2) it can directly incorporate and bond biological structures with inorganic structures to act as components in a system, and (3) it produces structures that are relatively defect-free. One of the best examples of self-assembly is the fabrication of carbon nanotubes. These nanostructures are composed of C atoms that assemble into cylinders of approximately 1.4 nm in diameter (see Figure 1.4). In the last decade, the idea of using carbon nanotubes to fabricate simple gears evolved by bonding ligands onto the external surfaces of carbon nanotubes to produce “gear teeth” (see Figure 1.5). The efficiency of these gears depends on placing the gear teeth just right in atomically precise positions. Researchers at the National Aeronautics and Space Administration (NASA) performed a molecular dynamics simulation to investigate the properties of molecular gears made from carbon nanotubes. Each gear is made of a 1.1 nm diameter nanotube with seven benzene teeth. The distance between two nanotubes is 1.8 nm. The simulations show that the gears can operate up to 70 GHz without overheating. As speed increases above 150 GHz, the gears overheat and begin to stall. Another very important bottom-up approach using molecular chemistry is employed in the fabrication of quantum dots. Quantum dots are crystals composed of a few hundred atoms. Because electrons in a quantum dot are confined to widely separated energy levels, the dots emit only one type of wavelength of light when they are excited (see Figure 1.6). A typical procedure used to make quantum dots involves a chemical reaction between a metal
FIGURE 1.4 Computer simulation of a single-wall carbon nanotube with a diameter of 1.4 nm. Carbon nanotubes can be thought of as wrapped sheets of graphene.
FIGURE 1.5 Computer simulation of nanogears made of carbon nanotubes with teeth added via a benzine reaction. (Courtesy of NASA.)
8 CHAPTER 1
Nanomaterials and Nanotechnologies: An Overview
FIGURE 1.6 Cadmium selenide (CdSe) quantum dots of different sizes and shapes in solution emit light at different wavelengths. (Courtesy of M. J. Bawendi, MIT.)
ion—cadium (Cd), for example—and a molecule that is able to donate a selenium ion. This reaction generates crystals of cadmium selenide (CdSe). The shape and size of quantum dots can be controlled by tuning the ratio of the molecules and by adding surfactants. Their size and shape are important because they determine their electronic, magnetic, and optical properties.
FIGURE 1.7 Xenon atoms arranged on a Ni substrate by a scanning tunneling probe, forming the word IBM. (Courtesy of IBM.)
The second important bottom-up method is the use of scanning probes. One of the biggest steps toward nanoscale control occurred in 1981 when researchers at the IBM research center in Switzerland, led by Gerd Binning and Heinrich Rohre, developed the scanning tunneling microscope (STM). The STM is, essentially, a fine tip that scans over a material’s surface. Since the tip is only a few atoms wide, electrons “tunnel” across the gap between the surface and the tip as the tip sweeps over the surface (see Chapter 8). In this way scientists developed several related instruments, now known as scanning probe microscopes (SPMs), to collect images and analyze the identities of atoms on a material’s surface. At the moment, SPMs can do more than simply look at atoms. They can also be used to move atoms. At IBM, Donald Eigler and Erhard Schweizer were able to displace 35 xenon atoms onto a crystal of Ni and write the word IBM (see Figure 1.7). These tools have opened up many new doors for further scientific discovery. The third relevant route for producing nanostructures using a bottom-up approach is the use of biotechnology. By 1998, biotechnologists were able to make DNA sequences and assemble artificial viruses, which are examples of molecular engineering. In addition, several devices, which looked like biomolecular motors, sensors, and actuators, could be integrated into systems made of molecular machines. One of the best biological examples of a molecular machine is the ribosome, which is a remarkable nanoscale assembler. The role of the ribosome is to act as a factory of proteins by combining amino acids in a very specific order. Section 2.2 discusses ribosome self-assembly methods in more detail.
Why Nanomaterials? 9
Another good example of self-assembly is the abalone (see Figure 1.8), an expensive appetizer in fine restaurants. This mollusk builds a strong shell by secreting proteins, which self-assemble into a configuration that resembles walls surrounding a room. Inside each room there is seawater saturated with calcium (Ca) ions and carbonate ions, which will eventually form crystals of CaCO3 (calcium carbonate). Therefore the abalone shell is a composite material composed of alternating layers of calcium carbonate and proteins. As we have seen so far, both the top-down and the bottom-up approaches are capable of producing nanostructures, which will soon be applied in many of the engineering fields. One area of great interest for the application of nanostructures is the area of nanoelectronics. In 1985, Konstantin K. Likharev, a professor at Moscow State University, postulated that it would be possible to control the flow of single electrons in and out of a coulomb island. This would form the groundwork for the single-electron transistor, which was first built successfully in 1987 by researchers at Bell Labs. This phenomenon can be very useful in situations where electrical currents are passed through molecules that can act like coulomb islands, for example, if they are weakly coupled to electrodes, which will transfer the signal to the macro world. It has also been proposed that organic molecules could make good transistors. It has already been demonstrated that clusters of molecules can carry electrons from one metal electrode to another. Each molecule is about 0.5 nm wide and 1 to 2 nanometers long. The switching mechanism that allows the molecules to act as transistors seems to involve a chemical reaction, where electrons move among the various atoms within the molecule. Under certain conditions, the chemical reaction twists the molecule, preventing the flow of the electrons. On the other hand, in the absence of the reaction, the molecule will conduct electrons. One other area of increasing interest for the application of nanomaterials is the field of nanomedicine. All of biology, even the most complicated creature, is made up of small cells that are constructed of building blocks at the nanoscale, such as proteins, lipids, and nucleic acids. There is, for example, the story of some bacteria that live in swampy waters. These bacteria can only survive in specific depths. Very close to the surface, oxygen is too abundant; too deep, oxygen is limited. So, how can the bacteria know their position? The answer lies on a string of about 20 ferromagnetic crystals, each 35–120 nm in diameter (see Figure 1.9), which act together as a compass needle influenced by the Earth’s magnetic field. Why are
FIGURE 1.8 The abalone, a marine mollusk whose shell is composed of calcium carbonate layers separated by a protein.
FIGURE 1.9 A magnetotactic bacteria containing a chain of magnetic crystals 35–120 nm in diameter is capable of orienting itself along Earth’s magnetic field lines. (Courtesy of Prozorov et al., Physical Review B, 76, 054406, 2007.)
10 CHAPTER 1
Nanomaterials and Nanotechnologies: An Overview
the particles so small? Because below a critical dimension, typically at the nanoscale, ferromagnetic crystals become single domain (see section 7.4) which helps increase the effectiveness of the bacteria as a compass. Following a similar approach, magnetic nanoparticles are now being employed to detect particular biological species, such as microorganisms that cause disease. Magnetic nanoparticles are coupled with antibodies that bind to their target. In this case the magnetization vector of all nanoparticles becomes parallel, which results in a strong magnetic signal. On the other hand, if the illness is not present, the antibodies do not recognize the target and do not bind. Thus, all magnetization vectors will remain randomly oriented, leading to a weak magnetic signal. Another interesting application in nanomedicine is related to the use of gold particles for bio-identification. One set of gold particles carries DNA that binds to one half of the target sequence. A second set carries DNA that binds to the other half. The DNA with the complete target sequence will couple to both sets of particles, binding them together. As gold nanoparticles aggregate, there is a shift in the wavelength of light from red to blue. Thus, the red and blue lights can be used to probe whether a certain DNA corresponds to a particular individual.
US dollars (millions)
1400 1200 1000 800 600 400 200 0
2001 2002 2003 2004 2005 2006 2007 2008 2009 Year
22.1% Nanoscale devices and systems
5.52% Instrumentation, research, metrology, and standards 4.2% Nanomanufacturing 10.9% Major research facilities and instrument acquisition 5.17% Environment, health, and safety 2.76% Education and societal issues
33.9% Fundamental nanoscale phenomena (b)
FIGURE 1.10 U.S. federal funding trends in nanotechnology, 2001–2009. (National Nanotechnology Initiative: Second Assessment and Recommendations of National Advisory Panel, April 2008.)
These examples are only a small fraction of what will become possible in the future. Though still in their infancy, nanoscience and nanotechnology have already demonstrated that they will have a tremendous impact on various aspects of human life, such as health, environment, energy, transportation, information technology, and space exploration. This fact has been recognized by most of the industrial world, as confirmed by government funding allocated for the study of this area (see Figure 1.10). Nanoscience and nanotechnology hold great promise for future innovation and transformation. If the field’s expectations are fulfilled, it will create sought-after sensors with improved detection sensitivity and selectivity; strong, lightweight bullet-stopping armor; energetic nanoparticles for fast-release explosives; miniaturization of aircraft to reduce payload; materials that perform under extreme temperatures and pressures; radiation-tolerant materials; nanostructures that lower waste disposal costs; self-healing systems for extended space missions, self-assembly, and processing in space; implants to replace worn or damaged body parts; nanomotors; and cellular implants. In the wake of these innovations, nanoscience and nanotechnology will transform and revolutionize life as we now know it.
Scale, Structure, and Behavior 11
SCALE, STRUCTURE, AND BEHAVIOR
As discussed in the previous section, nano stands for nanometer, one billionth (10−9) of a meter. This defines a length scale that is, for these materials, important in some way, influencing their mechanical, thermal, electrical, magnetic, optical, and aesthetic properties. Before embarking on a discussion of these, it is useful to have an idea of where nano lies in the broader scale of things. If you ask: What is the smallest particle in matter? Most people would reply: an atom. Atoms have a diameter of about one tenth of a nanometer. Atoms are themselves made up of units that can sometimes be thought of as particles: electrons, neutrons, and protons. They are much smaller, about 10−15 meters (a femtometer) in diameter, but when things get this small quantum-mechanical effects make them fuzzy, their size ill defined, so we shall stop there. What is the other extreme? It used to be of global scale (“the ends of the Earth,” “poles apart”), but space exploration has changed all that, enlarging the concept of scale to intergalactic dimensions: light-years, just under 10,000,000 million km (1016 meters, 10 pentameters). Figure 1.11 shows this wide range, from a femtometer at the bottom to 100 light-years on the top. Its utility is much like that of the time scale used by geologists in classifying rocks (5 billion years ago to the present) or of archeologists in charting human history (500,000 BC to 2000 AD): It is a ladder on which things can be hung. Start at the human scale. It is the one from which perception expands, one that is built into our language. At the lower end, the diameter of a hair (“it missed by a hair’s breadth”). The inch, originally the ell, is the length of the lower joint of the thumb. The foot is, well, the foot. A yard is a pace. A furlong is the length of a furrow, a league (about 5 km) is the distance a man or a horse can walk in an hour; thus 7-league boots take you a day’s journey at one step. Perhaps that is why these are called Imperial units. You would not design anything using units like these (although NASA apparently still does). It was France, a nation that has contributed so much to rational thinking, that gave us a system with some sense in it. The National Assembly of the First Republic, by decree in 1790, created the standards of length, volume, and weight that we know today as the metric system. The original proposal was that the meter should be some fraction of the circumference of the Earth at the equator, but this was not seen as sufficiently Gallic. The decisive vote went for a fraction of the length of the meridian that passes through Paris and both poles. The meter, then, is one ten millionth (10−7) of the length of the
12 CHAPTER 1
Nanomaterials and Nanotechnologies: An Overview
Metres Astronomical scale Nearest galaxy (2 × 1022 m) 1 light year (9.5 × 1015 m) Earth–sun distance (1 AU.1.5 × 1011 m)
Earth–moon distance (3.8 × 108 m) Terrestrial scale Circumference of the Earth (4.2 × 107 m) Thickness of the Earth’s crust (3 × 104 m) 106 Height of Mt. Everest (8 × 103 m) Depth of deep oceans (5 × 103 m) 103 Human scale League (3 miles, 4.8 × 103 m) Furlong (22 yards, 2 × 102 m) Foot (3 × 10–1 m) Inch (ell) (2.54 × 10–2 m) Diameter of a hair (2 × 10–6 m)
mega kilo meter
Molecular and atomic scale
Molecular scale Atomic scale
Subatomic scale Electron Neutron Proton
FIGURE 1.11 Length scales ranging from the subatomic through molecular, human, and terrestrial to astronomic. The nano range is shown on the lower right.
Infrastructure engineering Road systems Rail systems Water distribution systems Sewage systems
Conventional engineering Shipping Trains, aircraft Cars, trucks Household products Precision instruments Conventional electronics Nanoengineering Microelectronic components Nanostructured solids Nanoparticles and emulsions Thin films, multilayers Carbon nanotubes Amorphous materials
quadrant (a quarter) of the circumference of the Earth along this particular trajectory. A liter is the volume of a cube with an edge of one tenth of a meter. A kilogram is the weight of one liter of water at 4°C. Once the reformers of the First Republic got started, there was no way of stopping them. Imperial units may have charm, but metric units are logical, comprehensible, and (as Figure 1.11 shows) extendable. The tools of science allow the study of materials over this immense range. Of the many ways in which they can be probed, the most revealing has been the interaction with radiation. Electromagnetic (e-m) radiation permeates the entire universe. Observe the sky with your eye and you see the visible spectrum, the range of wavelengths we call “light” (400–770 mm). Observe it with a detector of X-rays or γ-rays and you see radiation with far shorter wavelengths (as short as 10−4 nm, one thousandth the size of an atom). Observe it instead with a radio telescope and you pick up radiation with wavelengths
Objects interact strongly with radiation that has a wavelength comparable to their size or, if they have internal structure, with the scale of that structure. They interact in much less interesting ways with radiation that has wavelengths that differ much from their structural scale. The strong interaction gives diffraction and scattering. The analysis of these phenomena has proved to be a tool of extraordinary power, revealing the structure of the atom, the organization of atoms and crystals and glasses, and complex organic molecules such as DNA. At the other end of the spectrum, microwaves (radar) and waves of radio frequencies give us information about the thickness of the Arctic ice sheet and even insight into the structure of deep space. E-m waves are not the only way of probing materials. Acoustic waves, too, give information about structure that is comparable to the acoustic wavelength. Here the range is narrower (see Figure 1.13). At the lower end is extreme ultrasonic, used to probe surface structures and to detect and image cracks and defects in castings. Medical CT scanners use the range 1–20 MHz, giving a resolution of a few millimeters. Bats, dolphins, and whales communicate and locate prey using ultrasonics, 20–100 kHz. Sonar spans much of the audible range, extending down to frequencies as low as 1 Hz, typical of seismic waves. Nano, on the scale of Figure 1.11, lies near the bottom. The wavelengths of the visible spectrum (Figure 1.12) lie at the upper end of this range, so we anticipate the potential for strong interaction of light with nanomaterials; indeed, it is this interaction that gives opals their elusive and shifting colors, imparts hues to butterfly wings, and allows paints that change color as you walk past them. The ultraviolet spectrum overlaps the central part of the range, X-rays the lower part, so these, too, interact strongly with nanomaterials, are used to study their structure, and can be exploited in devices to manipulate them. Acoustic waves, with wavelengths that are large compared with the nanoscale, are less useful. This strong interaction when length scales are comparable extends to other properties. Electric currents are carried by electrons; heat is carried by both electrons and phonons. The resistance to both depends on the electron or phonon mean-free path, meaning the distance between scattering events. It is the structural length
10 Wavelength (m)
measured in millimeters, meters, or even kilometers, known as radio waves and microwaves. The range of wavelengths of radiation is vast, spanning 18 orders of magnitude (Figure 1.12). The visible part of this spectrum is only a tiny part of it—but even that has entrancing variety, giving us colors ranging from deep purple through blue, green, and yellow to deep red.
Increasing frequency, decreasing wavelength
Scale, Structure, and Behavior 13
FIGURE 1.12 The spectrum of electromagnetic radiation, from gamma to radio waves, a range of 1015. The visible portion is a tiny sliver of this range. The nanoscale overlaps the visible, the ultraviolet, and the long X-ray regimes.
14 CHAPTER 1
Nanomaterials and Nanotechnologies: An Overview
Frequency (Hz) 10
Sea-floor mapping sonar Bats, dolphins, whales Medical CT scanners
20 Hz Audible range
Ultra long-range sonar Long-range sonar Middle C
FIGURE 1.13 The acoustic spectrum from the extreme ultrasonic to the seismic, a range of 10 8. The audible part is a thick slice of this. The figure is based on acoustic waves in air, velocity 350 m/s. For water, shift the wavelength scale up relative to the frequency scale by a factor of 3; for rock, shift it up by a factor of 10.
of the material that determines this: the finer the structure, the shorter is the mean-free path and the higher the resistance. Magnetism involves domains of locally aligned magnetic moments; the domain boundaries have a characteristic thickness, again of atomic or nanodimensions. Optical properties, particularly, involve scattering or diffraction, both with specific length scales. Strength, too, is influenced by structural scale. When materials deform—bend, twist, or stretch permanently—it is because sheets of the atoms that make them up ratchet over each other. The ratchet steps are fixed by the atomic size. The lower end of the nanoscale approaches this in scale, giving, as the structural length approaches it, increasingly strong interaction, meaning greater strength. Brittleness (and its opposite, toughness) has a characteristic length—that of the flaw that will just propagate at the yield strength. The flaw size is itself related to the scale of the structure. This intrinsic dimensionality, so to speak, of material properties is one of the reasons for the great interest in nanomaterials. If we can engineer the structural scale of a material (as particles, thin layers, or the crystal size in bulk materials) in the right way, we can influence or interact with the property length scale and thus manipulate the property itself. We live in a world in which everyday objects have a size—we shall call it scale and give it the symbol L, for length—in the range of millimeters to meters. Scale has a profound effect on the behavior of structures made from materials. A steel tuning fork 80 mm long with arms that are 3 mm thick oscillates with a frequency of middle C, 256 Hz. Vibration frequencies scale as 1/L. So change the millimeters of the tuning fork to microns and the frequency rises to 256 kHz. Change it to nanometers and it becomes 256 MHz. This is comparable to the clock speed of computers, stimulating the novel idea of mechanical computers (not such a new idea: think of the abacus). This is an example of scale-dependent mechanical response. Response time— the time it takes a mechanical latch to close or a switch to switch— scale in the same way, as 1/L ; it is this that allows automobile airbag triggers to react fast enough to save lives. Thermal response scales even faster. The time for an object to reach thermal equilibrium when the temperature is changed scales as 1/L2 so the thermal response time that, for mm-scale objects, is seconds or minutes becomes microseconds at the micron scale and picoseconds at the nanoscale. (There is, in reality, a limit set by the acoustic velocity that cuts in, preventing the response becoming quite that short.) That’s the big picture. Focus now for a moment on the small one: the nano. What is so different and special about it? There is more
than one answer to that question of which the most obvious is that of surface area. Almost all properties of the thin layer of atoms that lie in the surface or interface of things behave in a different way than those in the interior. Surfaces, you could say, have their own properties. We experience this in their propensity to corrode, to stick (or not stick) to things, or to release electrons in plasma displays. But most of the useful properties—stiffness, strength, thermal and electrical conductivities, magnetism—come from the inside of atoms. At the familiar macroscale, the fraction of atoms that lie in the surface is minuscule. At the micron scale it is still tiny. But approach the nanoscale and it takes off (see Figure 1.14). The combination of small scale and a large fraction of “surface” atoms gives a property set that can be very different from that of the bulk. It is only now being unveiled. Nanomaterials have different mechanical, thermal, electrical, magnetic, optical, and, above all, chemical properties than those of the bulk. They can offer strong, wear-resistant coatings; they can change the ways in which heat and electricity are conducted; they have the ability, through their electrical and magnetic behavior, to store information and via their chemical behavior to catalyze chemical reactions, distribute drugs in the human body, and much more. Some of this “science fiction” is already real. Much more is a promise, but one in which considerable confidence can be placed. As with most major innovations, there are two principle obstacles to be overcome. The first: to develop a sufficiently deep understanding of behavior to establish both the good and the bad, the benefits and the hazards, of the nanoscale. The second is that of economics. Nanomaterials are expensive and will remain so, at least for some time. Finding ways to cushion the transition to economic viability needs thought.
FURTHER READING R. Freitas Jr., in Nanomedicine, Vol. I: Basic capabilities, Landes Bioscience, 1999. R. P. Feynman, There’s plenty of room at the bottom, Engineering and Science (California Institute of Technology), p. 22, Feb. 1960. N. Taniguchi, Proc. International Conf., Prod. Eng. Tokyo, Part II, Japan Society of Precision Engineering, 1974. K. Eric Drexler, Molecular engineering: An approach to the development of general capabilities for molecular manipulation, Proc. National Academy of Sciences, p. 5275, Sept. 1981. K. Eric Drexler, Engines of creation: The coming era of nanotechnology, Anchor Press/Doubleday, 1986.
Fraction of surface atoms (%)
Further Reading 15
100 10 1
0.1 10–2 10–3 10–4
10 102 103 104 105 Dimension in nanometers
FIGURE 1.14 The fraction of atoms that lie in the surface or internal interfaces of a nanoscale or nanostructured material, expressed as a percentage (%).
16 CHAPTER 1
Nanomaterials and Nanotechnologies: An Overview
Interagency Working Group on Nanoscience, Engineering and Technology, National Science and Technology Council Committee on Technology, Nanotechnology: shaping the world atom by atom, Sept. 1999. Greg Bear, Queen of angels, Warner Books, 1990. K. Eric Drexler, Nanosystems: Molecular machinery, manufacturing and computation, John Wiley & Sons, 1992. A. Tesigahara et al., Fabrication of a shell body microcar, Proc. Third International Symposium on Micro Machine and Human Science, Nagoya, Japan, Oct. 14–16, 1992. Jie Han, Al Globus, R. Jaffe, and G. Deardorff, Nanotechnology 8, p. 95, 1997. B. O. Dabbousi, et al., Journal of Physical Chemistry B, 101, p. 9463, 1997. G. Binnig and H. Rohrer, Helv. Phys. Acta, 55, p. 726, 1982. D. M. Eigler and E. K. Schweizer, Nature, 344, p. 524, 1990. P. Ball, Designing at the molecular world: Chemistry at the frontier, Princeton University Press, 1994. T. A. Fulton and G. J. Dolan, Phys. Rev. Lett., 59 (1), p. 109, 1987. M. A. Reed and J. M. Tour, Scientific American, 2000. M. Sarikaya, Proc. National Academy of Science, 96 (25), p. 14183, 1999. Janine Benyus, Biomimicry: Innovation inspired by nature, Perennial (HarperCollins) Publishers, 1998.
C H APTER 2
An Evolutionary Perspective
A BRIEF HISTORY OF MATERIALS
Our species, Homo sapiens, differs from others most significantly, perhaps, in its ability to design and make things. Making implies the use of materials. Materials have enabled the advance of mankind from its earliest beginnings; indeed, the ages of man are named after the dominant material of the day: the Stone Age, the Copper Age, the Bronze Age, the Iron Age (Figure 2.1). If you have seen the movie 2001: A Space Odyssey, you might remember one of the first scenes, in which prehistoric humans fight using animal bones. It is known that the tools and weapons of prehistory, 300,000 or more years ago, were bone and stone. Stones, particularly flint and quartz, could be shaped for tools; these materials could be flaked to produce a cutting edge that was harder, sharper, and more durable than any other material that could be found in nature. Gold, silver, and copper, the only metals that occur in native form, must have been known from the earliest times, but the realization that they were ductile, could be beaten into complex shapes, and, once beaten, could be hardened seems to have occurred around 5500 BC—almost 300,000 years after the time stone and bone were first used. By 4000 BC there is evidence that technology to melt and cast these metals had developed, allowing more intricate shapes. However, metals in native form, such as copper, are not abundant. Copper occurs in far greater quantities as the minerals azurite and malachite. By 3500 BC, kiln furnaces, developed for pottery, could reach the temperature required for the reduction of these minerals, making copper sufficiently plentiful to usher in the Copper Age. But even in the deformed state, copper is not all that hard. Poor hardness means poor wear resistance; therefore copper weapons and tools were easily blunted. Nanomaterials, Nanotechnologies and Design Copyright 2009 Elsevier Ltd. All rights of reproduction in any form reserved.
Date Biopol biopolymers (1990) PEEK, PES, PPS (1983) LLDPE (1980) Polysulfone, PPO (1965) Polyimides (1962) Acetal, POM, PC (1958) PP (1957) HDPE (1953) PS (1950) Lycra (1949) Formica (1945) PTFE (Teflon) (1943) PU, PET (1941) PMMA, PVC (1933) Neoprene (1931) Synthetic rubber (1922) Bakelite (1909) Alumina ceramic (1890) Celllose acetate (1872) Ebonite (1851) Reinforced concrete (1849) Vulcanized rubber (1844) Cellulose nitrate (1835)
The nano age
(1980 - present) Nano materials
Age of silicon
(1985) ‘Warm’ superconductors (1962) Carbon fibers, CFRP (1961) Shape memory alloys
Age of polymers
(1957) Amorphous metals (1947) Transistor-grade silicon (1947) Super alloys (1909 - 1961) Actinides* (1942) GFRP (1940) Plutonium* (1828 - 1943) Lanthanides* (1912) Stainless steel (1890) Aluminum production (1880) Glass fiber (1856) Bessimer steel (1823) Silicon *
Age of steel
(1808) Magnesium*, Aluminum* (1791) Strontium*, Titanium* (1789) Uranium* (1783) Tungsten*, Zirconium* (1765) Crucbile steel (1751) Nickel* (1746) Zinc* (1737) Cobalt* (1735) Platinum* (1500) Iron smelting
1000 AD Gutta percha (800)
Tortoiseshell (400) Paper (105) Horn (50 BC)
Iron age 500 AD
0 BC / AD
Amber (80 BC) (1400 BC) Iron
Lacquer (1000 BC) Papyrus (3000 BC)
Glass (5000 BC) Cement (5000 BC) Pottery (6000 BC)
Wood (prehistory) Stone, flint (prehistory)
(3500 BC) Bronze (3500 BC) Tin (4000 BC) Silver (5000 BC) Smelted copper (7000 BC) Native copper (20,000 BC?) Gold
Bronze age Copper age Stone age Mike Ashby, Cambridge, 2007
FIGURE 2.1 The materials timeline. The scale is nonlinear, with big steps at the bottom, small ones at the top. A star (*) indicates the date at which an element was first identified. Labels with no stars give the date at which the material became of practical importance.
A Brief History of Materials 19
Sometime around 3000 BC the probably accidental inclusion of a tin-based mineral, cassiterite, in the copper ores provided the next step in technology: the production of the alloy bronze, a mixture of tin and copper. Tin gives bronze an additional hardness that pure copper cannot match, allowing the production of superior tools and weapons. This discovery of alloying and solid solution strengthening—the hardening of one metal by adding another—was of such importance that it, too, became the name of a new era: the Bronze Age. “Old-fashioned” sounds like 20th century vocabulary, but the phenomenon is as old as technology itself. The discovery, around 1450 BC, of ways to reduce ferrous oxides to make iron, a material with greater stiffness, strength, and hardness than any other then available, rendered bronze old-fashioned. Iron was not entirely new; tiny quantities existed as the cores of meteors that had impacted the Earth. The oxides of iron, by contrast, are widely available, particularly hematite, Fe2O3. Hematite is easily reduced by carbon, although it takes high temperatures, close to 1100°C, to do it. This temperature is insufficient to melt iron, so the material produced was a spongy mass of solid iron intermixed with slag; this was reheated and hammered to expel the slag and then forged into the desired shape. Iron revolutionized warfare and agriculture; indeed, it was so desirable that at one time it was worth more than gold. The casting of iron, however, was a more difficult challenge, requiring temperatures around 1600°C. Two millennia passed before, in 1500 AD, the blast furnace was developed, enabling the widespread use of cast iron. Cast iron allowed structures of a new type; the great bridges, railway terminals, and civic buildings of the early 19th century are testimony to it. But it was steel, made possible in industrial quantities by the Bessemer process of 1856, which gave iron its dominant role in structural design that it still holds today. The demands of the expanding aircraft industry in the 1950s, with the development of the jet engine, shifted emphasis to light alloys (those of aluminum, magnesium, and titanium) and to materials that could withstand the extreme temperatures of the jet combustion chamber. The development of superalloys—heavily alloyed iron- and nickelbased materials—became the focus of research, delivering an extraordinary range of alloys able to carry loads at temperatures above 1200°C. The range of their applications expanded into other fields, particularly those of chemical and petroleum engineering.
20 CHAPTER 2
An Evolutionary Perspective
Though the evolution of metals is interesting, the history of polymers is rather different. Wood, of course, is a polymeric composite, one used for construction from the earliest times. The beauty of amber (petrified resin) and of horn and tortoise shell (the polymer keratin) attracted designers as early as 80 BC and remained attractive into the 19th century. (In London there is still a Horners’ Guild, the trade association of artisans who worked horn and shell.) Rubber, brought to Europe in 1550, was already used in Mexico for the Mayan ball game Pok-a-Tok. Rubber grew in importance in the 19th century, partly because of the wide spectrum of properties made possible by vulcanization—cross-linking with sulfur that produced materials as elastic as latex and as rigid as ebonite. The real polymer revolution, however, had its beginnings in the early 20th century with the development of Bakelite, a phenolic, in 1909 and synthetic butyl rubber in 1922. This was followed in mid-century by a period of rapid development of polymer science. Almost all the polymers we use so widely today were developed in a 20-year span from 1940 to 1960, among them the bulk commodity polymers polypropylene (PP), used for food containers; polyethylene (PE), used for children’s toys; polyvinyl chloride (PVC), used for pipes and fittings; and popyurethane (PU), used for foams and car dashboards, the combined annual tonnage of which now approaches that of steel. Designers seized on these attributes— cheap and easily molded to complex shapes—to produce a spectrum of brightly colored, cheerfully ephemeral products. Design with polymers has since matured; they are now as important as metals in household products, automobiles, and, most recently, in aerospace. The polymers of transport and aerospace are, however, more complex than “pure” polymers because they do not have the stiffness and strength these applications demand. They are polymermatrix composites, reinforced with fillers and fibers. Composite technology is not new. Straw-reinforced mud brick is one of the earliest of the materials of architecture and remains one of the traditional materials for building in parts of Africa and Asia even today. Steel-reinforced concrete—the material of shopping centers, road bridges, and apartment blocks—appeared just before 1850. Reinforcing concrete with steel to enhance the tensile strength where previously it had none was easy. Reinforcing metals, already strong, took much longer, and even today metal matrix composites are few. But polymers, with many attractive properties but lamentable stiffness, got scientists thinking. The technology for making glass fibers had existed since 1880, when it was used to make “glass wool” insulation. Glass wool, or better, woven or layered glass
A Brief History of Materials 21
fibers, could be incorporated into thermosetting polyesters or epoxies, giving them the stiffness and strength of aluminum alloys. By the mid-1940s glass fiber reinforced polymer (GFRP) components were in use in the aircraft industry. The real transformation of polymers into high-performance structural materials came with the development of aramid and carbon fibers in the 1960s. Incorporated as reinforcements, they give materials with performance (meaning stiffness and strength per unit weight) that exceeded that of all other bulk materials, earning their now-dominant position in the creation of sports equipment and in aerospace. The period in which we now live might have been named the Polymers and Composites Era had it not coincided with a second revolution: that of silicon technology. Silicon was first identified as an element in 1823 but found few uses until the 1947 discovery that, when doped with tiny levels of impurity, it could act as a transistor. The discovery created the fields of electronics, mechatronics, and modern computer science, revolutionizing information storage, access, and transmission; imaging; sensing and actuation; numerical modeling; and much more. So we live in what is rightly called the Information Age, enabled by the development of transistorgrade silicon. The 20th century saw other striking developments in materials technology. Superconduction, discovered in mercury and lead when cooled to 4.2°K (–269°C) in 1911, found no applications outside scientific research. But in the mid-1980s, two physicists at the IBM research center in Zurich discovered a complex oxide containing barium, lanthanum, and copper that was superconducting at 30°K. This triggered a search for superconductors with yet higher transition temperatures, leading, in 1987, to a material with a transition temperature above 98°K, the temperature of readily available liquid nitrogen, making applications practical. In the last two decades, the area of biomaterials has developed rapidly. Implanting materials in or on the human body was not practical until an aseptic surgical technique was discovered in the late 1800s. In addition, when nontoxic metal alloys were introduced, they tended to fracture in service. It was not until the development of polymer-based systems and, subsequently, with a new wave of discoveries in cell biology, chemistry, and materials science, that synthetic biomaterials became a reality. During the late 20th century it was realized that the behavior of materials depended on scale and that the dependence was most evident when the scale was that of nanometers. Although the term
22 CHAPTER 2
An Evolutionary Perspective
nanoscience is new, some of the technology is not. For example, nanoparticles of carbon have been used for the reinforcement of tires for over 100 years, nanoscale proteins have been part of vaccines since the early 20th century, and nature’s own nanotechnology, such as photosynthesis, has been around for millions of years. The ruby-red color of stained glass, known and used in the Middle Ages, is due to the presence of gold nanoparticles trapped in the glass matrix (see the next section). The decorative glaze known as luster, also found on medieval pottery, is the result of special optical properties provided by the gold nanoparticles. However, modern nanotechnology gained prominence with the discovery of various forms of carbon, such as the C60 molecule and carbon nanotubes. Simultaneously, with the advance of analytical tools capable of resolving and manipulating matter at the atomic level, scientists started asking: What if we could build things the way nature does, atom by atom and molecule by molecule? This approach involves molecular manipulation and molecular engineering in the context of building molecular machines and molecular devices with atomic precision. We are now entering a new era—that of the nano (see Figure 2.2). The rate of development of new metallic alloys and new polymers is slowing. Much research is now focused on making the ones we have already got more reliably, more cheaply, and particularly with less damage to the environment. However, the drive for ever better and more exciting properties remains. The nanoroute appears, to many to be the most promising way forward.
FIGURE 2.2 The coming of the Nano Age. Image of a nanoparticle composed of platinum and cobalt and obtained from an aberration-corrected scanningtransmission electron microscope. Note the scale bar and the small dimensions of the nanoparticle. Each dot on the nanoparticle corresponds to an atomic column imaged in projection. (Courtesy of P. J. Ferreira, University of Texas at Austin; L. F. Allard, Oak Ridge National Laboratory; Y. ShaoHorn, MIT.)
If we now step back and view the timeline of Figure 2.1 as a whole, clusters of activity are apparent; there is one in Roman times, one around the end of the 18th century, one around 1940. What was it that triggered the clusters? Scientific advances, certainly. The late 18th and early 19th centuries were a time of rapid development of inorganic chemistry, particularly electrochemistry, and it was this surge that allowed new elements to be isolated and identified. The mid20th century saw the birth of polymer chemistry, an understanding that enabled the development of the polymers we use today. But there might be more to it than that. Conflict stimulates science. The first of these two periods coincides with that of the Napoleonic Wars (1796–1815), a time in which technology, particularly in France, developed rapidly. And the second was that of the Second World War (1939–1945), in which technology played a greater part than in any previous conflict. One hopes that scientific progress and advances in materials are possible without conflict. The competitive
Nanomaterials and Nanostructures in Nature 23
drive of free markets appears to be an equally strong driver. It is interesting to reflect that more than half of all the materials scientists and engineers who have ever lived are alive today, and all of them are pursuing better materials and better ways to use them. Of one thing we can be certain: There are many more advances to come.
(Billions of years) First life 11
2.2 NANOMATERIALS AND NANOSTRUCTURES IN NATURE The timing of life arising on Earth was around 3.8 billion years ago (see Figure 2.3). Since then life has learned to reproduce, live under extreme toxic conditions, transform sunlight into oxygen, live underwater, fly, and eventually think, talk, and show emotions. As humans, we have constantly tried to supersede and control nature. However, so far we have spent little time trying to do things the way nature does. In other words, humans have not shown interest or been too proud to mimic or at least have not been motivated by nature’s millions of years of evolution. This is somewhat strange, because nature is undoubtedly the most experienced and tested laboratory ever available to us and capable of making sophisticated materials, capturing energy, self-healing, and storing information with incredible efficiency. Interestingly, most of what nature does takes place at the nanoscale. Perhaps the best-known biological example of such molecular machinery is the ribosome, which is a remarkable nanoscale assembler. The role of the ribosome is to act as a factory of proteins by combining amino acids together in a very specific order. A typical ribosome is located in an aqueous solution surrounded by thousands of solutes. The work is difficult. The ribosome must identify among 60 possible options a specific transfer RNA, a task that demands precision at the nanoscale (Figure 2.4). In this fashion, the ribosome machine can assemble proteins at a frequency of 20 Hz and an error rate of 10−3. Thus, ribosomes can manufacture, with an accuracy greater than 99.9%, linear strings of aminoacids of great length, which then produce three-dimensional protein structures. Another beautiful example of the role of nanostructures in the world’s daily routine is photosynthesis. Every green plant and photosynthetic bacteria can take carbon dioxide, water, and sunlight (the fuel) and transform them into oxygen and sugar, a process that is accomplished with an amazing efficiency of around 95%. In the case of green plants, everything happens inside the so-called chloroplasts. These units, which are responsible for the green color of
Oxygen rises in atmosphere
Ocean lost to space?
Age of plants and animals
FIGURE 2.3 Earth’s clock of life. (Adapted from Peter D. Ward and Donald Brownlee, The Life and Death of Planet Earth: How the New Science of Astrobiology Charts the Ultimate Fate of Our World, Times Book Publisher, 2003.) Amino acid tRNA mRNA strand Peptide bond
Growing protein nanoproduct
FIGURE 2.4 The ribosome assembler first selects from among 60 possible transfer RNAs (tRNA) one that allows a particular amino acid to bind into the key (Condon) of the messenger RNA (mRNA). The ribosome continues to assemble in this fashion until a particular protein is produced. (Adapted from P. Ball, Designing the Molecular World: Chemistry the Frontier, Princeton University Press, 1994.)
24 CHAPTER 2
An Evolutionary Perspective
Outer membrane Inner membrane
FIGURE 2.5 Structure of a chloroplast. The thylakoid disks contain nanoscale pigments that convert light energy into chemical energy. (Adapted from Interagency Working Group on Nanoscience, Engineering and Technology, National Science and Technology Council Committee on Technology, “Nanotechnology: Shaping the World Atom by Atom,” Sept.1999.)
FIGURE 2.6 An abalone shell consists of platelets of calcium carbonate forming a layered structure and separated by a protein sheet 20 nm thick. (Courtesy of Nan Yao, Princeton Materials Institute.)
plants, exist by the millions in the leaves. Inside each chloroplast are many disks, called thylakoids, which are stacked on top of each other (see Figure 2.5). These thylakoids are fluid-filled sacs containing in their skin light-sensitive pigments. Hence, when sunlight reaches these chloroplasts, the light-sensitive pigments collect the photons and direct them to the photosynthetic reaction centers, which are also embedded in the thylakoid’s skin. Each reaction center is composed of approximately 10,000 atoms and 200 pigments. Furthermore, at every reaction center, there are two highly light-sensitive pigments that execute the actual photon absorption. Within the pigments, electrons become excited when they absorb the energy of the sun. This initiates a chain reaction whereby water is dissociated, oxygen and hydrogen ions are released, and carbon dioxide is turned into sugar. Although difficult to believe, the process of photosynthesis produces approximately 300 billion tons of sugar per year, a massive industrial operation. So why is it so difficult to reproduce the photosynthesis process? Because the 10,000 atoms in the reaction center are configured in such a way that excited electrons can jump from molecule to molecule without decaying to the old orbital. As a result, photosynthesis moves electrons to the outside of the thylakoid membrane, leaving positively charged ions inside. In other words, a battery powered by the sun is formed, generated by the membrane potential, which is then used to drive chemical reactions. Mimicking this configuration is still an immense challenge. Another good example of natural nanostructures is the abalone, a marine mollusk, which is served in upscale restaurants. The mollusk builds the shell from traditional materials, namely calcium carbonate (CaCO3) and a protein, forming a layered nanocomposite that is strong and resilient. Looking at the shell under an electron microscope at high magnifications, the shell looks like a brick wall, with calcium carbonate “bricks” separated by the protein “mortar,” which acts as the “glue” (see Figure 2.6). The formation of the abalone shell starts with the secretion of proteins, which selfassemble into “room walls” with a distribution of negatively charged sites.. Inside each “room” there is seawater filled with calcium and carbonate ions, which are attracted to the walls and eventually form crystals of CaCO3. The end result is a shell that exhibits twice the toughness of our best high-tech ceramics. The reason behind these outstanding mechanical properties is the layered architecture composed of the protein material, with nanoscale thickness, and the ceramic calcium carbonate. Under
Nanomaterials and Nanostructures in Nature 25
applied stress, any crack in the shell can readily propagate through the ceramic material, but it will be deflected on contact with the protein material. Therefore, instead of a brittle material in which cracks can rapidly move without stopping, the shell of the abalone behaves as a ductile material. One other quite talented mollusk is the mussel (see Figure 2.7). When these animals want to feed or reproduce, they move to tidal waves. Due to the inherent turbulence of ocean waves, mussels need to use a waterproof adhesive to anchor themselves to a solid surface, to overcome the forces created by the waves. Clearly, this is not an easy task, since we know how difficult it is to have an adhesive or glue that sticks under water. So, how do mussels do it? A closer look at an anchored mussel reveals the presence of translucent filaments extending from the soft body toward the solid surface (see Figure 2.8). These filaments, called byssus, exhibit at their ends a foamy plaque, which is used to attach the mussel to the solid surface. The mussel starts the anchoring process by pressing the end of its foot on a solid surface to push the water away. Because it cannot repel all the water, the mussel attaches itself to a single point, then builds a loose structure, enclosing the water. In fact, it secretes a protein and forms a long vertical groove, which is under vacuum and acts as a mold for the following step. Next, the mussel sends out a series of proteins that self-assemble and harden, forming the plaque and the thread. Still in the vacuum space, the mussel then secretes liquid proteins that harden into a very strong adhesive, gluing the plaque to the solid surface. From a structure point of view, the filaments are quite interesting. The thread exhibits a concentration gradient of various proteins along its length, showing a rubbery-type behavior near the mussel and stiffer properties close by the plaque. The plaque itself is a solid foam that can easily expand and contract during tidal cycles without breaking. As with mussels, geckos (a type of lizard) have an extraordinary ability to adhere to a surface. They can stick to walls or ceilings, even on a single toe (see Figure 2.9). This behavior is due to keratin hairs, 200 nm in diameter, that cover their feet. Each hair produces a very small force of 10−7 N (due to Van Der Waals interactions). However, half a million of these tiny hairs produce an extremely strong adhesive force, as high as 10 N/cm2. The hairs can readily bend to conform to the topography of a surface, which allows geckos to stick to even flat surfaces such as glass. The connection breaks when the gecko shifts its foot enough to change the angle between the hairs and the surface. This discovery has launched
FIGURE 2.7 Mussel anchored to a surface by filaments called byssus. (Courtesy of Mieke C. van der Leeden, TU Delft.) Mussel
FIGURE 2.8 Schematic view of the byssus structure. The thread is rubbery-like near the mussel and stiffer close by the plaque. The plaque is a solid foam. (Adapted from Mieke C. van der Leeden, TU Delft.)
26 CHAPTER 2
An Evolutionary Perspective
several research groups into developing tapes based on the gecko adhesive force. In one example, the tape is made by microfabrication of dense arrays of flexible plastic pillars, the geometry of which is optimized to ensure their collective adhesion (see Section 10.4). Now imagine a material capable of catching an airplane traveling at cruise speed. Although at a very different scale, a spider web (see Figure 2.10) has such energy-absorbing properties, enabling the capture of flying insects at high speeds. It turns out that the secret behind the combined strength and flexibility of a spider web lies in the arrangement of nanocrystalline reinforcements embedded in a polymer matrix. A closer look at the spider web microstructure reveals the existence of strongly oriented nanocrystals, which adhere to the stretchy protein that composes their surrounding polymeric matrix. In other words, the spider web is a nanocomposite material composed of relatively stiff nanocrystals dispersed within a stretchy matrix that is now stronger and tougher. The spider web starts as raw silk (a liquid protein) secreted by a gland. The protein is then pushed through channels at the spider’s back end. What emerges is a water-insoluble, highly ordered fiber with outstanding mechanical properties. Although this process is not fully understood, it is believed that the raw silk transforms into a liquid crystal phase just before entering the channels, whereas the passage through the channels aligns the molecules, which are anisotropic in nature.
FIGURE 2.9 The base of geckos’ feet is covered by half a million keratin hairs, 200 nm in diameter. (Daniel Heuclin, above and middle; Andrew Syred/Photo Researchers Inc, top.)
Following the properties exhibited by spider webs, several research groups have been trying to develop materials capable of emulating this nature’s marvel. Recently, a group at MIT has focused on developing a commercial polyurethane elastomer (a rubbery substance) reinforced with nano-sized clay platelets. These molecular nanocomposites are likely to be good candidates for lightweight membranes and gas barriers due to the fact that the nano-sized clay platelets enhance the mechanical and thermal properties. In addition, materials based on the characteristics of spider webs are suitable for body-armor components, thin and strong packaging films, and biomedical devices. If you’ve ever observed two rhinos fighting with each other, you were probably impressed by the properties exhibited by their horns. Despite the enormous forces involved when the animals clash, the horns remain intact without fracturing. The reason for this is the presence of keratin, a fibrous protein that is also present in hair and fingernails and that is self-assembled into a very specific structure.
Nanomaterials and Nanostructures in Nature 27
The horn is a composite made of two types of keratin. One type is in the form of tubules that are densely packed (see Figures 2.11 and 2.12). These tubules, which range from 300 to 500 µm, comprise around 40 layers of cells. Surrounding these tubules is another type of keratin that is continuous and acts as a matrix. Because the matrix and the tubules are the same material, the interfacial strength is very good, which leads to a rigid material that is very tough to break. Following this concept, there is now great interest in emulating these horn structures at the nanoscale by designing materials with nanotubules embedded in a matrix. In other words, this approach is not very different from dispersing nanowires or nanotubes in a polymer matrix. Another remarkable property of natural materials is their ability to self-repair and adapt to the environment. This is crucial for efficiency and, ultimately, survival of the fittest. By contrast synthetic materials rarely exhibit this property. Therefore, producing materials capable of repairing cracks, restoring functions, or selfproducing is still a challenge that nanotechnology can help meet. Two interesting examples of natural materials that exhibit selfhealing properties are bone and skin. Bone is essentially a composite material formed by an organic matrix (collagen) and reinforced by mineral particles (apatite). The collagen is in the form of fibrils of about 100 nm in diameter and 5–10 µm long that consist of an assembly of 300 nm long and around 1.5 nm thick. The apatite are platelike crystals with a thickness around 1.5– 4.5 nm that fill the collagen fibrils. The collagen fibrils are separated by extrafibrillar material, which consists of extrafibrillar collagen and apatite that coats the fibrils (see Figure 2.13). The remarkable result of this hierarchical configuration is that the bone can hold weight and toughness to absorb energy and not break into small fragments (see Figure 2.14). When subjected to a load, the whole bone deforms to different degrees. In fact, the tissue, fibrils, and mineral particles absorb successively lower levels of strain, in a ratio of 12 : 5 : 2. Although the mechanisms of deformation are not fully understood, it seems that the interface between the extrafibrillar matrix and the collagen fibrils breaks and reforms under load, providing a way for damage repair at the molecular scale. On the other hand, the hard nanoparticles of apatite are shielded from excessive loads, although they can achieve strains of 0.15–0.2%, which is twice the fracture strain of bulk apatite. Bone is also capable of constant remodeling, eliminating damaged bone and replacing it with new material. Strain sensor
FIGURE 2.10 Spider web.
Horn tubules 2 mm
FIGURE 2.11 Microstructure of a white rhinoceros horn. The horn tubules, surrounded by the intertubular matrix, act as a composite material. (Courtesy of Tobin Hieronymus et al., Ohio University.)
28 CHAPTER 2
Cortex Horn tubule
An Evolutionary Perspective
Single horn lamina
Mellanized intertubular matrix
Inter tubular matrix
FIGURE 2.12 Schematic three-dimensional view of a white rhinoceros horn, where the various components of the composite material forming one horn lamina are indicated. Each horn tubule is composed of the cortex and medullary cavity, which is surrounded by melanized and non-melanized intertubular matrix. (Courtesy of Tobin Hieronymus et al. Ohio University.)
~1 – 2 nm ~2 – 4 nm
extrafibrillar mineral particles
~0.1 – 10 mm
FIGURE 2.13 Hierarchical structure of bone. The yellow regions are the collagen fibrils and the red plates are the apatite crystals. The multidimensional configuration of the various bone components is crucial for efficient load transfer. Typically, the strain decreases from the tissue level to the mineral particle level by a factor of 6. (Courtesy of Himadri Gupta et al. Max Planck Institute of Colloids and Interfaces.)
cells (osteocytes) associated with the bone tissue first detect material that has been subjected to large deformations and damaged. Subsequently, these sensors send information to a group of cells that will remodel the old bone and form a new one. However, by far the most striking property of bone is its capacity to self-heal a fracture. Typically, a broken bone starts by experiencing a cut in the blood supply, and cells die. This process cleans up the area of dead material before reinitiating the blood supply and sending stem cells. These cells are a precursor to cells that eventually will produce cartilage, fibrous tissue, and new bone (Figure 2.14). The skin is also an outstanding self-healing system. How many times through life have you had your wounds completely regenerated? The wound-healing process starts with the formation of a blood clot on the wound to avoid unwanted chemicals from penetrating healthy tissue. Subsequently, a network of capillaries forms, with diameters around 8–10 µm, to supply nutrients through the blood and accomplish cell division and cellular growth. Inspired by these ideas, researchers at the University of Illinois have recently developed self-healing materials that consist of a microencapsulated healing agent and a catalyst distributed throughout a composite matrix. If the material cracks, microcapsules will break and release a healing agent. The healing agent will react with the catalyst to repair the damage. This is similar to the case in which a cut in the skin triggers blood flow to promote healing. To create these materials, the researchers begin by building a scaffold, which consists of polymeric ink in the form of continuous filaments in three dimensions. Once the scaffold has been produced, the ink filaments are embedded with a resin. After curing, the resin is heated, turning the ink into a liquid. The ink is then removed, leaving behind a substrate with a network of microchannels. Finally, an epoxy coating is deposited on the substrate while the network of microchannels is filled with a liquid healing agent. Under these conditions, when a crack forms, it propagates until it finds one of the fluid-filled microchannels. At this point, the healing agent moves from the capillary into the crack, where it interacts with the catalyst particles and repairs the damage. Last but not least, we ought to discuss the human brain. It is definitely the most incredible piece of machinery we have encountered so far. It allows us to think and even dream. We have tried to emulate or surpass the human brain with the development of computers. However, we now know that computers are nothing like our brains. Brains are essentially carbon; computers are mainly
Nanomaterials in Art and Cultural Heritage 29
silicon. The brain’s neurons have thousands of connections (see Figure 2.15); a computer’s transistors have a few. The brain expends 10−15 Joules per operation, whereas a computer expends 10−7 Joules per operation. But the major difference is that brains compute with molecules that “work” together and produce a result, instead of the “on” and “off” switches used by computers. And the reason for this distinct behavior is that carbon can establish a large variety of bonds with other atoms and thus can form many molecules of different shapes. On the other hand, silicon tends to be less flexible in bonding and thus cannot assume many shapes, as carbon does. The shape of molecules is crucial in identifying other species and deciding what to do, whether joining, separating, or passing messages across. In other words, each neuron is a computer controlled by nanoscale components.
FIGURE 2.14 Different phases in bone fracture healing. Upon fracture, the broken bone is initially restored by a blood clot. After removal of dead bone fragments, the healing process sets in with the formation of primitive bone tissue ordered by precursor cells. Finally, the cells that produce cartilage and fibrous tissue take over and produce new bone.
2.3 NANOMATERIALS IN ART AND CULTURAL HERITAGE Examples Found in Art In the opening of this chapter, we noted that the ruby-red color of many stained-glass windows from the Medieval era was a consequence of embedded nanoscale metallic particles within the glass (see Figure 2.16). These rich colors in stained glass, like the metallic sheens associated with naturally embedded nanoparticles in many ceramics, were appreciated and highly valued by artisans, patrons, and laymen alike. Stained-glass artisans sometimes treasured small vials of materials that we know were metallic oxides, obtained from special mines and handed down within their families with careful instructions on how to work with them. As we will see later in this chapter and in Section 7.5, when the size of material particles is reduced to the nanoscale, optical properties—particularly color— can be dramatically affected. In such cases, the wavelength of light is very close to the size of the particles themselves, which causes the way that color is reflected, scattered, or absorbed to be dependent on the size and shape of the nanoparticles themselves. There was no scientific understanding of these phenomena at the time, nor were there deliberate attempts to produce what we now know as nanomaterials. Early knowledge relied on craft-based trial and error to achieve effects. It was known, for example, that the introduction of certain materials from specific mines and according to empirically understood methods did indeed produce rich colors
FIGURE 2.15 Network of neurons. It is estimated that a human brain contains around 100 billion neurons, each one with thousands of connections.
30 CHAPTER 2
An Evolutionary Perspective
in glass. Metallic compounds (which we now know were cobalt oxide) from mines in Bohemia were added during the fusion process to achieve the deep blues so widely admired in the glass at Chartres Cathedral. Likewise, the intense ruby-colored stained glass is now known to have been obtained from the dispersion of solid silica particles or of nanosized gold particles within the glass. We must keep in mind, however, that not all interesting color phenomena are a result of embedded nanomaterials.
FIGURE 2.16 Window from Chartres Cathedral. The intense colors of many Medieval stained-glass windows resulted from nanosized metal oxide particles added to the glass during the fusion process.
One of the most interesting specimens is the Roman-era Lycurgus cup. Roman glassware has often been used to characterize the material cultural achievements of the late Roman Empire. Glassproducing techniques were highly developed, and workmanship was superb. In the Lycurgus cup, now housed in the British Museum, the 324 AD victory of Constantine over Licinius in Thrace was represented through the death of an enemy of Dionysius, Lycurgus, who is shown being overcome by vines. The most remarkable characteristic of this goblet is that under normal external lighting conditions the glass appears green, but when lighted from within, it assumes a strong red color (see Figure 2.17). The Lycurgus cup has now assumed an almost iconic status in the nanomaterial field as an early example of the surface plasmon phenomenon, in which waves of electrons move along the surface of metal particles when light is incident onto them (see Section 7.5 for a detailed description of the surface plasmon phenomenon). Analyses have demonstrated that the glass in the Lycurgus cup contains rather small amounts of gold powder embedded within it (on the order of 40 parts per million). These tiny metallic particles suspended within the glass matrix have diameters comparable to the wavelengths of visible light. As a consequence, a form of plasmonic excitation (an oscillation of the free electrons at the surface of a metal particle at a certain frequency) can occur. Light reflections are enhanced as the waves are highly absorbed and scattered, reducing transmission. This absorption has an orientational dependence. Interestingly, other colors aside from the red and green seen in the Lycurgus cup could be achieved by altering metal particle sizes. In the cup, however, color properties depend primarily on reflection when the light is external to the cup and on absorption and transmission when the light source is internal. Many Medieval and Renaissance ceramics have surfaces characterized by a remarkable iridescent metallic shine (see Figure 2.18). This form of ceramic decoration, a type of luster, appeared in the
Nanomaterials in Art and Cultural Heritage 31
Middle East in the ninth century or before and subsequently spread through Egypt, Spain, and other countries. A particularly fine period of development occurred in Spain with Hispano-Moresque ware, a glazed ceramic made by Moorish potters largely at Málaga in the 15th century and later at Manises near Valencia in the 16th century. To produce this type of lusterware, a glaze was first applied over a design and the piece fired to produce a thin, hard coating. Glazes were based on dry powdered minerals or oxides, which commonly included tin and copper. After the first firing, the luster coating, consisting of metallic pigments (normally copper or silver compounds) mixed with clays, was brushed on over the glaze. Then the piece was fired again but at a lower temperature and within a reducing atmosphere (a condition whereby a reducing agent chemically causes a change in a material with metallic compounds to a metallic state by removing nonmetallic constituents as it is itself oxidized by donating free electrons). Afterward the piece was cleaned and polished to reveal the resulting metallic sheen. Later examples include the “tin-glazed” pottery of 15th and 16th century Italy and the “copper glazed” lusterware porcelains of Wedgwood in early 19th century England. Several studies of medieval lusterware via transmission electron microscopy (TEM) have been undertaken to understand the composition and microstructure of luster. Results have clearly indicated that various luster characteristics can be described in terms of the presence of different levels of silver or copper nanoparticles within the glassy matrix. The associated surface plasmon effects (described previously) cause the appealing metallic sheen to develop. Again, though the artisans producing lusterware lacked an understanding of the chemical processes that achieved the optical effects and were unaware that their empirical processes led to the creation of nanoparticles, the craft-based development of the requisite knowledge was remarkable. Similarly intriguing was the development of the beautiful blue paint found in the murals and pottery of the ancient Mayan world (see Figures 2.19 and 2.20). The Mayan blue has long been admired for its marvelous color qualities as well as its inherent resistance to deterioration and wear over long periods of time. Various natural alkalis, oxidants, mineral acids, and other agents seem to have little effect on the blue paint of the Maya. Unlike the blues of Europe and Asia, largely based on ground lapis lazuli, the origin of the Mayan blue was likely a dye known as anil, which is found in preColumbian textiles and is obtained from a local plant to produce indigo. Normal indigo, however, is not acid resistant and its use
FIGURE 2.17 The Lycurgus cup looks green when light shines on it but red when a light shines inside it. The cup contains gold nanoparticles. (Courtesy of the British Museum.)
32 CHAPTER 2
An Evolutionary Perspective
would not in itself account for the many interesting properties of Mayan blue. A predominant presence of palygorskite clays in the paint that were found to have a plate- or needle-shaped internal structure have been identified.
FIGURE 2.18 Medieval lusterware, circa 16th century, Manises, Spain. The glaze was made by firing metal oxides.
Within these clays very small amounts of impurities (iron -Fe, manganese -Mn, chromium -Cr) were also found. The host clays appear to have originated in a mine near Merida (and were subsequently heated to high temperatures), whereas the embedded impurities came from the anil plant used to make the indigo. Most of these impurities were in metallic states. Some oxidized elements were near the surface. Detailed studies have been made of these materials (see Figures 2.21 and 2.22). Interestingly, even minor amounts of nanosized particles in the impurities can be expected to have significant effects on optical properties due to the surface plasmon excitation effects. The particular blue color thus results from the exact type of absorption curve present, which is in turn influenced by the exact size, shape, and dispersion of the nanoparticles. These effects, along with those from the oxide metals, appear to help account for the strong blue color. Meanwhile, it is the intercalation (insertion of foreign atoms into the crystalline lattice of another material) of indigo molecules within the clay that may account for the corrosion resistance exhibited by the paint. Thus, the interesting properties of the final product result from a complex sequence of circumstances involving naturally occurring nanomaterials. Like the glass and ceramics examples described earlier, the process developed by Mayan artisans did not involve an understanding of chemistry or nanomaterials as we know them today but rather a persistent search in visual effects in the service of fine art.
FIGURE 2.19 Detail of Feathered Serpent from a wall painting at Cacaxtla, Mexico. (Courtesy of Barbara Fash, Peabody Museum, Harvard University.)
Conservation and restoration of works of art and other forms of cultural heritage have been a constantly evolving pursuit in which nano-based techniques play increasingly valuable roles (see Figures 2.23 and 2.24). A great number of factors can play a role in the degradation of artworks. For instance, microbial growth can have a range of detrimental effects on various media. Significant damages can be inflicted on both paintings and sculptures by the many pollutants in the atmosphere. The problem of nitric oxides in polluted atmospheres slowly degrading the surfaces of marble statues and marble buildings from ancient times is well known. In wood artifacts, acids can cause degradation of the cellulose structure present.
Nanomaterials in Art and Cultural Heritage 33
FIGURE 2.20 Mayan wall painting from Cacaxtla, Mexico. The intense blue results from an amorphous silicate substrate with embedded metal nanoparticles and oxide nanoparticles on the surface. (Courtesy of Barbara Fash, Peabody Museum, Harvard University.)
Paintings that are exposed to air and elements can become covered with foreign particles that change visual appearances and begin to act mechanically on the artifact. The paint itself as well as the substrate that has been painted on can begin to crack. There can be a loss of cohesion between paint layers on various media. Particles can flake off. Among the greatest of our cultural treasures are Medieval wall paintings done in the fresco technique. They adorn many Medieval buildings, particularly in Italy. In the buon fresco method, pigments mixed with water were applied to freshly placed and still-wet lime mortar after initial carbonation, thus embedding the pigments well into mortar (or, more precisely, into the crystalline structure of the newly formed calcium carbonate). Paintings not only had marvelous color and visual qualities, they were quite stable as well. With time, however, salts can begin migrating through pore structures in the mortar due to dampness and other reasons, and salt crystallization can occur. The consequence is that severe degradation can occur in the form of flaking of paint layers or powdering of colors. Deeper damage can occur to the overall porous structures as well. Damaging salts or particulates can also come from wind-blown sources.
FIGURE 2.21 (Left) Metallic and oxide particles on SiO2 support and (right) an atomic resolution image of a particle showing its cubo-octahedral shape. (Courtesy of J. Yacaman, et al.)
FIGURE 2.22 Image of a palygorskite crystal showing a superlattice period of about 1.4 nm. (Courtesy of J. Yacaman, et al.)
34 CHAPTER 2
An Evolutionary Perspective
Conservation work was carried out in the 1970s using the Ferroni-Dini method for cleaning from sulfatation and consolidation of frescoes. Preand post-restoration images under raking light.
According to undocumented tradition, the face of the saint is a self-portrait of the artist, Beato Angelico. Pre- and post-restoration under glazing light.
FIGURE 2.23 Fra Angelico, Saint Dominic in Adoration Before the Crucifix, Convento di San Marco, Florence, Italy, c. 1438. (Conservation images courtesy of Piero Baglioni, Center for Colloid and Interface Science, CGSI, University of Florence.)
Post-restoration image; nanostructured systems were used for conservation.
FIGURE 2.24 Santi di Tito, The Musician Angels,15th century. (Courtesy of Piero Baglioni, Center for Colloid and Interface Science, CGSI, University of Florence.)
Nanomaterials in Art and Cultural Heritage 35
These and other sources and types of damage have long plagued curators and owners of these delicate frescoes. Many early attempts to conserve artworks ultimately did more damage than good. At one time, for example, varnishes were used over paintings in a misguided attempt to protect them. These now-darkened varnishes are a major problem in restoration efforts today. In more recent years, less problematic acrylic polymers such as ethyl methacrylate (paraloid) as well as others have been used to consolidate wall paintings. Even the best of current techniques, however, can still result in some type of change, not be very effective, or simply be short lived. Methods of conservation have come a long way since the use of varnishes, but the many inherent challenges have not been entirely overcome and the process remains painstaking. Current restoration and conservation standards demand that any conservation or restoration technique be reversible and should in no way alter the fundamental chemical or physical composition of the original artifact or otherwise affect its properties. New techniques were developed as a consequence of the terrible floods in Florence and Venice in 1966 that caused widespread damage to the art and architecture of these cities. One important method developed shortly thereafter, the barium or Ferroni-Dini technique, used chemical methods for consolidation and restoration of wall paintings suffering from salt crystallization. The method seeks to reconstitute the calcium carbonate layer. Surface applications of aluminum and barium hydroxides are applied so that harmful calcium sulfates are ultimately converted into inert barium sulfates. These, in turn, ultimately act to consolidate the substrate and to create a fresh binder. This technique has been widely used throughout the world and has led to the development of other sophisticated techniques as well. Researchers at the Center for Colloid and Interface Science (CSGI) at the University of Florence have extended the Ferroni-Dini method using nanomaterial technologies. Calcium hydroxide would be especially desirable for conservation use with carbonate-based materials because of compatibility. A saturated calcium hydroxide water solution, known as lime water, has been used, but its low solubility has presented problems. The use of calcium hydroxide suspensions has been explored, but these are not stable enough and create surface effects. Researchers at the Center explored the use of dispersions of nanosized calcium hydroxide in nonaqueous solvents. Nanoparticles of this type can be obtained from a simple homogeneous phase reaction in hot water. Going to smaller sizes
36 CHAPTER 2
An Evolutionary Perspective
changed the physical and chemical features of the calcium hydroxide particles. Nanoparticle sizes ranged from 10 nm to 200 nm and were found to be able to penetrate within pore structures of wall paintings and limestone and without leaving surface effects. The particles increased cohesion to the painted layers. After a short period of time, the calcium hydroxide particles were found to react with carbon dioxide in the air and create a greatly improved binder in the host material, thus consolidating it. The process essentially replaces calcium hydroxide lost during degradation. The same methods have been applied to many fresco paintings, including at the Maya archeological site of Calakmul. Interestingly, this consolidation method can be applied to other materials, including ancient brick mortar.
FIGURE 2.25 Acid paper. (Courtesy of Piero Baglioni.)
FIGURE 2.26 Nanoparticles of calcium hydroxide on paper— deacidification. (Courtesy of Piero Baglioni.)
FIGURE 2.27 Calcium hydroxide nanoparticle.
Using approaches similar to that just described, nanoparticles can also be used for conserving or restoring old textiles, paper, and wooden objects (see Figure 2.25). It is well known that paper made from wood pulp in the last few centuries is extremely prone to deterioration. With rising demand for paper, older medieval techniques of producing paper from rags (which yield quite good and long-lasting paper) were replaced with approaches that extracted cellulose from wood. Acid sizings, such as alum, were often used on the papers as well. The unfortunate combination results in acidcatalyzed degradation of the cellulose in papers that is hastened by the high reactivity of cellulose obtained from wood pulp. As a consequence, the failure of papers has become all too familiar in our archives and libraries—and even to the amateur old book collector. Deacidification processes can be used to stabilize documents and increase the life of these papers, but these methods are expensive and slow. Nanoparticle-based paper treatments have been suggested for use to achieve more efficient and long-lasting deacidification. Smaller particles allow easier penetration and more complete dispersion (see Figures 2.26 and 2.27). The approach generally suggests an improved way of dealing with one of our most delicate preservation problems. The work on cellulose structures described previously has led to other applications. In the 17th century the royal battle galleon Vasa was built on the order of King Gustavus Adolphus of Sweden (see Figure 2.28). The ship was built of large oak, and its two gun decks held 64 bronze cannons. On its maiden voyage on August 10, 1628, the Vasa fired a farewell. A sudden squall caused it to list, and water poured through still open gun ports. The vessel capsized and sank with great loss of life. Amazingly, the ship’s largely intact hull was salvaged in 1961. To prevent the hull from drying out,
Nanomaterials in Art and Cultural Heritage 37
shrinking, and decaying, preservationists immediately treated it with polyetheylene glycol (PEG) by intermittent spraying and slow drying. It was moved to the Vasa Museum in Stockholm, where alarming rates of acidity increases in the wood were observed and again threatened the hull by acid wood hydrolysis. Sulfuric acids were proving especially harmful. The development of sulfurs was traced back to metabolic actions of bacteria in the harbor water and was subsequently oxidized by the iron released from longcorroded bolts as well as from more recent ones put in during salvaging. Preservation efforts focused on removing iron and sulfur compounds. Neutralization treatments using alkali solutions helped in only outer wood layers and can potentially cause cellulose degradation itself. A new method of neutralizing the acids by the use of nanoparticles has recently been explored by the group from the University of Florence, mentioned previously. The immediate preservation focus was to slow the production of acids inside the wood and, if possible, remove the iron (or render it inactive) and sulfur. Prior treatments and conditions further complicated the problem. The Florence group focused on deacidification. Wood samples were obtained from the Vasa and then treated with an alkaline solution was used to remove the PEG, which would prevent nanoparticles from penetrating the wood and provide neutralization. Nanoparticles of calcium hydroxide were synthesized and samples soaked in an alkaline nanoparticle dispersion (see Figure 2.29). Progress of the penetration of the nanoparticles through the wood was tracked with the aid of scanning electron microscopes (SEM analysis—see Chapter 7). The nanoparticles were found to adhere to wall fibers and the dispersion medium volatized, leaving an alkaline presence. The application led to a marked decrease in the pH levels present (reduced acidity). Other benefits were noted as well. Work with nanotechnology has only recently been emerging in the conservation area, but initial results look very promising. Later chapters will look at other nano-based techniques that may prove beneficial in conserving our cultural heritage. For instance, the airborne pollutants from traffic or smog, which are known to attack the surface of sculptures and architectural monuments made of marble and other stones that form part of the cultural experience of our finest urban environments, might be combated with the self-cleaning actions of certain kinds of nanomaterials described in Chapter 10. Indeed, the potential value of inert self-cleaning surface treatments would be literally enormous, but considerable gaps
FIGURE 2.28 The Vasa sank in 1628 and was salvaged in 1961. Originally treated with PEG, the hull was still threatened by acidification.
FIGURE 2.29 Experiments have been conducted with embedding nanoparticles of calcium hydroxide to stabilize wood. Ca(OH)2 nanoparticles on the wall fibers of wood are shown in this scanning electron microscopy (SEM) image. (Courtesy of Piero Baglioni, Center for Colloid and Interface Science, CGSI, University of Florence.)
38 CHAPTER 2
An Evolutionary Perspective
must still be bridged before we can safely benefit from these new nanotechnologies.
FURTHER READING The History and Evolution of Materials C. Singer, E. J. Holmyard, A. R. Hall, T. I. Williams, and G. Hollister-Short (eds.), A history of technology (21 volumes), Oxford University Press, 1954–2001, ISSN 0307-5451. (A compilation of essays on aspects of technology, including materials.) J. Delmonte, Origins of materials and processes, Technomic Publishing Co., 1985, ISBN 87762-420-8. (A compendium of information about materials in engineering, documenting the history.) R. F. Tylecoate, A history of metallurgy, 2nd ed., The Institute of Materials, 1992, ISBN 0-904357-066. (A total-immersion course in the history of the extraction and use of metals from 6000 BC to 1976 AD, told by an author with forensic talent and love of detail.) www.tangram.co.uk.TL-Polymer_Plastics_Timeline.html/. (A Website devoted to the long and full history of plastics.)
Nanomaterials and Nanostructures in Nature Peter D. Ward and Donald Brownlee, The life and death of planet earth: How the new science of astrobiology charts the ultimate fate of our world, Times Book Publisher, 2003. R. Freitas Jr., in Nanomedicine, Volume I: Basic Capabilities, Landes Bioscience, 1999. P. Ball, Designing the molecular world: Chemistry at the frontier, Princeton University Press, 1994. Janine Benyus, Biomimicry: Innovation inspired by nature, Perennial (HarperCollins) Publishers, 1998. Himadri S. Gupta, Jong Seto, Wolfgang Wagermaier, Paul Zaslansky, Peter Boesecke, and Peter Fratzi, Cooperative deformation of mineral and collagen in bone at the nanoscale, PNAS, 103, pp. 17741–17746, 2006. Tobin L. Hieronymus, Lawrence M. Witmer, and Ryan C. Ridgely, Structure of white rhinoceros (Ceratotherium simum) horn investigated by X-ray computed tomography and histology with implications for growth and external form, Journal of Morphology, 267:1172–1176 2006. Yao et al., Organic inorganic interfaces and spiral growth in nacre, Journal of the Royal Society Interface, 2008 (in press).
Nanomaterials in Art and Cultural Heritage P. Baglioni and Rodorico Giorgi, Soft and hard nanomaterials for restoration and conservation of cultural heritage, first published as an advance article on the Web, Feb. 10, 2006. DOI: 10.1039/b516442g, RSG, Soft Matter, 2, 293–303, The Royal Society of Chemistry, 2006.
Further Reading 39
Piero Baglioni, Rodorico Giorgio, and Ching-chih Chen, Nanoscience for the conservation of cultural heritage and the emergence of a powerful digital image collection, Proceedings of the 8th Russian Conference on Digital Libraries, RCDL’2006, Suzdal, Russia, 2006. Rodorico Giorgi, David Chelazzi, and Piero Baglioni, Nanoparticles of calcium hydroxide for wood conservation: The deacidification of the Vasa warship, 10.1021/la0506731 CCC, American Chemical Society, 2005. M. Jose-Yacaman, Luis Rendon, J. Arenas, and Mari Carmen Serra Puche, May Blue Paint: An Ancient Nanostructured Material, Science, 273: 223–225, 1996.
CH A PTER 3
The Design Context
MATERIALS IN DESIGN
In this chapter we begin to look more directly at the use of new nanomaterials and nanotechnologies in design. There are already many applications of nanomaterials in design, and more are expected soon (see Figure 3.1). We look at these topics from the perspective of designers and within the larger cultural-socioeconomic context in which designers operate. Making effective design application use of new scientific findings that seemingly appear every day within the nanomaterial field is not as easy as might first appear. History is replete with examples of seemingly fabulous scientific discoveries that surely seemed to the discoverers to have huge potential applications in many areas, only to have them lie idle for many years or not be developed at all. Reams of studies in fields such as technology transfer have looked into why this is so. Reasons vary widely but are rarely of any surprise to individuals working in a real-world development context. Design ideas may often be simply naïve, or design objectives can be confused or unclear. Target markets or user audiences may be undefined or unclear, nonexistent, or simply not large enough to be of commercial interest. Other existing products may already accomplish similar desired ends better or in a more costeffective way than the proposed product. Proposed products may never have been benchmarked against existing products. There might not be adequate test results to convince anyone of the efficacy of the product. Actual manufacturing processes for converting a science-based finding into implemental technology suitable for use in a commercial environment may either not be actually feasible or be cost-prohibitive (or not yet explored enough to know). There may be legal or institutional barriers that would prevent Nanomaterials, Nanotechnologies and Design Copyright 2009 Elsevier Ltd. All rights of reproduction in any form reserved.
42 CHAPTER 3
The Design Context
FIGURE 3.1 The Kurakuen house in Nishinomya City, Japan, designed by Akira Sakamoto Architect and Associates, uses a photocatalytic self-cleaning paint—one of the many architectural products based on nanomaterials. (Courtesy of Japan Architect.)
active consideration of a new product or cause an interested developer to think twice before proceeding. There can be user resistance from sources that should have perhaps been anticipated but perhaps were not (e.g., environmental health hazards in using new materials) or come from sources that simply could not have been easily anticipated a priori. The list can go on and on. In thinking about how we might use nanomaterials in design, it is useful to step back considerably and not define the issue simply as a technology-transfer problem—a self-limiting approach—but rather to think about it first in more fundamental terms. What is the role of materials in design? How do material properties influence the shape or form of objects and environments? What are we trying to do when we are using a specific material? On what basis do we compare nanomaterials to other high-performance materials? Do we really expect new products to be made of just nanomaterials, or if not, what specific role do we expect them to play? In what kind of product or building system might they be best used? What can we hope to accomplish? The first of these questions is by no means new. Questions surrounding the way an artifact or environment has been conceived, how it was made, and the materials of which it has been made have been a particular preoccupation of designers, engineers, and builders for ages. An understanding of the potential benefits and
Materials in Design 43
limitations of various materials is clearly evident in early works of art, architecture, and engineering (see Figure 3.2). Examples abound. Medieval builders, for example, are often said to have clearly understood the properties of stone, and they used this knowledge to help shape the arches and vaults of history’s great Romanesque and Gothic cathedrals. But what is exactly meant here by this kind of reference? Is it that the knowledge of certain properties of stone— that it is quite strong when carrying forces that cause compression within it and relatively weak when subjected to forces that cause tension to develop—somehow led directly to the creation of these complex cathedrals as we now see them? Clearly this direct line of thinking—a form of technical determinism—is highly suspect in this example, to say the very least. We do know that the use of arches and vaults, which we now know to naturally carry internal forces by a compression action, has been known since antiquity to be a good way of spanning large spaces with stone and would sensibly have been used by Medieval builders, and that this knowledge was clearly fundamental in the development of history’s great cathedrals, but it was obviously only one of many contributing factors in a landscape of complex reasons that range from the symbolic to the societal and cultural. We thus need to keep in mind that the nature of our world of designed objects and environments is not dictated by a consideration of the technical properties of a material alone, no matter how fascinating they might be; but it is equally important to acknowledge their fundamental role—we know that the introduction of new materials with improved technical properties has also led to innovative new designs (see Figure 3.3). From the point of view of this book, the best approach to understanding the use of materials in design remains through an examination of the benefits and limitations associated with the specific properties of materials. For this initial discussion, material attributes can be very broadly thought of in terms of their technical properties that stem from the intrinsic characteristics of the material itself (its density and its mechanical, thermal, optical, and chemical properties); their perceptual qualities that stem from our senses (sight, touch, hearing, taste, smell); and those culturally dependent qualities that fundamentally stem from the way our society or culture views materials. The intrinsic characteristics of materials are dependent primarily on the fundamental atomic structure of the materials and are discussed extensively in Chapter 4. Typical technical properties include failure strengths, elastic moduli values that relate deformations to stress levels, electrical conductivities, thermal conductivities, and a host of
FIGURE 3.2 The evolution of arches that act primarily in compression only was related to the inherent material properties of masonry, which can carry large stresses in compression but little in tension.
FIGURE 3.3 The introduction of materials such as steel that can carry bending stresses involving both tension and compressive stresses has allowed designers to explore new shapes.
44 CHAPTER 3
The Design Context
INTRINSIC TECHNICAL QUALITIES Strength, elastic moduli, thermal and electrical conductivity, other
VISUAL QUALITIES Transparency, opaqueness, reflectivity, texture, other
TACTILE QUALITIES Smooth/rough, hard/soft, warm/cool
SOUND/SMELL QUALITIES Sharp, ringing, dull, muffled, other
ASSOCIATIVE QUALITIES Memory/understanding transference
HEALTH QUALITIES Odors, outgassing, other
ENVIRONMENTAL QUALITIES Embodied energy, outgassing, other
FIGURE 3.4 Primary material characteristics.
other measures related to the mechanical, optical, thermal, and chemical qualities of materials (see Figure 3.4). Clearly, these kinds of properties are of fundamental importance to an engineering perspective on the use of materials in the context of designing products or buildings, and we can expect that work in the nanomaterials field can lead to dramatic improvements in these kinds of properties. At the moment, the important point here is simply that they intrinsically result from a material’s internal structure and are not dependent on any kind of societal or cultural view of the material. The perceptual qualities of a material relate to the way humans perceive them in terms of our basic senses. Visual qualities stem from a combination of specific characteristics such as transparency, translucency, opaqueness, reflectivity, and the texture of the surface (which in turn produces glossy, matte, or other appearances). Tactile qualities related to the sense of touch stem the texture of the surface—whether it is rough or smooth, its relative hardness or softness, and the feeling of warmth or coldness experienced. The qualities of materials that relate to our sense of hearing have to do with the kind of sounds—dull, sharp, ringing, muffled, low or high pitch— produced when the material is set in a vibrational mode, including by simply striking it. The sound of a metal object striking a sheet of lead is quite different than when it hits a piece of glass. In some design situations, the senses of smell or taste can be important as well. Certainly these qualities are directly related to the intrinsic properties and structure of a material. Polycrystalline materials are normally opaque or translucent because of the way light impinging on them is scattered. The sense of warmth or coldness depends on the way heat is conducted away at the point of touch, which in turn depends on both the thermal conductivity and specific heat of the material. We look at these kinds of relationships in more detail in Chapters 4 and 5. For the moment, what is important to note is that there is a basis for these qualities in the intrinsic properties of the material. But here we should also note that the way we ultimately perceive these same qualities in a neurological sense is also dependent on our own receptive mechanisms. The spectrum of light that is visible to humans or the sound wavelengths we can hear, for example, are quite different than for other animals. What we actually perceive can be quite a complex topic. We can still note, however, that since these qualities that relate to the senses remain in some way linked to specific mechanical, thermal, optical, or chemical properties, enhancing or otherwise modifying these qualities through the use of nanomaterials is entirely possible. Thus, the sense of warmth on
Materials in Design 45
touching a surface might be enhanced using nanomaterials to modify the thermal conductivity and/or specific heat of the surface material. The associative qualities of a material are placed on it by both its use context and its users (see Figure 3.5). As such, these characteristics are coupled with the context in which a material is found or used, and consequently, are ultimately dependent on the view of both individuals and society toward these materials, which are in turn culturally dependent. Specific examples are abundant and obvious here. For one, diamond is a material possessing many highly interesting intrinsic and technically oriented properties that make it extremely attractive for use in many circumstances in which extreme material hardness—an intrinsic property—is desired, as is the case in many industrial processes. At the same time, diamonds clearly possess many associative qualities placed on them by our culture and society that are fundamentally symbolic but nonetheless of real importance. The role of diamond jewelry in our society, for example, is fascinating. Yet even here, intrinsic properties of diamonds remain relevant. Humans are fascinated with the stunning color characteristics that we see when we peer into the material itself. This effect is in turn directly related to the material’s high index of refraction. As another example, we also see associative qualities present in the many synthetic materials that were historically widely introduced and used as substitutes for more expensive materials (for example, various synthetic materials introduced for flooring, such as linoleum, or for kitchen countertops). In some instances, these materials often became viewed as exactly that—cheap substitutes—no matter whether their physical properties are superior to those of the original or not. (Many technical properties of some new synthetics are indeed superior to common traditional materials.) In other cases, such as with the introduction and use of Bakelite in early radio housings, there were few negative perceptions of this type because
FIGURE 3.5 Many materials have strong associative qualities, such as diamonds or gold with wealth. In the 19th century, early buildings made of Portland concrete or cast iron, then new materials, were deliberately designed to look like stone buildings, since stone was the most prestigious building material of the era. Only later did architects such as Le Corbusier and others exploit the inherent technical properties of concrete and other new materials to create new and exciting forms. Some modern materials are still intended to resemble stone.
An early concrete building: Le Vesinet, 1864, by Francois Coignet.
A 19th century cast-iron facade in New York City.
A 21st century floor synthetic material: vinyl flooring designed to look like stone.
46 CHAPTER 3
The Design Context
the synthetic material came almost immediately to be associated with exciting new technological advances and wonderful new emerging lifestyles that allowed broad connectivity to the world at large (see Figure 3.6). Countless other examples exist. Understanding and dealing with these associative qualities is an important part of a designer’s role in dealing with objects used by the population at large.
FIGURE 3.6 The introduction of Bakelite, with its many positive qualities that allowed inventive product forms, became a symbol of forward progress and an exciting future.
Societal health concerns with the use of materials were not a terribly important consideration in describing or selecting a material until fairly recent years, when the impact of material selection on human health became better understood. We now know that the outgassing of materials within closed environments, for example, can produce a form of indoor air pollution that can cause occupant sickness. Nanomaterials are seen by some as posing potential health threats but by most others as a way of reducing them (see Chapter 11). Issues of sustainability and general environmental concerns span the spectrum from notions of how much embodied energy is used to produce a material all the way through its susceptibility to recycling are, again, responsive to societal concerns and mandates. Economic concerns, including the literal cost of a material, are everpresent. Costs of nanomaterials are known to be extremely high, which in turn suggests that they be selectively used. Both initial and long-term or life-cycle costs are important, but again these are values placed on the materials by their use in our society and our culture. There are also many forces for change that are strong drivers for new product forms. Figure 3.7 illustrates some of these driving forces at a very broad level. Many are opportunity based and evolve from either changing population characteristics or the availability of new technologies that allow needs to be met that could not be met before. Indeed, in many instances nanotechnologies are expected to be disruptive technologies that radically alter product forms. In other cases, nanomaterials and nanotechnologies will afford continuous improvement opportunities. Other broad forces for change can be characterized as concern driven. These include a wide array of issues relating to the environment, national security, and so forth. Many new products have been spawned in response to concerns of this type. In both opportunity- and concern-driven forces, a remarkable range of new scientific understandings contribute to the evolution of new or significantly adapted products. Given that externally based qualities are dependent on societal and cultural values, it is likewise to be understood that there is no
Materials in Design 47
Increasing population New science and technology Increasing functionality
Safety, health, and liability National security New or changed materials and processes
Market forces and competition Energy, water, and food
uniform agreement on the relative importance of these different qualities, as is evidenced by the intense societal debates that still occur over recycling. Though reuse of materials has been accepted as a value by broad segments of our society, anyone can still go into any store and buy products that are fundamentally designed to be cast away after use, made from materials deliberately chosen with disposability rather than recycling in mind. These societal debates are ultimately played out in very specific material choices. It is the outcome of these debates over broad societal and cultural values, however, that provides impetus for some of the greatest forces for change in the development and selection of materials.
Design Focus In thinking in more detail about how to use nanomaterials in a design context, a first consideration is simply to define what is being designed. In general, this book broadly addresses common products for everyday use as well as in architecture and related works. In this section, we briefly review the characteristics of each field separately. Ultimately, however, we will see that there are marked similarities in the basic design processes and issues present in each of these fields, despite the fact that there are also dramatic
FIGURE 3.7 Forces for change. Many societal, economic, and technological drivers lead to the development of innovative new products.
48 CHAPTER 3
The Design Context
differences as well. In many ways, differences are more easily characterized than similarities and have to do with factors such as the markets or target audiences addressed, the product’s physical size and scale, functional and assembly complexities, the number of units produced, the nature of the industry that produces the final objects, and the kind of design, engineering, and manufacturing or construction teams that bring a design from an idea to final fruition. In terms of similarities, both fields share similar issues about the need to identify product or project design objectives as well as ways to translate these needs into design requirements, generate one or more design responses (including the selection of appropriate materials) that meet requirements, resolve conflicting design objectives, and ultimately make or construct the product or project. Both products and buildings can also be generally thought of in terms of their constituent environments, systems, and assemblies. It is here where material selection issues occur. Environments may be an integral part of a design, such as spaces within a building, or they can define the external context within which a product operates. Systems and subsystems provide specific functions (e.g., heat sources, lifting). Physical assemblies and subassemblies house the components of functional systems or otherwise provide support or enclosure functions. Products can range from very simple singlefunction items (where single material type responses are common) to highly complex objects involving many complex and interacting systems that provide multiple functions. Buildings are invariably complex objects when considered as a whole and do involve complex functional systems, but they also incorporate many quite elemental components. In general, as system and assembly complexities increase, problems related to the need to resolve conflicting design objectives invariably increase as well, as do problems associated with optimizing design solutions. The idea that any single material approach will dominate a design tends to decrease. The question becomes more one of decomposing the design problem into its constituent parts that are addressable in terms of different material responses (including whether nanomaterials can be feasibly used) and orchestrating the whole to achieve design goals. We will return to these issues in Chapter 5. Another important way of understanding how nanomaterials and nanotechnologies fit into the broader design picture is via a close look at general design processes and their objectives. Many formal design processes proceed from a determination of design needs
Product Design, Architecture, and Engineering 49
and requirements and move to the determination of needed material properties and subsequent material type selection. Materials are seen as a factor to be chosen to implement a desired objective. Needs, objectives, and constraints are thus first established for a particular design approach, and a material is subsequently selected from among many on the basis of its material qualities best meeting specific design requirements. This is a common approach used in a great many design situations, particularly in engineering and in many product designs with a technical orientation. Any of several materials might meet requirements, and a design process objective is to find the best among them. We will look in detail at these kinds of structured design processes for materials in Chapter 5. An alternative design process approach is the inverse of this process. A designer becomes familiar, and perhaps even fascinated, with a particular property or set of properties and then quite literally imagines or identifies interesting design uses for the material.
3.2 PRODUCT DESIGN, ARCHITECTURE, AND ENGINEERING Products Organizations normally make products to be sold in quantity. Successful products meet market needs or demands and are associated with general user appeal and satisfaction for market targets, usability, and technical performance vis-à-vis intended functionalities and costs—all broad categories that also ultimately reflect factors related not only to direct material characteristics but to the nature of user interfaces and control systems, manufacturing process concerns, and other considerations. All successful products are in some way responsive to a market need or problem definition. Many needs have been with us for a long time, and established product forms respond to them. Lighting fixtures that provide common room illumination serve basic functions that are not likely to go away soon. The performance, control, and forms of products such as this may change, and the use of nanomaterials or nanotechnologies might offer significant performance improvements, but many basic characteristics will not be radically altered. There are, however, many opportunity- or concerndriven forces for change that are incentives for brand-new product forms. These same drivers for change are then manifested in a series of forces that characterize different kinds of more specific product
50 CHAPTER 3
The Design Context
FIGURE 3.8 General types of products according to the fundamental considerations that characterize their design forms and development processes.
development activities (e.g., market push, technology driven, user driven, or platform) briefly discussed in the next section.
Characterizing Products: A Broad Perspective There are many different ways of formally characterizing products and the design and production organizations that create them (see Figure 3.8). These distinctions become of critical importance in assessing the needed makeup of a design team, the roles played by various players at different times, the physical and use characteristics of the products, and ultimately, the selection or engineering of materials used within the final products. A user-driven product is one in which the primary value of the product depends on its visual appeal or on the perceived functionality—how a user would relate to it or use it. Though underlying technologies might be either simple or sophisticated, design emphasis remains focused on factors such as appearance, ease of use, ease of maintenance, and so forth. Industrial designers are frequently engaged at an early stage in products of this type. In a technology-driven product the primary value of the product lies with its technology or its functional capability to accomplish some specific task. User perceptions of the technical performance dimensions of the product influence selections more than appearance or even ease of use. Design emphasis thus initially focuses on assuring the technical performance of the product. For example, many products for making precise measurements fall into this category in that a user’s paramount need for accurate measurements might outweigh an obviously clumsy interface when product selections are made. The design team for these kinds of products is usually led by an engineering group of one type or another. Industrial designers might well play a role in packaging the product, but typically they are engaged later in the overall process. There are companies that produce technology-driven products for a clear or already established market area—for example, a company producing nano-based products (e.g., recording media) for use in the music industry. There are, however, many instances wherein a company starts with either a proprietary technology or a particular technological capability and then looks for a market in which these technologies could be effectively employed in creating a responsive product. In the current world of nanotechnology development, many individuals and organizations find themselves possessing unique and seemingly valuable technologies before they
Product Design, Architecture, and Engineering 51
know what can actually be done with them vis-à-vis commercially viable products other than harboring a general belief in their broad applicability to an industry, such as the automotive industry. Many current startup nanotechnology firms can be characterized in this way. Many successful products have been developed via “technology-push” processes, but the dangers and pitfalls are obvious and many. Seemingly brilliant emerging technologies have died on the vine for lack of a clear application domain. For the general “technology-push” process to be successful, there must clearly be a match with identified market needs for a product based on the technology, and then development must be carefully done to assure that the resulting product does indeed meet a market need at a competitive price. Positive benefits are that many leaders of the design team needed to develop the technological aspects of the product are typically already in place and have been involved with the core technology before. Other members are added as needed. Obviously, many products are both technology- and user-driven simultaneously or fall somewhere on the spectrum between the two extremes. Various product lines within the same family also can be targeted for positions along the spectrum. For example, many camera companies known to produce the very best of cameras with lenses designed to meet the needs of the most demanding professional photographer also make “easy-to-use” cameras designed for a consumer oriented and less technically demanding market. Interestingly, many products have been historically defined in the literature as “technology driven” on the assumption that the driving selection factor was indeed technical performance, but as these products matured and technical distinctions became less compelling, “user-driven” characteristics became more and more a determinant in users’ product selections. Many companies find themselves with existing technologies, termed platform products, developed for one application that they seek to apply elsewhere. In comparison with new technologies associated with “technology-push” products, these platform products generally have proven performance and customer acceptance records. Here we might have a product such as a paint employing nanoparticles that was developed for the automotive industry being advocated for use in another industry where similar functional needs are present, even though the industry sector is different. Many products can be described as being process intensive. In these cases, the manufacturing and production processes involved are so
52 CHAPTER 3
The Design Context
intensive, and often expensive, that product characteristics are highly determined by them. (This stands in marked contrast to products for which a market is identified and a product and appropriate process determined later.) These products are often produced in bulk form and then used as parts of other products as more or less raw constituents. Many nano-based products that could be potentially produced in bulk form, such as nanocomposites using polymeric or metal matrix materials, are process intensive and can be thought of in these terms as essentially primary products to be used in other more functionally complex products.
Production Volumes Another broad and traditional way of characterizing products has to do with long-made distinctions between high-, medium-, and low-volume production quantities—considerations that are best made in relation to the cost of the product, its technical sophistication, and its manufacturing process determinants. Clearly, many common “high-production/low-cost/low-sophistication/intensiveprocess” products are produced with great economy of scale in huge numbers by strongly deterministic manufacturing processes. The humble stamped pie plate provides an example. In terms of our discussion, these are “process-intensive” end products for which care must be taken in assuring that a competitive advantage would accrue before any even seemingly minor design variations are undertaken. (For example, is there really a market pull for elliptically shaped pie plates made of expensive high-strength nanocomposites as the base material?)
Value Further product characterizations hinge directly around relative product value as perceived by the target market. Higher perceived value is often accompanied by premium final costs to the user, particularly in technologically sophisticated products. High final product costs on the market—especially if coupled with high production volumes—can in turn justify larger research and development costs (including more extensive design and analysis activities) that are oriented toward further increasing the actual or perceived value of the product. The sporting equipment field, for example, has long been a test bed for the introduction of new materials. The value perceived by the buying audience of having a better golf club made of a new material that improves its driving power can be so persuasive that final product costs to the consumer can be surpris-
Product Design, Architecture, and Engineering 53
ingly high, often seemingly outrageously so. Even the mere suggestion that a new material or technology is employed can improve sales. Many nano-based products are already finding their way into sporting goods and are expected to continue to do so. Conversely, low-value products do not commonly enjoy the same advantages and rarely provide a setting for extensive research and development efforts that might employ new nano-based materials or technologies. The nano-based paper clip will probably not be available for some time.
General Product Complexity and Performance Products can somewhat simplistically be thought of in terms of varying degrees of complexity and performance levels. At the lowest level, products are near raw materials and provide only a few basic benefits. Many are low-value, inexpensive product forms that can be used in bulk to make other, more sophisticated products. Simple product forms such as films or sheets can be dramatically increased in value if they are engineered or processed to have particularly useful specific qualities that are fundamental to the performance of other products. This would be the case with many nano-based films, paints, or sealants as well as some other bulk forms of basic metal, polymeric, or ceramic nanocomposites. Many of these simple-appearing product forms that can be used to impart particular functionalities to other products may in themselves be quite technically sophisticated and complex internally, such as dichroic films, and be of very high value. In all cases, product forms appear relatively simple but vary in levels of technological sophistication, benefits, and relative value. To go to the other end of the value spectrum, at the highest end are finely tuned, technologically sophisticated products that provide multiple sets of controllable, specialized high-performance functions and typically involve complex electromechanical components. Extensive use of nanotechnologies are expected here. At varying levels on the spectrum, we find also items that are lowvalue products and of low complexity, such as common dishware, or relatively low-value products that serve only limited and relatively low-value functions that nonetheless have electromechanical components, such as lawnmowers and many other items. There are also high-value products not involving any kind of electronic controls, which are designed to provide the very best performance available regardless of cost, such as clubs for professional golfers (or wannabe professionals).
54 CHAPTER 3
The Design Context
Incerasing relative value of components or products
Where might nanomaterial technologies fit into this broad view of product development? Figure 3.9 speculatively suggests, in very general and admittedly oversimplified terms, relations among product value, complexity, and other general product descriptors. Trends suggest that the kinds of products or components that would initially benefit most from exploiting the unique characteristics of nanomaterials and nanotechnologies would be very high-value products with controllable functions accomplished via embedded electromechanical devices where extremely high performance, small sizes, and high strength-toweight ratios are important. Nanotechnologies and nanomaterials can make real contributions here (see Chapter 9). Disruptive changes are potentially present. One would also expect nanomaterials to be used in other high-value, high-performance products, such as sporting equipment, even when functionalities
are more limited. It is also expected that many relatively simpleappearing large-scale production forms, albeit of relatively high value, will benefit strongly from nano-based technologies, such as nano-based films, optical coatings, paints, and coverings. Here there are expected high-performance improvements in products that are very widely used in many different settings and in which performance outcomes are noticeable and important. Conversely, few immediate applications are expected in large bulk-form products for low-value applications. In some low- to mediumvalue products, one might expect to see incremental applications of nano-based technologies in specific product parts, such as enhancements to the hardness of cutting edges of lawnmower blades made possible via special nanocoatings. Many of these expected improvements are better described as continuous improvements rather than disruptive changes.
High-value components, high-performance needs, multiple controllable specialized functions and components, all appropriate for miniaturization– e.g., embedded electronic MEMS or NEMS devices. Nanomaterials can be used extensively.
Higher-value product forms, highperformance needs, specialized limited functions–e.g., films, coatings, composites for sports gear. Nanomaterials in primary structures.
Basic or raw product forms, one or few simple functions, and inherently large parts–e.g., partitions. Nanocoatings possible.
High-value products, high-performance needs, multiple controllable specialized functions and components, some appropriate for miniaturization and others inherently large–e.g., consumer products such as cell phones. Nanomaterials can be use in selected components.
Low-value products, several functions, and inherently large components–e.g., lawnmowers. Selective use.
Increasing product or component performance Increasing complexity of products (functions, controls) Decreasing size of components or products
FIGURE 3.9 General trends in product types and forms in relation to nanomaterial and nanotechnology applicability.
Product Design, Architecture, and Engineering 55
Architecture, Building Engineering, and Civil Engineering This section looks at the characteristics of the primary environments and systems that are present in architecture and civil engineering. These are individually huge fields, of course, with distinctly different design objectives and final products. Yet again there is a surprising amount of overlap in concerns, viewed from the perspective of introducing new materials into design vocabularies. These professions also necessarily come together and interact in complex design situations. Any major building, for example, is designed by a whole team of designers from different professions who undertake different roles within the process. Initial forms and organizations may well be developed by the architectural team, with the primary responsibility for interfacing with the client and assuring that overall design objectives are met, but as design development occurs, structural, mechanical, and electrical engineers quickly become involved, as do a host of other consultants (acousticians, lighting experts, and so forth), depending on the nature of the building. These disciplines interact with one another, and decisions made by each influence design acts of the others. In other domains, structural engineers would normally take primary responsibility for civil works such as bridges, but again other disciplines are quickly involved. Other branches of civil engineering would assume primary responsibility for other kinds of infrastructure of projects, but even a casual reading of newspaper accounts of any big civil engineering infrastructure projects reveals how many other disciplines are involved (from planners and architects to lighting and telecommunications experts). We obviously cannot treat nuances in detail in this text but rather attempt to highlight some of the major issues that collectively face designers of projects such as these.
The Design and Development Context Unlike products that are normally produced in quantity and sold to customers, most complex buildings are typically uniquely designed and are one-off constructions, albeit they incorporate many mass-produced products (e.g., doors) that are targeted for general use in buildings. Building projects may be sponsored by private or public groups. In the private arena, it is common for a single developer or development team to determine the general project intent and acquire a specific site for the building. The development team, often with the aid of an architect, also typically
56 CHAPTER 3
The Design Context
goes through various legal and community approval processes that are necessary to enable a project to go forward. Many feasibility studies are also naturally made at the time, since the high costs of any building generally necessitate that the costs be amortized over a long period of years. The development team typically will then engage an architectural firm to assemble a multidisciplinary project team to do the design and engineering work. This same team typically then facilitates making a contract with a construction firm to actually construct the building. Though many building components are bought as “products” (e.g., windows or air-handling units) and are simply installed by the contractor, a vast portion of the act of constructing a building is still idiosyncratic and occurs on site—for example, structural steel frames typically go up piece by piece. The design and construction team assembled to do a project might or might not ever work together again on future projects. In some cases the development team may retain ownership of the new building, but it is often the case that the development team sells it to other buyers. Whereas many exceptions can be identified, such as clients wanting “signature” buildings for one reason or another, it remains generally true that this prototypical process unfortunately does not naturally encourage exploration or risk taking with new designs—much less research that leads to a new design—that might use unproven materials, even if they might prove ultimately beneficial. In situations where the building is ultimately to be owned and operated by the same group that develops it, prospects for innovation improve. Some ownership groups might well be interested in material innovations that have particular long-term economic benefits that are not easy for a private developer to justify, particularly in the area of energy sustainability. The employment of some new approach or new material might also enhance the image of a company in a positive way and thus increase the market appeal of its products and hence the company’s ultimate revenue stream. Apple Computer stores in the United States, for example, have successfully promoted a particular kind of high-tech lifestyle image that is achieved via innovations in design and material choice—an image that ultimately improves the company’s bottom line. Other examples include many stores that sell sophisticated sporting equipment, racing bicycles, fashion clothing, or other high-end goods. These are “high-value” buildings where high-end design is considered worth paying for. It is here that most interesting and innovative material explorations in architecture occur. The fact that a line of buildings is being built also helps defray additional design
Product Design, Architecture, and Engineering 57
costs over several buildings rather than just one. In terms of exploring where nanomaterials might eventually find building owners immediately receptive to their use, it is indeed this kind of highvalue building where the association with nanotechnologies could also serve to enhance the appeal of the company’s products. Another important aspect of the way buildings are designed and built is that their nature is highly dependent on not only the specific programmatic needs to which the building is responding but also to specific site locations and conditions. Climatic conditions associated with specific locations, for example, can dramatically influence external environmental conditions and must be taken into consideration and impact material choice. We can see obvious manifestations of the way that building shapes, forms, and material choices have evolved over time in indigenous building construction throughout the world in response to local climatic conditions. High-mass masonry walls such as adobe are commonly found in hot and arid parts of the world—a consequence not only of material availability but also because the thermal lag cycle associated with the way the material absorbs and emits heat is particularly useful in creating comfortable interior environments in areas where there are hot and dry days but where nights are cold. Heat is absorbed by the thermal mass during the day and reemitted at night, when it is needed. We can see other responses in hot and humid areas or in temperate zones. Even with today’s seemingly advanced mechanical technologies, many interesting technologies and related material choices (including many of the interesting active double-layered curtain wall systems) that have proven so successful in energy-sustainable buildings in the temperate climate of Europe have not proven equally successful in the more extreme climates of other countries. Electrochromic glass that is now benefiting from developments using nanomaterials, for example, has been widely touted vis-à-vis its usefulness in meeting sustainable design objectives, but the heat gain associated with current types of electrochromic glass is dependent on sun angle and makes it most effectively used primarily in high-latitude zones. Many of these kinds of locational dependencies can ultimately affect material choice. There are, of course, many other locational dependencies related to urban or rural conditions, access to transportation, and so on that could be noted here as well. This kind of location dependency is normally less prevalent in product design. The general processes noted here are quite different from those associated with thinking about developing a product. In the building field, there are indeed some cases in which a building is
58 CHAPTER 3
The Design Context
conceived, designed, built, and marketed much more like a product. A salient example here might be modular housing, which is now so ubiquitous. Multiple units are built in a factory and marketed and sold more like a product than a building. Specific sites are not considered, but broad locational dependencies remain important. The same is true for various kinds of premade “industrial” buildings. In current practice, however, these are usually fairly low-end products resistant to significant innovations, despite many attempts to the contrary.
Building Types One of the most important characteristics of buildings to always keep in mind is that they must provide habitable spatial environments for living, work, or other common life activities that range from the cultural to entertainment; thus we can think about buildings in terms of different kinds of fundamental spatial environments. One way of looking at these environments is simply by building type—hospitals, laboratories, housing, and the like. A whole host of defining characteristics spring to mind when thinking about each, as do differences among types. Essential differences between hospitals and housing complexes are patently obvious and suggestive of not only uses but differences in overall forms and spatial organizations, types and uses of spaces, types of infrastructures (mechanical, electrical, telecommunications, etc.)—all the way down to images of specific material requirements or needs (as might be present in hospital operating rooms, for example, with their needs for surfaces that do not host bacteria and that are easily cleanable). Thus, a building types perspective can suggest a whole host of design requirements and subsequently stated design objectives that are useful for designers and engineers. The perspective becomes considerably less useful in other instances, particularly in cases where buildings serve multiple functions and must be designed to adapt to different uses over time. Building types also come and go; we have very few harness shops being built today. More generally, a types perspective can detrimentally lead to framing broad design questions in a restrictive way. Nonetheless, the approach is often used and it is valuable within the context of this book. Other approaches to thinking about buildings are from the perspective of physical assemblies and systems (structural, mechanical, and so on). The following section briefly explores the idea of systems, particularly their functional definition.
Environments, Systems, and Assemblies 59
3.3 ENVIRONMENTS, SYSTEMS, AND ASSEMBLIES The design of any product or building is a complex undertaking. It requires both understanding and manipulating the whole form as well as orchestrating the many components and systems that make up the form and give it usability or functionality. As a way of understanding the design tasks at hand, it is useful to take a moment to first look at products and buildings via the nature of the involved physical environments, systems, and assemblies. Environments may be alternatively considered as either an integral part of a design, such as spaces within a building, or as defining the external context within which a product operates (see Figure 3.10). Systems are generally defined as physical components or parts that work interactively to provide some particular type of function. In architecture, systems of one type or another may serve to support building environments. In products they might provide the immediate function that characterizes the product itself, as in a lighting system. Assembly considerations spring largely from issues of manufacturability or constructability as well as from broader ideas about modularity and other assembly architectures.
Environments The notion of thinking of design in reference to various kinds of critical environments is a common approach. For buildings and some products, such as automobiles, we might think about the nature of the spatial environments that are occupied by humans. For products, we might think as well about the special characteristics of surrounding environments or those that are intrinsic within a product that might influence design approaches. In both products and buildings, broad considerations of thermal, sound, lighting, and mechanical issues are invariably important. In many situations, chemical factors might be a concern, as in designing a product for use within a surrounding environment that is corrosive or in considering the health effects of material outgassing in a closed habitable environment. Electromagnetic environments might be important in designing specific products. Common material properties play a fundamental role vis-à-vis these issues, and thus nanomaterials can be expected to play a role as well. Many other products can be described in terms of their use environments. Interface characteristics are particularly important here. Chapter 9 addresses these environments in detail. Here we review salient issues.
ENVIRONMENTS Spatial Surrounding
GENERAL CHARACTERISTICS Lighting Thermal Mechanical Sound Chemical Electromagnetic
FIGURE 3.10 Basic kinds of design environments in buildings and products.
60 CHAPTER 3
The Design Context
In a building, for example, the spatial environments where we live, work, or play are the raison d’être for the whole building. These spatial environments have specific configurations that are geometrically defined. They also have particular environmental qualities that support our well-being, make us comfortable, or support our tasks. We can consider these environmental qualities in terms of their primary thermal, lighting, and sound characteristics (Figure 3.10). For example, designers must provide an overall thermal environment that is comfortable for inhabitants. This, in turn, is normally accomplished via a complex set of passive material and ventilation elements and supporting mechanical systems (e.g., ubiquitous heating, ventilating, and air-conditioning systems) that function together to maintain the temperature of the room at prescribed levels. The geometric characteristics of the space, the nature of the surrounding walls, or the kinds of glass present in fenestrations, including their material characteristics, are all contributors to defining the thermal environment actually perceived by the occupant. Similar observations could be made about lighting environments. There are lighting systems that provide specific lightemission capabilities, but the physical characteristics of surrounding walls and windows contribute to the kind of luminous environment provided. The material reflectivity of wall surfaces or the amount and kind of light that passes through windows (which depends on the relative transparency of the window material) all play a fundamental role in defining the kind of lighting environment that’s ultimately provided. In these and similar situations, the primary evaluation metric is invariably associated with some type of measure that is related to the environmental parameter itself, such as final lighting levels at a particular task or living area within the space, rather than to a specific supporting component, such as emissions from a lighting system, albeit the latter’s contribution to this measure can and should be assessed due to its integral contribution. In a product design situation, the performance of a thermos bottle with an internal volume designed to keep liquids hot or cold can be evaluated vis-à-vis the degree to which it can maintain the temperature of the liquid inside. Various kinds of mathematically based simulation tools can be used to aid in these kinds of performance predictions. Thus, in the thermos bottle, various analytical approaches or models can be developed that take into consideration temperature differentials between the inside and outside of the bottle and the thermal heat-transfer properties of the bottle material. The performance would be found to obviously depend on particular material properties but also on other parameters, such as the geometry of
Environments, Systems, and Assemblies 61
the bottle, that are not directly material dependent. The use of these kinds of computational models that play out the role of material properties in relation to other design parameters is intrinsically important in designing any object. Figure 3.11 suggests several typical examples of where and how nanomaterials are now or potentially can be applicable. Note that nanoscale coatings are expected to be used in many applications—lighting control or manipulation, surfaces that are self-cleaning, scratch-resistant, or anti microbial, and others.
Systems and Assemblies Systems are normally defined as those sets of subsystems and components that perform some type of functionally defined role. A sophisticated design may consist of several primary systems that have both functional and physical characteristics but that are primarily thought about in functional terms. In this discussion, a system is generally defined as a series of lower-level subsystems and related functional components that collectively provide a larger function important to the use and operation of the whole configuration and that interact with one another. The provided function is intrinsic to the operation or existence of the whole. Several systems typically make up a complex design (e.g., a lifting system is part of a forklift assembly; a heating system is part of a building). Systems may have both functional and physical connotations (e.g., a power supply is defined primarily in functional terms, but the system is necessarily ultimately made up of a physical set of components that exist within a given layout). Primary systems in turn may consist of several subsystems that can each be considered as serving a specific function that contributes to the role of the system as a whole. Subsystems usually have functions that are quite well defined but of greater complexity than the lower-level functions served by components such as simple motors. Assemblies are defined in terms of the sets of physical subassemblies and parts that are ultimately assembled as physical objects in a manufacturing or construction sense. This is a purely physical definition of the way individual parts are assembled into everlarger groupings to eventually form a whole. At the lowest level there are parts that are more or less irreducible from an assembly hierarchy perspective—for example, basic cast housings—and that typically have limited and well-defined functions. The metrics defining the relative success or failure of a particular assembly design normally have less to do directly with product performance or use but everything to do with manufacturing assembly speed
GENERAL ENVIRONMENTAL Air and water and other fluid purification and movement, odor control, other LIGHTING ENVIRONMENTS QLEDS, lasers, optics Nanofilms and nanocoatings Reflection, transmission, absorption, refraction, wavelength tuning Antireflective, antiglare, brightness enhancing, other Transparency/color-changing films and glasses Electro-optical displays Other THERMAL ENVIRONMENTS Nanoporous materials–insulation Nanofoams, aerogels, other Nanocomposites–conduction Thermal barriers, heat exchangers, heat spreaders Heating/cooling devices Thermoelectric, other Other MECHANICAL ENVIRONMENTS Nanocomposites for strength, stiffness, hardness, other Nanocoatings–hardness, corrosion resistance, other Vibration/damping control Damage monitoring Active/responsive structures Other SOUND ENVIRONMENTS Speakers, microphones, damping, other CHEMICAL ENVIRONMENTS Fuel cells, catalytic converters, corrosion, purification, other ELECTROMAGNETIC ENVIRONMENTS Nanotechnology-based chips, magnetic storage, supercapacitors, batteries, shielding, solar cells, electro-optical displays, other
FIGURE 3.11 Basic design environments in buildings and products and typical examples of where nanomaterials or nanotechnologies can be applied (see Chapters 9 and 10).
62 CHAPTER 3
The Design Context
and ease, assembly time, types of machines required, special conditions, and so forth. In many cases, functional and assembly systems might be identical, but in other cases they might well be different; for example, various components of a functional system might be distributed in several different but interconnected subassembly units. However, constituents in a subassembly must still share a logic for being housed together. Reasons can vary: Constituents of a subassembly might be of similar sizes. They might all need to be assembled using a particular robotic device. They might all share a need to be protected from moisture or heat. Other criteria for creating subassemblies might be the stipulation that maximum external housing dimensions for all subassemblies be the same—a requirement that might literally force the placement of elements from various functional subsystems into different housings. The basic distinctions we’ve drawn here are not always clear in real design situations, and terminology is by no means always agreed on (for example, what is one person’s functional subsystem may be another’s physical component). The use of multifunctional parts or subassemblies obviously complicates the making of simple characterizations. A simple connecting bolt may well serve to position multiple parts of a power supply system and a cooling system simultaneously and cannot easily be “assigned” to one larger system or another. Indeed, a major task in early design phases is to identify where parts or components serve multifunctional or cross-functional roles. Failure to do so can sometimes result in redundant and needlessly complex overall solutions. There is not really any overarching way of describing or characterizing the kinds of systems and assemblies found in product design. As a simple gesture for discussion purposes, the diagram shown in Figure 3.12 suggests some basic characteristics of common products. Most sophisticated products contain control/logic systems or interfaces used in the direct operation of the product or in monitoring its functions. An energy system for power input, storage, conversion, or transfer is often present. Products exist for some purpose; hence an action system or process system is invariably involved that includes many supporting components. Many other elements are present as well, including structures or frameworks for which the function is to house other systems. Often many subsystems that have their own characteristics and functionalities are present. Obviously, not all products have all these characteristics; some might not be present at all (as in a simple table). In other cases, the basic
Environments, Systems, and Assemblies 63
CONTROL/LOGIC COMPONENTS: INTERFACES User interfaces–direct operation and control, monitoring (sensors, other), component/assembly interfaces, other
Action/process Structures Surfaces/enclosures
ENERGY SYSTEM COMPONENTS Energy or power input, storage, conversion, and transfer components
Other Control/logic Devices/control/logic
ACTION SYSTEM DEVICES AND PROCESS COMPONENTS Sensors, control and logic components, signal carriers, transducers and modifiers, direct action or process components Mechanical/electrical/thermal/ chemical/optical devices Sound/light and other devices
COMPONENT SUPPORT STRUCTURES
Structures Surfaces/enclosures Other
Control/logic Energy Action/process Structures Surfaces/enclosures
STRUCTURES AND FRAMEWORKS SURFACES, ENCLOSURES, AND CONTAINERS Surface structures, coatings, finishes, sealants, other ACCESS. HANDLING, AND OTHER COMPONENTS Structures and surfaces Mechanisms and other devices
PRIMARY STRUCTURE AND ENCLOSURE
TYPICAL PRODUCT Diagrammatic illustrations of common types of functionally defined systems and subsystems in an electronically complex product. Nanomaterials or nanotechnologies have applicability in most of the systems and subsystems illustrated, e.g., sensors, energy, enclosures.
GENERAL Self-cleaning, self-repairing HEALTH Antibacterial, antifungal, antimold, antipollutants, and purification COLOR/LIGHT Reflective and antireflective, emissivities, brightness enhancing, other THERMAL Reflection and emissivities, thermal barriers TRIBOLOGICAL FUNCTIONS Hardness, wear, lubrication ELECTRICAL Conductive/dialectric Static dissipation, other OTHER
Surfaces of products are always of crucial importance. The list to the left suggests some of the possible applications of nanomaterials and nanotechnologies for surfaces or surface treatments.
FIGURE 3.12 Diagrammatic illustrations of common types of functionally defined systems and subsystems in an electronically complex product. Obviously, not all products have this complexity or all the subsystem elements shown. For other products, few of the systems shown may apply; for example, a box is a structure and enclosure and nothing more. Nanomaterials or nanotechnologies have applicability in most of the illustrated systems and subsystems.
64 CHAPTER 3
The Design Context
description presented is actually played out many times over in a highly complex or sophisticated product, with many components that are “products” in their own right becoming “constituent” components within a larger and more complex product. Figure 3.12 suggests examples in which nanomaterials and nanotechnologies can play a role in systems found in products. To industrial designers, the role of the “surface” of a product is particularly important. There are many potential applications of nanomaterials in surfaces, such as self-cleaning, antimicrobial, improved abrasion or scratch resistance, self-healing, and others (Figure 3.12). In buildings, the common description used for constituent systems includes structural systems; heating, ventilating, and cooling systems; lighting systems; sound systems; enclosure and fenestration systems (walls, doors, windows); transportation systems (elevators, escalators); fire-protection systems; various kinds of information and control systems; and others (see Figure 3.13). Basic ideas of hierarchical system/subsystem/component and assembly/subassembly/part relations are fundamental to the field. Similar observations can be made about systems and assemblies in bridges and other civil works, albeit bridges and similar constructions tend naturally to focus primarily on specific systems (e.g., structural). Many components that make up the assemblies and systems in buildings, such as telecommunication or lighting components, are in themselves complex and high-value “products” in every sense of the word. On the other hand, the nature of building often requires many on-site construction activities that make massive use of relatively low-level “products” that are almost raw materials or marginally removed from them, such as concrete. Large sizes of components and low volume of use and production issues are even more present in these conditions than in more traditional products. Figure 3.13 suggests where nanomaterials and nanotechnologies might play a role in relation to building systems—for example, nanotechnologies in control systems or electro-optical displays, sensors, energy systems (including solar cells), films and coatings on enclosure panels or glass windows, water and air purification, and others. Figure 3.14 shows a brief selection of several buildings using some type of nanoscale material. As with products, surface characteristics of the type listed in Figure 3.12 are again extremely important. Many of these functionalities, such as self-cleaning or antimicrobial, are based on photocatalytic effects. Large surfaces with photocatalytic properties can also contribute to pollution reduction to a limited but useful extent (see Chapter 10).
Environments, Systems, and Assemblies 65
Indoor air-quality improvements Air cleaning and purification Water cleaning and purification Thermal, lighting, sound Wastes
PRIMARY AND SECONDARY STRUCTURAL SYSTEMS ENERGY SYSTEMS LIGHTING SYSTEMS
COMPONENTS AND SYSTEMS
THERMAL/AIR–HEATING, VENTILATING, AND AIR CONDITIONING SOUND SYSTEMS TRANSPORTATION SYSTEMS WATER/WASTE SYSTEMS FIRE PROTECTION SYSTEMS ENCLOSURE AND FENESTRATION SYSTEMS Interior and exterior walls Windows Other
Surfaces and enclosures Self-cleaning, self- repairing, antimicrobial, light and color, hardness, thermal, sound, other Structural Members, vibration damping and active response and control, damage, monitoring, other Energy Solar cells/films, fuel cells, batteries, sensors, controls Communications, information, alerts Electro-optical displays sensors and control systems Environmental, including biohazard alerts Fire, other
FIGURE 3.13 A typical way systems are described in buildings is shown at left. The list on the right suggests examples of where nanomaterials or nanotechnologies might find applications in buildings. Many of the surface-related applications are based on hydrophobic, hydrophilic, and/or photocatalytic technologies (see Chapter 10).
Trends II As we delve more deeply into nanomaterials in subsequent chapters, it will become increasingly clear that certain forms of nanomaterials or nanotechnologies can play a more effective role in some systems or assemblies than in others. Whole complex products consisting of multiple components will not normally be made exclusively of nano-based materials or technologies. Specific components might very well involve their use, depending on performance requirements. We can expect, for example, that nanotechnologies will play a central role in high-value electronic control and interface systems that support products, as well as in energy systems (generation, storage, distribution) or lighting systems. Nanocomposites might also find use in specific situations in which high performance is necessary, such as making high-value components lighter and stronger. Other nano-based products, such as films, coatings, and paints, are also
expected to be used widely because of their interesting potential for self-cleaning, self-repairing, and other capabilities, discussed in Chapter 10. In general, widespread uses will initially be highly selective. In buildings, similar trends are expected. Developing nanomaterial use can be expected in control, monitoring (including sensors), and other systems with high-value components or where performance needs are particularly high. Applications in lighting are expected to be high. Nano-based films, coatings, paints, and insulation are also expected to quickly find wide applications. Nano-based paints and other surface treatments based on photocatalytic properties are expected to become widespread quickly. (Making photocatalytic surfaces is relatively inexpensive.) Nanoporous materials can benefit thermal insulation as well as air and water purification objectives. Chapters 10 and 11 discuss these expected trends in more detail.
66 CHAPTER 3
The Design Context
Many optical films with nanoscale layers have light transmission and reflection properties that are angularly dependent and are thus affected by the relative positions of the object, the light source, and the viewer. The same object is shown in both images at right.
The Dragon’s Lair in London uses a self-cleaning glass. The glass has a nanoscale coating but does not contain actual nanoparticles; see Chapter 10. (Courtesy of Pilkington.)
The Strucksbarg housing project by Renner Hainke Wirth Architekten uses a self-cleaning paint based on photocatalytic technologies. (Courtesy of Christof Gebler, Hamburg)
Concrete is poised to benefit from nanomaterial innovations in its mixing qualities, strengths, and other properties. Self-cleaning and antipollutant concrete has also been explored (see Chapter 10). The Dives Church in Misericordia in Rome, by Richard Meiers and Partners, shown here, uses self-cleaning concrete.
FIGURE 3.14 Several examples of how nanoscale materials are currently being used. Applications include many optical films for light, color, or thermal control; light-emitting devices (QLEDs); surfaces that are self-cleaning, antibacterial, or self-healing and that aid pollution reduction; nanofoams and nanogels for thermal insulation; solar cells; and a host of applications related to the strength and stiffness of members (see Chapters 9 and 10).
Textiles are being made stronger, tougher, and more abrasion resistant using nanocomposites, as well as imparting properties such as self-cleaning, antistaining, antimold, flame retardancy, and others. The Columbo Center in Lisbon is shown. (Courtesy of Birdair.)
Thermal insulation properties of enclosures can be improved through the use of nanofoams. Translucent nanogel-filled panels are shown in this view of the Four Points Hotel, Manchester, New Hampshire.
Environments, Systems, and Assemblies 67
Unitary and Modular Design Approaches to Systems and Assemblies Determining appropriate relationships between functionally driven and physically driven design responses is one of the major tasks of a designer. There are design choices that can be made about how specific functions may be assigned to particular physical parts or subassemblies, or, alternatively, distributed among several. Pursuing one or another direction has dramatic implications on the resulting qualities of the design and the way it is ultimately produced. Here we look at consequences of carrying one or the other of these approaches to an extreme. The broad distinction introduced here is between two general design approaches. In the first approach, holistic designs evolve from a systemic arrangement of discrete but interactive modules that house particular functions and/or that have particular standardized geometries. In the second approach, the overall design is carefully built up as a single whole and without subassemblies or components that are easily or necessarily distinguishable as such. First, it is useful to consider what is meant by the term module in relation to any design activity. The term refers to a selfcontained or distinct and identifiable unit that serves as a building block for an overall structure, but within the context of a prescribed or orchestrated set of interactions that relate to the performance of the whole object (see Figure 3.15). This broad meaning can have both physical and functional connotations. A general implication of a modular design approach is that all modules are replaceable without completely disassembling or changing the whole configuration. There are many ways the term module is actually used. For example, the term modular design can assume a primarily functional meaning. In computer programming it generally refers to an approach in which separate logical tasks are reduced to “modules” of manageable sizes and programmed individually, albeit within the context of carefully prescribed interactions. In product design there are many examples of modules that are primarily functionally defined, such as a power module, although some physical shaping and dimensional implications are usually present as well. By contrast, the term module can also assume primarily a physical meaning. Here, it refers to a standardized unit of size. In its more extreme form, a “modular” physical design thus generally refers to an overall design based on the
Module 1 Function 1
Interfaces and Controls Shared Components - Power - Other
Module 2 Functions 2 Module 3 Function 3 Module 4 Function 4 ... Module n Function n
Modular design with functional subsystems housed within dedicated subassemblies; subsystems and subassemblies are identical.
Module 1 Functions 1a/2b
Interfaces and Controls Shared Components - Power - Other
Module 2 Functions 2a/1b Module 3 Function 3/1c Module 4 Function 1c/1d ... Module n Function n/n+
Modular design with functional subsystems distributed across several physical subassemblies; functional subsystems and physical subassemblies are not identical.
FIGURE 3.15 Modular design approaches.
68 CHAPTER 3
The Design Context
use of a prespecified dimensional array (typically in the form of integral multiples of given dimensions) that serves to define the sizes and locations of all parts and subassemblies (locations of connection or interface points are often predefined as well). This latter physically based approach is widely used in many diverse fields. In building design, this approach is widely used in connection with prefabricated building elements, whereas in electronics the same conceptual approach is used to structure the sizes and shapes of electronic devices to go on larger circuit boards. This physically based notion of modular design is extremely important when it comes to manufacturing and assembly and can literally define the maximum “envelope” and location of “connectivity” points that a designer of any component must respect. In many physical approaches, there is often a literal supporting physical infrastructure (e.g., the board with the holes in largely modularly designed electronic devices) that provides a rationalized support system. Connective systems that are usually primarily functionally defined are used to link one module to another. This modular approach clearly places a premium on the potential positive benefits associated with design ease and rationality, the potential for easy product variety and upgrades (vis-à-vis module interchangeability capabilities), direct maintenance (in the form of access and component replaceability), and straightforward manufacturing and assembly. The whole must obviously be made to work functionally. However, there is nothing implicit in the modular approach that a priori guarantees ideal part or component locations with respect to functional or use issues. In poor modular designs, there can be high redundancy, the need for additional support and infrastructure elements, and sometimes a loss in ideal performance. Interface and Control Shared Components - Power - Other
Function 2 Function 1
FIGURE 3.16 Holistic design approaches. All systems and subsystems are tightly housed within a single assembly fabric.
These modular design techniques stand in marked contrast to single holistic design approaches. In these approaches, rarely are specific functions associated with specific distinguishable physical subassemblies (see Figure 3.16). Rather, the actual parts and elements making up various functionally defined systems or subsystems may coexist in the same internal spaces and be located throughout the whole design in an integral way. Single constituent entities often serve multiple or cross-functions. The driving force in this design approach is to focus on the final characteristics of the end product and to position elements internally such that they perform their respective roles in a collective way that
Environments, Systems, and Assemblies 69
is most optimal for the performance of the whole design. Following this objective can result in tight designs with little redundancy and high performance. Shapes can become highly complex and derivative of the need to integrate all systems together (normally in a closely packed arrangement). These same holistic design strategies often make replacement of components difficult in a unitary design and correspondingly can potentially make upgrades and maintenance concerns much more difficult as well. Whole units may well have to be replaced for even simple upgrades (albeit this is already a common trend in microelectronics and other fields that has proven acceptable to the market). For many products there have been increasing pushes toward smallness. This is particularly true for sensors, chips, and other electronic devices that are commonly integrated into some larger product form. This push has long been under way and has led to some remarkable technological developments in the form of microelectromechanical systems, or MEMS, devices. These devices are fabricated using the same technologies employed in the microchip industry, and hence they can be extremely small. They need not be solely electronic but can be small mechanical systems as well. Figure 3.17 illustrates several MEMS devices. Functionalities can be highly developed, such as “labs on chips” for performing various analyses (also see Chapter 11). These devices are invariably holistic designs. There is no notion of part exchangeability or subsequent repair. They is highly focused devices. The next step in the evolution of these devices is expected to be nanoelectromechanical systems (NEMS) that utilize nanotechnologies and synthesis methods.
A dust mite walking across gears in a MEMS device.
A tiny gear train.
FIGURE 3.17 The recent push toward smallness is exemplified by MEMS, which are normally made using microchip technologies. NEMS are expected to be the next stage of evolution. (Courtesy of Sandia National Laboratories.)
Trends III In terms of nanomaterial and nanotechnology use, the continuing affordances offered by nanomaterials and nanotechnologies in achieving ever greater size reduction and miniaturization of even highly complex functional subsystems are highly compatible with holistic or unitary design philosophies. Figure 3.18
suggests general trends. The adoption of nanotechnologies, with their small sizes and increased functionalities, will enable far more tightly integrated unitary designs than are now commonly available. Miniaturization trends already in progress via MEMS technologies will undoubtedly continue. MEMS devices Continued
70 CHAPTER 3
The Design Context
may well be enhanced via nanotechnologies, or whole new families based on nanoconcepts alone will emerge as NEMS devices. Many products that have complex functionalities may well appear as simple small objects with few or no visible distinguishable features. Still, the miniaturization trend will apply to certain products only, particularly those special-function devices that are intended for integration into other more complex product forms. Many components that require direct human interfaces will grow smaller, but interface needs will keep aspects
of them larger. Other products might have large features because of certain of their functionalities, such as tennis racquets, which must exist at the macroscale in order for them to be useful. Even macroscale products, however, can be expected to become stiffer and lighter because of nanocomposites and have enhanced functionalities. Ideas of modularity and other design approaches will remain applicable with large products. At the building scale, modularity will remain a common design approach.
Increasing use of nanomaterials and nanotechnologies. Increased miniturization, increased functionalities relative to size, decreased weight, changes to precision manufacturing techniques necessary for nanotechnologies. Increasing use of unitary designs.
METER SCALE: Conventional products, large- and small-scale components. Modularity common.
CENTIMETER SCALE: Overall size reductions are limited by human interfaces. Process, mechanical, or lightemitting and sound components can remain large.
FIGURE 3.18 Impact trends in technologically complex products as a consequence of introducing nanomaterials and nanotechnologies. Some products are expected to become very small, whereas others will have size limitations due to functionalities or interfaces.
MILLIMETER SCALE: Products without human interfaces. Overall size decreases are easier. Any lighting/sound components remain fairly large.
MEMS SCALE: Miniaturization. Sophisticated functions.
NANOSCALE: Sophisticated special functions. Extreme miniturization.
3.4 THE DESIGN AND DEVELOPMENT PROCESS The Overall Development Process Typical product development processes may be generally thought of as occurring in several broad steps: definition of design needs or requirements, concept development, concept and preliminary design, design development, preproduction prototyping and evaluation, and production design. The design process does not necessarily march so literally from one step to another without a backward look. Good design work often comes from processes characterized as being the result of convergent back and forth iterations. Wellreceived design proposals are typically those that both meet functional requirements and have the kinds of design appeal with respect to both visual and user interface qualities that have long been known to characterize successful product designs. Of particu-
The Design and Development Process 71
PRODUCT DESIGN Market need: Design requirements
Define specification Determine function structure Seek working principles Evaluate and select concepts
Develop layout, scale, form Model and analyze sassemblies Optimize the functions Evaluate and select layouts
Analyze components in detail Final choice of material and process Optimize performance and cost Prepare detailed drawings
lar importance in user-driven products are critical issues that center around classic design characteristics such as form, proportion, materiality, color, tactility, and so forth. Also critical are issues of what designers frequently call design consistency. Terms such design coherency or design integrity imply broadly similar concepts. These concepts generally refer to the extent to which a design collectively holds together with respect to a collective view of visual, interface, and functional issues. Figure 3.19 suggests a broad view of the design flow process, from identification of market needs or a new idea to a final product specification. A first step is typically that of identifying what the product needs to do and what kind of market the product is addressing. What needs must be met or what requirements must the product fulfill? Are there specific constraints that the product must be designed to respect? More broadly, how is the design problem framed? Ultimately, design requirements are established. There are formal and informal methods for accomplishing this end (see the
Program or brief
Concept, feasibility, and approvals
Design development and engineering
FIGURE 3.19 Design flowcharts for product design and architecture. Overall processes are similar, but terminology is different. In product design terminology, the design proceeds from the identification of a market need, clarified as a set of design requirements, through concept, embodiment, and detailed analysis to a product’s specifications. Architectural processes are broadly similar.
72 CHAPTER 3
The Design Context
section on structured design processes that follows). In formal methodologies in product design, early steps often include decomposing the problem into as many subproblems as possible (sometimes creating a subsolution importance hierarchy). Not all subproblems necessarily have to be solved at once by a proposed design. Some subproblems may have preexisting solutions, whereas others do not. Many are ultimately more important than others in determining the critical design essence of a final solution. Concept development stages follow. Generating initial design proposals is a straightforward task to a design professional; it involves its own internal structures and logics. (The process is not nearly so mysterious as is sometimes portrayed.) For an overall project, many designers typically internalize fundamental product requirements and goals as well as characteristics of prior design precedents and then identify, quickly explore, and rapidly delineate one or more generative design concepts. Frequently, new material characteristics will suggest original design solutions. Preliminary and design development stages follow, whereby the functionality and physical form of the promising concepts are increasingly resolved and studied. (This is sometimes called the embodiment stage in product design or preliminary design in architecture; see Figure 3.19.) A series of geometric and functional modeling and technical evaluation studies are normally undertaken, as are initial cost studies. Subsequent steps include defining in detail the series of related systems and subsystems that provide a given function or set of functions. A result of the first part of this general process is to have a set of design requirements for each system or element detailing what it needs to do in unambiguous terms. These specifications are normally performance oriented but are much more technically directed than the more generic target requirements used in preliminary designs, which typically relate more to user need perspectives. For some subsystems, input and output values must be within specified ranges. Other examples might be those of specifications for a mechanism that require it to provide a given pushing force over a specified stroke distance. A pressure vessel might have to be able to contain a specified internal volume and pressure. By this stage of the process, there should also be clear understanding of the maximum envelope dimensions of any particular assembly of subsystem components and where (in a physical layout sense) connections are made to related subsystems. The detail or design development and engineering phase of the development process
The Design and Development Process 73
builds explicit material solutions and/or physical devices. Specialized design and engineering teams usually undertake this process. Final material selections are determined at this point. Numerical simulation analyses (e.g., functional, structural, thermal, or other) are normally used to verify that an anticipated product meets original design requirements. Once all systems and subsystems have been physically and functionally defined, the design team again addresses the overall design form that has been evolving in parallel. A major objective here is to make sure that there are no physical or functional system “conflicts.” Quite often a system might simply not be able to fit in the intended space. There may be spatial conflicts between elements of different systems. (In building design, structural and mechanical system components often seem to have affinities for occupying the exact same physical spaces.) Or, in other situations, the proximity of one electronic system to another might require special shielding. The list goes on and on. All these events would require design alterations, either to the whole assembly or within its systems. The process is typically iterative. In product design, the term systems approach is often used to characterize these procedures (see Figure 3.20). In subsequent stages, physical objects are also generally shaped in relation to anticipated production processes, that is, designing parts so that casting or molding procedures are ultimately possible. Specific design for manufacturability or design for assembly principles may be explicitly followed as well. Sometimes formal design for manufacturing and assembly methodologies with proprietary components can also be used.
FIGURE 3.20 The systems approach to the analysis of a technical system, seen as transformation of energy, materials, and information (signals). This approach, when elaborated, helps structure thinking about alternative designs.
74 CHAPTER 3
The Design Context
As part of the design efforts we’ve noted, various kinds of experimental prototypes may also be made during this stage. These prototypes serve to test one aspect or another of a design and help in the refinement and integration process. They may be functional prototypes that work as intended but are not yet physically packaged in their final anticipated physical form. These prototypes serve many broader roles as well, including fostering communication with all members of the design team (and with management and clients as well). Alpha prototypes are built using part geometry and intended final materials but are not necessarily fabricated in the same way intended for final production processes or by using the same machines. As part of this process, several competing final-use materials may still be tried for different parts. Actual material testing could occur, in which products are placed in intended-use environments that are known to be difficult (e.g., a high-temperature environment). The look, feel, and performance of the alpha prototype, however, must match its final production descendant. Beta prototypes are further developed and normally use parts produced directly by the actual production processes intended for use. Individual parts, however, might be assembled differently. Beta testing by the user community within its own operational environments is widely acknowledged as a good way of debugging the final design and uncovering any reliability problems. Final design corrections are subsequently made. The final stage of production design involves making initial runs of the product, normally done using the actual intended production process. Initial runs are quite carefully monitored for production quality. Some units may be again placed into a user context for further evaluation and testing. Normally production levels are quite small at first while process bugs are worked out and the workforce is trained. In combination with a marketing and distribution plan timetable, the product then goes into higher-volume production and is subsequently officially launched.
Structured Design Processes in Relation to Materials Despite the complexities of overall development process issues we’ve discussed, specific material characteristics remain fundamental shapers of the design result. Some design problems can be very limited in scope and dictated primarily by the technical properties of various materials. By contrast, there are also more open-ended design problems in which many external factors might
The Design and Development Process 75
influence material choices, and there can be little or no determinism based solely on singular technical factors. The latter often also include multiple design objectives involving material choices that might even be in conflict with one another. In many situations involving well-defined design problems, design processes including materials can be relatively straightforward and consist of a series of sequential steps. A structural engineer designing a beam that is part of a flooring system for a building, for example, typically assesses the external loads acting on the member and determines the forces and bending moments using welldeveloped structural analysis algorithms that relate the geometrical and material properties of a beam to the kinds of internal stresses and deformations that are developed. Cost functions could also be constructed. Depending on the design objective, such as minimum weight or minimum depth, the process can then be structured so that by specifying design criteria related to strength and stiffness, variables such as specific required material properties (minimum yield stress levels or needed modulus of elasticity) can be determined explicitly for the material to be used in a specified beam crosssection. (Alternatively, material properties could be specified and geometric properties of the cross-section determined.) Subsequently, different kinds of screening processes can be used to select real materials with the needed properties from existing databases of material properties. Design processes of this general type occur in many engineering fields literally by the thousands each day and form the working basis for many common design development activities. In the scenario just illustrated, we clearly defined the function of the object to be designed. Clear design objectives, such as minimum weight or minimum cost, could also be easily specified. Constraints—for example, how much load the member has to support—could be specified as well. Design variables or parameters might then be either the geometric and dimensional characteristics of the beam for a given material or material properties themselves for a given beam geometry. Material selection procedures directly follow. More generally, the process of selecting a material includes the following steps: the translation of design requirements, screening using constraints, ranking using objectives, and documentation (see Figure 3.21). These processes are elaborated on in Chapter 5. As design objectives become more complex, so do design processes. Meeting more complex design conditions might involve trying to achieve multiple design objectives simultaneously as well as meeting multiple constraints. These are invariably difficult goals
Translate design requirements: Express as function, constraints, objectives, and free variables
Screen using constraints: Eliminate materials that cannot do the job
Rank using objective: Find the screened materials that do the job best
Seek documentation: Research the family history of top-ranked candidates
Final material choice FIGURE 3.21 Material selection processes. Chapter 5 discusses in more detail structured approaches for selecting materials.
76 CHAPTER 3
The Design Context
to accomplish. Optimally meeting some design objectives might necessitate a relaxing of others. In thinking yet again about simple thermos bottles, the function might be thought of as a need to hold and provide a transport container for hot or cold liquids. Dimensional constraints might exist—for example, such that the bottle could be carried in a typical bicycle bottle holder. An externally imposed constraint might initially be that the unit cannot exceed a certain cost (benchmarked from an analysis of a competitor’s product). The choice of primary material might be open. Here the designer might want to optimally meet several design objectives: minimizing the weight of the container since it is for use by bicyclists, maximizing the length of time a contained liquid would remain at an initial temperature level, or minimizing the cost of the whole unit. Meeting all these design objectives simultaneously (i.e., optimizing all design objectives) is at best a difficult and sometimes unachievable task. Compromises are often made and tradeoffs normally occur. Nonetheless, the designer can choose which of the design objectives is initially most important and which are less so (i.e., rankorder design objectives for optimization). For serious cyclists, weight might well be most important to the user and thus be the governing design objective for the designer. Thermal performance might well have to be compromised, and cost constraints may simply be ignored for all practical purposes. For everyday cyclists, costs and thermal performance might well be more important than absolute weight. Different design solutions will invariably result, depending on what objectives are most highly valued. Definition or prioritization of design objectives, therefore, often depends on the use context or other external driving forces. Situations with design objectives that are inherently conflicting can, on one hand, try the souls of designers, but on the other hand they have provided both the spark plug and the setting for innumerable innovations in the materials world. Tradeoffs and value stipulations are invariably required to move forward.
Unstructured Design Processes In the prior section, material-oriented design processes were seen to progress from a determination of design objectives and requirements to the determination of needed material properties and subsequent material type selection. Materials are seen as a factor to be chosen to implement a desired objective. Needs, objectives, and constraints are thus first established for a particular design
The Design and Development Process 77
approach, and a material is subsequently selected from among many on the basis of its material qualities best meeting specific design requirements. This is a common approach used in a great many design situations, particularly in engineering and many product designs with a technical orientation. Any of several materials might meet requirements, and a design process objective is to find the best among them. The process is certainly relevant to designing with nanomaterials, but it obviously demands that the useful mechanical, optical, thermal, and chemical properties of the nanomaterials be reliably known. At the current time, data of this type in a form useful to designers is often not readily available. An alternative approach, often initially viewed as not rigorous and even unseemly by more scientifically oriented designers, flips the whole process. A designer becomes familiar, perhaps even fascinated, with a particular property or set of material properties and then quite literally imagines or identifies interesting design uses for the material. In this scenario, formal definitions of needs or design requirements do not come first. To be sure, the considered material does ultimately respond to some perception of needs or uses in a particular design context, but a material orientation is set first. This process is less deterministic and more opportunistic than the former. Its procedural steps are more difficult to formalize, but they are surely there for the experienced designer. It involves the systematic study and experimentation of the properties of a material by a designer, who internalizes these findings and who has a large portfolio of design problems to solve or design opportunities to explore. An internalized “fit” process occurs between material affordances and design opportunities. It is a time-honored and effective way of designing with materials. Interestingly, it appears to be one of the primary modalities that is operative in the nanomaterial world at the moment. Various nanomaterials have different technical properties that can be fascinating. What can we do with these kinds of nanomaterials? What applications can we imagine? Many other approaches evoke different processes or are somehow combinations of the two extremes we’ve noted. Many designers’ long preoccupation with objects that are “strong and light” is a case in point. In some cases there might be a strong technical or use reason for making something strong and light, as is the case with many handheld consumer products on one hand or aircraft components on the other hand, whereas in other cases there simply might not be (e.g., it is only marginally important that a park bench be really light in weight, and, indeed, extreme lightness could be
78 CHAPTER 3
The Design Context
problematical). The design value of “strong and light,” however, might remain as an initial generative factor for a design, perhaps because the idea is symbolically associated with other designed objects that have captured our societal imaginations, such as aircraft. Why were many objects that were designed in the 1930s— including not only locomotives but vacuum cleaners and other common household goods—given “streamlined” appearances? It is, after all, rather hard to argue that the wind resistance provided by a floor vacuum cleaner is a particularly important functional generator of design form. The associative design value of “streamlining” and its related material suggestions of “sleek metallic,” however, have long been with us and remain widespread as symbolic of newness and innovation. This is particularly true in many consumer-oriented products in which the ideas of “associative” properties, briefly discussed earlier, can be highly important.
A DESIGN VIGNETTE
FIGURE 3.22 Boston Symphony Hall. This concert hall is well known for its fine acoustics.
As a way of entering into a discussion of design issues in relation to materials in architecture, let’s first look at a highly particularized vignette: the design of a concert hall for listening to music. Here the material issues would seem to immediately devolve into classical technical problems of choosing materials with the right acoustical properties in relation to sound absorption or reflection. We, however, poke at this assertion here. This same vignette is used as a brief introduction to the way design processes occur.
FIGURE 3.23 Vienna’s Grosser Musikvereinssaal is another fine concert hall. Designing concert halls for premier acoustical performance is extremely difficult. Halls suitable for one music type are rarely optimum for other types.
Any music aficionado knows that there are great halls—Vienna’s Grosser Musikvereinssaal, Amsterdam’s Concertgebouw, Boston’s Symphony Hall, and many others that are well known to performers and listeners alike (see Figures 3.22 and 3.23). By contrast, many others—some recent—have been designed with good intent but have simply failed to become known as good concert halls. Even the casual music listener knows that the quality musical experience an audience receives is very much dependent on the acoustics of the hall and that the seemingly odd shaping of a hall has something to do with this experience. The more careful observer would comment that in some places and not others, drapes are hung, and that many walls are covered with different kinds of soft materials in various places. Undoubtedly, our more knowledgeable observer would also know or suspect that these same materials might have something to do with absorbing or preventing unwanted sounds and their reflections from reaching the listener. But not only are the surfaces absorptive; hard surfaces can also be seen to be
A Design Vignette 79
suspended in selected locations—clearly to direct sound reflections without reducing them significantly. To the designer, all these issues—geometric configurations, placements of different materials with different properties (which might indeed have different absorptive qualities appropriate for different locations), placements of reflectors, and many other factors—are surely things that someone in this situation (presumably an architect working with an acoustical engineer) has to decide. To the developer of a new material, including nanomaterials, who is seeking to develop application domains, the situation would be viewed as a design case where there is a need to have materials with different sound absorptive or reflective characteristics. The question might merely seem to be one of, “What values?” In developing a design for a concert hall, experienced architects know that all the issues we’ve noted are interrelated and each affects the other; they would also know that there are no single solutions, and many variants might have similar performances. The design team charged with the task of developing a design would do many things, but thinking about specific material choices would come fairly late in the design process. The exact framing of the problem leading to these choices, however, is done quite early. In terms of steps, a series of immediately relevant programmatic issues are first identified (often through interviews and other techniques), and subsequently a series of stated design requirements are worked out: what kind of hall, for what type of music, for how many listeners, what ancillary facilities must be present, and so forth. Within this context, specific design objectives would be established. Broad design objectives might be at a seemingly obvious level: to design a hall that provides a high level of musical experience for the audience (an objective that could presumably be subsequently defined more precisely in terms of various descriptors of the acoustical performance of the hall). A more precise objective might be to say that each listener seated somewhere in the hall must have the same high level of experience no matter where he or she is seated (something potentially much harder to accomplish). These and other factors are usually defined in a design brief or design program of some sort. The designers would then generate a series of initial conceptual design proposals that impart an initial physical design sensibility to the programmatic requirements (e.g., initial layouts showing locations of the stage, seating arrangements, and so forth). This would have to be done with conscious consideration of the actual site involved (not only its area and shape but also its
80 CHAPTER 3
The Design Context
relation to streets and proximities to other buildings and elements of the urban infrastructure). Most of this work is primarily configurational and normally does not yet involve detailed material considerations. Initial internal configurations for the acoustical space are often based on the designer’s own professional knowledge of what configurations might work and be worth further development or, as is often the case with concert halls, the shaping might come from a series of precedent studies of other concert halls known to perform well that are of a similar size and in a similar situation. Preliminary reviews and evaluations are then typically made with all stakeholders in the final hall. These stakeholders include client/ owners, representatives from the music world (perhaps the conductor or others who will eventually play there), and any other person or group with a vested interest in the hall. During this process, broad design possibilities are invariably narrowed, and, ultimately, one is normally selected for further development. Preliminary design proposals are then developed that show the design in more detail. Here a better shaping of the internal acoustical volume is defined. At this point in current practice, the building is represented (via traditional means such as drawings or via a computer-generated model) in sufficient detail for all involved to understand the nature of the design. After further evaluations with stakeholders, a design proceeds to an intensive design development and engineering process to resolve the design even further. During this process, design teams involving various disciplines— acoustical engineering, lighting, structural, and so on—work together to develop the building. During this process, both twoand three-dimensional computer models of the whole building are commonly used to represent the design and to allow participants in the design process to share information with one another. The design development and engineering step is normally where intensive studies are made of the potential acoustical performance of the space. To the material’s engineer, the immediate and obvious point of interest is that the sound absorptive and reflective qualities of the materials undoubtedly play a pivotal role here. But exactly what role is this? What specific values are needed? If an acoustical engineer is asked what single metric is of primary importance in evaluating the acoustical performance of a space, it is undoubtedly not whether a measure of sound absorption in a particular material or set of materials is high or low, but it might well be the reverberation time of the whole acoustical volume. (Reverberation time is a measure of the length of time, in seconds, in which a listener hears an emanated sound
A Design Vignette 81
as it arrives at various direct and reflected paths to his or her ear; see Figure 3.24.) Long rolling sounds can be heard, or quick sharp ones. Reverberation time is a measure that involves a consideration of material properties, but it is not limited to them and includes a measure of the geometric characteristics of the room. This idea of a primary evaluation metric being associated with the phenomena of interest rather than solely a material measure is common in all design fields. Materials may well play a crucial role, but the focus is invariably on the phenomena of interest. The common way the role of material properties is understood with respect to a phenomenon such as sound is via the use of analytical or mathematical models that relate the involved variables to one another with the overall goal of performance prediction in relation to the phenomena of interest. Here various kinds of computer-based analysis or simulation models are typically used to scientifically model the way sound flows throughout the space. These models typically require the specification of configurations, materials, and all other design factors, including material qualities, that influence the way sound propagates through the space. The designer or acoustical engineer can then make various studies of how specific spatial shapings or material placements would affect the acoustical qualities of the space and attempt to ascertain whether original design objectives are met. By this time, broad criteria such as “musical experience” are no longer useful; more well-defined measures must be employed. Sometimes actual scale models of the space as well as mathematically based simulation models are constructed so that designers and acoustical engineers can use other mediums to gain this same kind of understanding. (The making of prototypes in the product design field is analogous.) All through this complex procedure, other detailed architectural or engineering studies are being worked on as well. Some of these, such as structural design considerations or fire protection or egress requirements, might well have an impact on the acoustical qualities of the space and need to be taken into account. A typical problem encountered here is that many common materials currently used for sound control are poor choices when viewed from these other perspectives. The soft, sound-absorbent materials that have historically been used in this connection, for example, have also long been known to contribute to the spreading of flames and the development of toxic gases during fire circumstances. Special attention must be paid to make sure that focus is not solely on one design
Listener Direct sound from source
Direct plus multiple reflections
Sound arrives at different times, creating a reverberant field
Sound reflectors and absorbent materials modify reverberant field and sound heard at a point
FIGURE 3.24 Reverberant sound fields in building design. The actual sounds from a source heard by a listener include both direct and reflected sounds that take different lengths of time to reach the hearer, thus leading to reverberation effects. Reflected sounds are affected by the absorption qualities of the materials used in reflective surfaces. Absorption qualities are often varied by using soft or hard materials, depending on how sound paths need to be controlled for optimum listening.
82 CHAPTER 3
The Design Context
consideration at the expense of another equally important one. Common practice in this kind of situation is to be sure that the materials used meet certain minimum conditions with respect to each considered phenomenon. In many cases, design objectives for the materials are directly conflicting, and making material choices again often involves making considered compromises, as was the case with the closely related design optimization problem noted previously. This simple example brings up the need to consider materials with multidimensional properties, which we return to in Chapter 5. To the developer of nanomaterials or other new materials for use in a situation such as this, the problem is no longer one of how to impart only sound absorption qualities nor even one of what specific values are needed, but how to develop materials that meet multiple objectives. Any number of other considerations might come into play as well. A designer intent on working with a company that might have developed a new nanomaterial coating that has seemingly attractive sound absorption or reflectance qualities may also have to face perfectly reasonable questions of environmental safety. An obvious question that arises is one of whether or not the coating poses a health hazard in any way. Does it contribute to indoor air pollution through offgassing, or are there particulates that might come from the application of the material? What test results are available to demonstrate that this is or is not a problem? If not already available, tests or experiments can only rarely be commissioned in the architectural world. Costs are high and would have to be borne by the project’s owner. Unlike products for which costs can be distributed over multiple units, costs in a building are normally associated with a single product that is designed and produced only once—a problem that clearly militates against testing and experimentation. The list of other considerations goes on and on. The interior designer might want to have shiny surfaces in some places and matte surfaces in others. An owner would undoubtedly ask, “How long will it last?,” “Can it be cleaned?,” as well as the obvious “How much does it cost?” As the design development progresses, stakeholder evaluations and inputs continue but necessarily become oriented to more detailed considerations. Ultimately, a decision is made to advance to construction—a process often requiring specific types of drawings and other representations of the design and involving yet other parties in a consideration of the design’s buildability. Minor changes to the design typically occur all the way through the final construction phase.
A Design Vignette 83
Now that we have gone through the typical steps in a design process, let’s look more critically at parts of it. Was the original design objective reasonable? Consider the objective “to design a hall that provides a high level of musical experience for the audience.” Though it’s seemingly reasonable, if we stopped at only this objective we could get a hall that is unexciting or uninteresting to musicians themselves—a feeling that would undoubtedly affect more general perceptions of the hall. It is well known, for example, that the qualities of not only the hall but the stage and other components affect how musicians play a hall. The stage, for example, can literally vibrate in a way such that it becomes rather like an orchestral instrument. Common experience also suggests that there is a relationship between the type of music played and the acoustical qualities of the performance space. Gregorian chants sound marvelous in spaces with long reverberation times (5 to 10 seconds)—times commonly found in spacious Medieval cathedrals. Secular Baroque music, with its clear articulated sounds and low fullness of tone, was originally played in relatively small rooms with hard surfaces— rooms with low reverberation times. Music of the Romantic period plays best in halls with longer reverberation times and low directto-reflected sound ratios that produce a fullness of tone and low definition. Music historians have long known that composers of these periods well knew the acoustical qualities of the halls in which their works were to be played. Richard Wagner is known to have composed his romantic Parsifal especially for the Festspielhaus in Bayreuth, Germany. In a like way, hall qualities evolved in response to the music of the day, which was in turn dependent on a whole realm of complex cultural conditions. What is fascinating here, but problematic in design terms, is that, if this idea is carried to its logical conclusion, there is only one type of music that can be best played in a hall with a particular configuration and choice of materials qualities. Even if we speculate on the contributions that nanomaterials might make in terms of the optimization of selected material properties, such as absorption, the overall design for a concert hall can be truly optimized for only one music type as long as the property is a static one. The sound absorption coefficients of various materials that play so critical a role in the acoustics of the space are not actually constant for a given material but rather depend on the frequency of the impinging sound waves. Ultimately, this means that a set of materials can be chosen to optimize a single configuration and single type of music to be played within it but not necessarily for all types within the same hall! Choices come
84 CHAPTER 3
The Design Context
down to optimizing the hall for specific music types or using a series of suboptimal solutions that allow a wider variety of music to be played within it, albeit not in an optimized way. On a more general level, this same broad problem of design optimization with respect to various performance measures runs through most complex design problems and is not an easy one to address. We will return to this problem in Chapter 5. These realizations make the overall design problem more acutely difficult, and the problem of there being no single solution that optimizes all performance needs necessarily requires that design goals and objectives be clarified. For many settings, a preferred aspiration might be to have a hall that works well for as many musical venues as possible, albeit not necessarily ever optimized for any one. Implications vis-à-vis specific design issues, such as material choice, ensue. Choices must be made. A further assumption made in the overall design scenario we initially presented is quite simply that the discussion immediately assumed only natural acoustical music; no consideration was made of electronic assists in either amplification of direct sound or in its distribution through speakers located throughout the performance setting—an unthinkable assumption to many current musicians but natural to others. The impact on music of developments in electronics needs no comment here; it is all around us. This impact has been extended to concert halls. Why should the all-important reverberation time depend solely on geometrical and material characteristics? In this day and age, the reverberation time can be electronically altered and controlled through a careful orchestration of speakers and responsive manipulation and control systems. Many music settings of this type no longer even have any internal shaping designed to promote natural acoustics, and material implications follow. These interesting developments pose even further challenges to the designer. Electronic advocates would argue that electronic assists offer improved performance in general, and surely much current music is designed specifically to be played in “electronic” halls but would sound poor in even the best of the 19th century concert halls. Others would simply offer a pitying smile at assertions that equivalent quality exists. These interesting matters might not be solely the province of the architect and acoustical engineer to determine, but their resolution surely has an impact on the final nature of the building and the materials selected. Just as surely, these designers can play a fundamental role in helping the electronic vs. nonelectronic decision process by playing out design implications and providing performance simulations. The
Further Reading 85
fundamental role of the design team as clarifier of design intent thus reappears. Now that we have explored the seemingly endless chain of interdependent design issues that invariably affect material choice in a concert hall, let’s go back just for a moment and look again at our original design assumptions: that our purpose was to design a hall that provides a high level of musical experience for the audience. Everything followed from this seemingly perfectly reasonable design objective. How could anyone argue? The history of architecture and other design fields, however, is literally filled with examples in which a metric associated with a seemingly unassailable functionally driven design objective is overshadowed by some other, and perhaps less obvious, design objective. In designing for stage performances, for example, optimum views of the stage from the spectator boxes and seats as defined by clear sight lines and proximity would seemingly be a primary design determinant. Yet in the Renaissance period, we know that desirable seats were often those that had only adequate views of the stage but excellent views of the remainder of the theater. This reflected the understood social value at the time that seeing the audience was as important as seeing the stage. In many Baroque theaters, the royal box did have a good view of the stage, whereas other spectator seats often had poor orientations toward the stage. Here, the most desired seats were often the ones with the best view of the royal box, with it’s vice versa implication (“to see and be seen”). Clear lines of sight and proximities to the stage were simply less important. Thus, the social interactions and conventions provided the dominant design context. We note this example simply to serve as a warning that design problems can often be too easily characterized. A good design team will spend a good amount of time being sure that the initial design question is correctly framed in its broadest possible sense.
FURTHER READING The language and approach in sections of this chapter dealing with characterizing products were largely adopted from sources such as Karl T. Ulrich and Steven Eppinger, Product Design and Development, McGrawHill, 1995, although terms such as modular have been used for years in many and various design contexts. The ideas are certainly not new to experienced designers. Design process discussions were drawn from several sources, including the following books by Michael Ashby that elaborate in much more detail on many of the topics presented here. The book by Leo Baranek is an immensely interesting book on acoustics.
86 CHAPTER 3
The Design Context
Michael F. Ashby, Materials selection in mechanical design, 3rd ed., Butterworth-Heinemann, Elsevier, 2005. Michael Ashby and Kara Johnson, Materials and design: The art and science of material selection, Butterworth-Heinemann, 2002. Leo Baranek, How they sound: Concert and opera halls, Acoustical Society of America, 1996. Karl T. Ulrich and Steven Eppinger, Product Design and Development, McGraw-Hill, 1995. Frederick Sports, Bayreuth, Yale University Press, 1994.
CH A PTER 4
Material Classes, Structure, and Properties
CLASSES OF MATERIALS
If you stop for a moment and look around you, you will notice a wide variety of materials, either artificially produced by humans or naturally existing in nature. Both types can be categorized in particular classes to provide a better understanding of their similarities and differences. In this book, we distinguish seven classes: metallic, ceramic, polymeric, composite, electronic, biomaterials, and nanomaterials. However, as you will note, some materials have characteristics across various classes.
Metallic Materials Metallic materials consist principally of one or more metallic elements, although in some cases small additions of nonmetallic elements are present. Examples of metallic elements are copper, nickel, and aluminum, whereas examples of nonmetallic elements are carbon, silicon, and nitrogen. When a particular metallic element dissolves well in one or more additional elements, the mixture is called a metallic alloy. The best example of a metallic alloy is steel, which is composed of iron and carbon. Metallic materials exhibit metallic-type bonds and thus are good thermal and electrical conductors and are ductile, particularly at room temperature.
Ceramic Materials Ceramic materials are composed of at least two different elements. Among the ceramic materials, we can distinguish those that are predominantly ionic in nature (these consist of a mixture of metallic elements and nonmetallic elements) and those that are covalent in nature (which consist mainly of a mixture of nonmetallic elements). Nanomaterials, Nanotechnologies and Design Copyright 2009 Elsevier Ltd. All rights of reproduction in any form reserved.
88 CHAPTER 4
Material Classes, Structure, and Properties
Examples of ceramic materials are glasses, bricks, stones, and porcelain. Because of their ionic and covalent types of bonds, ceramic materials are hard, brittle, and good insulators. In addition, they have very good corrosion resistance properties.
Polymeric Materials Polymeric materials consist of long molecules composed of many organic molecule units, called mer (therefore the term polymer). Polymers are typically divided into natural polymers such as wood, rubber, and wool; biopolymers such as proteins, enzymes, and cellulose; and synthetic polymers such as Teflon and Kevlar. Among the synthetic polymers there are elastomers, which exhibit large elongations and low strength, and plastics, which exhibit large variations in properties. Polymeric materials are in general good insulators and have good corrosion resistance.
Composite Materials Composite materials are formed of two or more materials with very distinctive properties, which act synergistically to create properties that cannot be achieved by each single material alone. Typically, one of the materials of the composite acts as a matrix, whereas the other materials act as reinforcing phases. Composite materials can be classified as metal-matrix, ceramic-matrix, or polymer-matrix. For each of these composite materials, the reinforcing phases can be a metal, a ceramic, or a polymer, depending on the targeted applications.
Electronic Materials The electronic class of materials is a bit broader than the previous classes because electronic materials can encompass metals, ceramics, and polymers, such as the metal copper that is used as interconnects in most electronic chips, the ceramic silica that is used as optical fibers, and the polymer polyamides, which are used as a dielectric. However,the term electronic material is used to describe materials that exhibit semiconductor properties. The most important of these materials is silicon, which is used in practically all electronic components. Other materials such as germanium and gallium arsenide are also part of this class.
Biomaterials The biomaterials class is related to any material, natural or synthetic, that is designed to mimic, augment, or replace a biological
The Internal Structure of Materials 89
function. Biomaterials should be compatible with the human body and not induce rejection. This class of materials is rather broad and can comprise metals, ceramics, polymers, and composites. Typically these materials are used in prostheses, implants, and surgical instruments. Biomaterials should not be confused with bio-based materials, which are the material parts of our body, such as bone.
Nanomaterials The nanomaterial class of materials is extremely broad because it can include all the previous classes of materials, provided they are composed of a structural component at the nanoscale or they exhibit one of the dimensions at the nanoscale. The prefix nano represents a billionth of a unit, so the nanoscale is normally considered to span from 1 to 100 nanometers. Nanomaterials are typically categorized as 0-D (nanoparticles), 1-D (nanowires, nanotubes, and nanorods), 2-D (nanofilms and nanocoatings), or 3-D (bulk), which represent the number of dimensions that are not at the nanoscale (see Chapter 6).
4.2 THE INTERNAL STRUCTURE OF MATERIALS Atomic Structure What are things made of? Everything is made of atoms. How do we know? It is a hypothesis that has been confirmed in several ways. To illustrate the idea of how small an atom is, observe Figure 4.1. If a strawberry is magnified to the size of the Earth, the atoms in the strawberry are approximately the size of the original strawberry. Let’s now ask another question, which is: What are the properties of these entities called atoms? We shall divide the properties of atoms into two main categories, namely inertia and forces. First, the property of inertia: If a particle is moving, it keeps going in the same direction unless forces act on it. Second, the existence of short-range forces: They hold the atoms together in various combinations in a complicated way. What are these short-range forces? These are, of course, the electrical forces. What is it in the atom that can produce such an effect? To answer this question, consider the Bohr atomic model, depicted in Figure 4.2. In the Bohr atomic model, there is a nucleus consisting of protons with a positive charge and a mass of 1.67 × 10−27 kg and neutrons with no charge but with the same mass as the protons. The nucleus is surrounded by electrons with a negative charge and a mass of
FIGURE 4.1 Relative dimensions of an atom, a strawberry, and the Earth.
n=1 n=2 n=3
FIGURE 4.2 Schematic representation of the Bohr atom.
90 CHAPTER 4
Material Classes, Structure, and Properties
9.11 × 10−31 kg that revolve around the nucleus in discrete orbits. Thus, the nucleus is positively charged and very heavy and the electrons are negatively charged and light. Let’s now think about another aspect: What is particular about particles such as electrons, protons, neutrons, and photons? Newton thought that light was made up of particles and therefore should behave the way particles do. And in fact light does behave like particles. However, this is not the whole story. Light also behaves like a wave. How can particles such as electrons and light exhibit this dual behavior? We don’t know. For the time being we need to accept this, keeping in mind that on a small scale the world behaves in a very different way. It is hard for us to imagine this because we have evolved in a different kind of world. However, we can still use our imagination. This is the field of quantum mechanics. Let’s explore the first idea of quantum mechanics. This idea claims that we are not allowed to know simultaneously the definite location and the definite speed of a particle. This is called the Heinserberg Uncertainty Principle. In other words, we can only say that there is a probability that a particle will have a position near some coordinate x. This is akin to watching Shaquille O’Neal throw a basketball to the basket. You can’t say that he is going to hit the basket for sure! There is also a certain probability. This explains a very mysterious paradox, which is this: If the atoms are made of plus and minus charges, why don’t the electrons get closer? Why are atoms so big? Why is the nucleus at the center with electrons around it? What keeps the electrons from simply falling in? The answer is that if the electrons were in the nucleus, we would know their position and then they would have to have a very high speed, which would lead to them breaking away from the nucleus. 0
3d 3p 3s 2p 2s
-1.55 -3.45 -5
FIGURE 4.3 Electron energy states for a hydrogen atom.
So far, when we have been talking about atoms, we have considered their lowest possible energy configuration. But it turns out that electrons can exist in higher-energy configurations. Are those energies arbitrary? The answer is no. In fact, atoms interchange energy in a very particular away. An analogous idea is to have people exchange paper currency. Imagine that I want to buy a CD that costs $17 and that I only have $5 bills. Further imagine that the CD store only has $5 bills in the cash register. In this case, the CD I want to buy will cost either $15 or $20, depending on which party wants to assume the loss. Atoms are very similar. They can only exchange certain “dollar bills.” For simplicity, let’s look at the hydrogen atom (see Figure 4.3). As shown in this figure, the ground energy for the hydrogen atom is −13.6 eV (electron volts). Why is it negative?
The Internal Structure of Materials 91
The reason is because electrons have less energy when located in the atom than when outside the atom. Therefore, −13.6 eV is the energy required to remove the electron from the ground energy level. If an atom is in one of the excited states E1, E2, and so on, it does not remain in that state forever. Sooner or later it drops to a lower state and radiates energy in the form of light. The frequency of light υ that is liberated in a transition, for example, from energy E3 to energy E1, is given by
υ = (E 3 − E1 ) h
where h is Planck’s constant. Each energy level or shell is represented by the principal quantum number n, as shown in Figure 4.3. However, if we have equipment of very high resolution, we will see that what we thought was a single shell actually consists of several subshells close together in energy (Figure 4.3). In fact, for each value of n there are n possible subshells. In addition, in each subshell, it is possible that different energy states may coexist. We are still left with one thing to worry about, and that is: How many electrons can we have in each state? To understand this problem, we should consider that electrons not only move around the nucleus but also spin while moving. In addition, we should consider a fundamental principle of atomic science, which is the exclusion principle. The exclusion principle says that two electrons cannot get into exactly the same energy state. In other words, it is not possible for two electrons to have the same momentum, be at the same location, and spin in the same direction. What is the consequence of this? Two electrons can occupy the same state if their spins are opposite. Where can we put a third electron? The third electron can’t go near the place occupied by the other two, so it must take a special condition in a different kind of state farther away from the nucleus (see Figure 4.4). From this discussion, we can now realize that there is a spin moment associated with each electron, which must be oriented either up or down. Because every spinning electrical charge is magnetic, the electron acts as a tiny magnet. However, when two electrons are in the same orbital with opposite spins, the magnetic effect is counteracted and there is no magnetic effect. With the ideas mentioned so far, we can now understand the periodic table. We should keep in mind that (1) the number of electrons in an electrically neutral atom depends on the number of protons in the nucleus, (2) an electron will enter the orbital possessing the least possible energy, and (3) only two electrons can fit into any one of the energy states.
+ + +
Spin-up electron Spin-down electron
FIGURE 4.4 Atomic configurations for real spin one-half electrons.
92 CHAPTER 4
Material Classes, Structure, and Properties
All elements can be classified in which the position of the elements enables the prediction of the element’s properties. The periodic table is subdivided into horizontal periods and vertical groups. The group indicates the number of electrons in its outermost shell. This property is very important because the outer electrons, being less tightly held to the nucleus than the inner ones, play the most important role in bonding. These are called the valence electrons. Thus, all atoms in Group I have one valence electron; those in Group II have two, and so on. On the other hand, the Period indicates the outermost energy shell containing electrons. Thus, all atoms in Period 3 have electrons in the third shell; atoms in Period 4 have electrons in the fourth, and so on.
r = 0.57 A
r = 0.57 A
FIGURE 4.5 Two atoms of hydrogen widely separated. The atomic radius is 0.57 Å.
d = 0.74 A
FIGURE 4.6 Sharing of electrons in the hydrogen molecule. The covalent radius r = 0.37 Å is now less than the atomic radius.
Atomic Bonding In the last section, we looked at the elements one by one. Now, based on the information we have acquired, we can imagine that it is possible to form a large variety of materials simply by combining different atoms with each other. How is that possible? If an atom is electrically neutral, why will an atom combine with other atoms? Remember what we have discussed before! When an electron is closest to the nucleus it will possess the least amount of energy. Hence, the closer it is to the nucleus, the more tightly it is held. In this context, we might now understand why atoms can combine with each other. For simplification, look again at the hydrogen atom (see Figure 4.5). As shown in the figure, when two atoms of hydrogen are sufficiently apart, their atomic radius is 0.57 Å. Now let’s see what happens when you bring the two atoms close enough (see Figure 4.6). The nucleus remains unchanged, but the electrons become attached to each nucleus and are brought closer to them. In this fashion, the electrons are shared by the two atoms, and as a consequence the system reduces its overall energy. Therefore, atomic bonding occurs because both electrons are now attached to both nuclei. This is why hydrogen usually occurs as the molecule H2. The distance of 0.74 Å is then the equilibrium distance between the two atoms of hydrogen when forming the molecule, and thus the net force is zero. This can be expressed as FN = FR + FA = 0
where FN is the net force, FA is the attractive force, and FR is the repulsive force. This net force of zero corresponds to a minimum in energy. As a result, the system is in a state of less energy when
The Internal Structure of Materials 93
the atoms are bonded together than when the energy used in each individual atom is added. In other words, the hydrogen molecule is more stable than each individual hydrogen atom. Thus, the hydrogen molecule is the result of overlapping electron orbitals. This overlapping of orbitals is called a chemical bond. Despite the fact that chemical bonds can be formed by atoms of the same kind, when atoms bond chemically, the properties are very different from those of the individual atom. For example, atoms of sodium (Na) and chlorine (Cl) bond to form NaCl, which is common table salt; however, individually, Na burns exposed to air, and Cl is a poisonous gas. The reason we are so interested in chemical bonding is because the material properties and the processing of materials will depend strongly on the kind of chemical bonding that exists between the atoms. For example, materials that exhibit different bonding energies between their atoms will possess very different melting temperatures. Hence, high melting temperatures are associated with strong bonding energies. What about materials with high stiffness properties? By the same token, these materials also possess high bonding energies. The same applies for the coefficient of thermal expansion. It is now evident that materials with large bonding energies will possess smaller atomic vibrations and thus lower coefficients of thermal expansion. Let’s look at the types of chemical bonding that exist in nature. We start with perhaps the easiest type. This is ionic bonding (see Figure 4.7). It always happens in compounds composed of both metallic (Groups I and II A) and nonmetallic (Groups VI and VII A) elements. The role of the metallic element is to give its valence electrons, whereas the role of the nonmetallic element is to accept them. Again, the best example of this type of bonding is common table salt, NaCl (Figure 4.7). The sodium atom, with only one very loosely held electron in its outermost shell, bonds with one atom of chlorine, which has two paired orbits and one half-filled orbit in its outermost shell. When the sodium atom approaches the chlorine atom, overlapping takes place, resulting in bonding. However, the electron donated by the sodium atom spends most of its time near the chlorine atom, making the sodium atom a positively charged ion and the chlorine atom a negatively charged ion. As a result, the bond formed is ionic. In terms of properties, the ionic bonding is isotropic, which means that the bonds have the same characteristics in all directions and possess high bonding energies. As a result, ionic bonded materials exhibit higher melting temperatures, brittleness, and poor electrical conductivity.
FIGURE 4.7 Ionic bonding in sodium chloride—NaCl. The sodium atom “lends” one electron to the chlorine atom and becomes a positively charged ion, whereas the chlorine atom becomes a negatively charged ion.
94 CHAPTER 4
Material Classes, Structure, and Properties
One other type of chemical bonding is covalent bonding. In this type of bonding, there is a high probability of electrons spending most of their time in the region between atoms. Thus, for example, when two atoms of hydrogen form a molecule, the shared electrons spend most of their time in between the two hydrogen atoms. What would happen to the bonding if, for some reason, both electrons were on one side? The bonding would no longer be covalent. It would become an ionic bond because one atom would have an excess of electrons, whereas the other one would have a depletion of electrons. In general, although covalent bonds are very strong, materials bonded in this manner have poor ductility and poor electrical conductivity. Thus, for example, when silicon is bent, bonds must be broken for deformation to occur. This is not easy. In addition, for electrons to be mobile, bonds must be again broken. Therefore, covalent bonded materials are usually brittle and insulators. Core
FIGURE 4.8 A metallic bond forms when atoms give up their valence electrons, which then form an electron sea.
FIGURE 4.9 The path of an electron in a metallic structure.
Other materials are only partially covalent. Compounds, in general, are neither purely ionic nor purely covalent. Take, for example, sugar, which is composed of many units of the monomer C12H22O11. In sugar, the atoms are tightly held by covalent bonds. However, between the various C12H22O11 units, there are no covalent bonds and the interaction is weak. As a result, the crystals of sugar are easy to break. For a compound, the degree of either ionic or covalent bonding depends on the position of the elements in the periodic table. The greater the difference in electronegativity between the elements, the more ionic the bond, whereas the smaller the difference, the greater the degree of covalency. Another important type of bonding is metallic bonding. We define that term as the ease with which atoms of elements lose valence electrons; it provides a basis for classifying atoms into two general groups, namely metals and nonmetals. In general, an element that has one, two, or three valence electrons in to its outermost shell will tend to lose the electrons and thus is considered a metal. What, then, is particular about metallic bonding? In fact, it is the idea that a metal is an aggregate of positively charged cores surrounded by a “sea” of electrons (see Figure 4.8). In the metallic structure, the electrons actually hold the ions in place; otherwise they would attract each other. One can think of this cohesion as a mass of solid balls bonded by a very strong liquid glue. As a result of this metallic structure, the path of an electron in the metallic bond is completely random around the aggregate of ions (see Figure 4.9). Therefore, metals are of course good conductors because electrons can easily move in any direction. Second, metals usually have a high
The Internal Structure of Materials 95
degree of ductility because when the metal is bent, the electrons can easily rearrange their position, and thus bonds do not need to broken. We are now left to discuss another type of chemical bonding, called Van der Waals bonding or secondary bonding. These are weak bonds that are typically electrostatic attractions. They arise from atomic or molecular dipoles, which are polar molecules (see Figure 4.10). Typically, some portions of the molecule tend to be positively charged, whereas other portions are negatively charged. A good example is water (see Figure 4.10). To show the polarity of water, a good experiment is to rub a comb against a piece of wool. As the wool becomes electrically charged, it attracts a thin stream of water.
Crystal Structure In the last section we discussed the atomic structure and the various types of atomic bonding. We now examine the order in which atoms arrange themselves when they form a particular material. Argon, for example, is a gas, and thus it does not exhibit any atomic order. Water vapor is also a gas and hence behaves in a similar way to argon. However, water polar molecules can interact due to electrostatic forces. Therefore, when we compare the boiling temperatures of Ar (−185°C) and H2O (100°C), it is clear that there is some degree of interaction between the water molecules, leading to stronger bonds. Now if we decrease sufficiently the temperature of the water vapor, there is less kinetic energy, and water vapor will transform into the liquid state. In this case there is some ordering but only at short distances. If we decrease the temperature even further, liquid water will turn into ice, a crystal that exhibits a high degree of order in three dimensions. This long-range order represented by a repeated array of atoms in three dimensions is called a crystal. How do crystals form? In fact, it is really a statistical process. In general, nature is trying to come up with a structure that has the lowest possible energy configuration. But wait! How does an atom know how to recognize another atom? Actually, it uses a trial-anderror mechanism. What do we mean by this? Let’s assume that we are talking about a metal in the liquid state. In this case, each atom in the liquid jumps about 1013 times/sec. In other words, a metal in this form has been testing over millions of years, at a rate of 1013 times/sec; this type of atoms would turn the compound more energetically favorable. Let’s now look in more detail at a crystal. The first thing we should know about a crystal is that it is composed of unit cells. A unit cell is a pattern that repeats itself in space (see Figure 4.11). Now
(a) Polymer molecules
Van der Waals bonding
(b) Water molecules
FIGURE 4.10 A Van der Waals bond is formed due to polarization of molecules or groups of atoms. In water, electrons in the oxygen tend to concentrate away from the hydrogen. The resulting charge difference permits the molecule to be weakly bonded to other molecules.
FIGURE 4.11 Concept of a unit cell. In this example the unit cell is formed by four solid circles arranged in a square array, which is repeated in a 2-D space. In a 3-D space, the unit cell could be for example a cube.
96 CHAPTER 4
Material Classes, Structure, and Properties
Basecentered or thorhombric
Facecentered or thorhombric
FIGURE 4.12 The 14 Bravais lattices.
FIGURE 4.13 (a) Face-centered cubic unit cell, (b) body-centered cubic unit cell and (c) hexagonal closed packed unit cell.
that we know what a unit cell is, we can introduce another idea: the notion of a crystal lattice. This is the structure that arises from the repetition of a particular pattern or unit cell in a 3-D space. In nature, there are 14 possible unit cells, also called the Bravais lattices (see Figure 4.12). These 14 types of unit cells are grouped into seven possible crystal systems: cubic, tetragonal, orthorhombic, hexagonal, rhombohedral, monoclinic, and triclinic. The simplest crystal structures typically belong to pure metals. The most common are the face-centered cubic (FCC), the body-centered cubic (BCC), and the hexagonal closed packed (HCP) crystal structures (see Figure 4.13). The FCC structure is composed of atoms located at each corner and at the center of each face. Some examples of elements that have this structure are the metals copper, silver, gold, nickel, and aluminum. The BCC unit cell has a configuration in which the atoms are located at each corner of the cube, with one atom at the center of the cube. Some examples of this crystal structure are iron, tungsten, and chromium. The HCP crystal structure has a configuration in which atoms are located in the corners of a
The Internal Structure of Materials 97
One important aspect to point out is that some elements can assume more than one crystal structure. It all depends on certain thermodynamic conditions, such as temperature, pressure, stress, magnetic field, and electric field. These changes in crystal structure in a pure element are called allotropic transformations. A good example of this behavior is iron (Fe), an element that undergoes several changes in crystal structure. Iron is BCC at room temperature and atmospheric pressure, but it will change to an FCC crystal structure at around 750°C (see Figure 4.14). On the other hand, if we maintain the ambient temperature and increase the pressure to high levels (125 kbar), the BCC structure will transform to an HCP structure (Figure 4.14). However, ceramic structures are considerably more complex. Most ceramic materials are compounds formed by metallic and nonmetallic elements. In addition, due to the fact that ceramics are predominantly ionic, they are usually described in terms of ions instead of atoms. Metallic ions are called cations (ions depleted in electrons), whereas nonmetallic ions are called anions (enriched in electrons). How can these ions affect the crystal structure? The answer is, by the magnitude of their electrical charge as well as the relative size of cations and anions. Regarding the first effect, the crystal will try as much as possible to be electrically neutral. With respect to the second effect, because cations are in general smaller than anions, the size ratio between the cations and anions will dictate the number of nearest neighbors surrounding each cation. The most common ceramic structures are the rock salt structure, the cesium chloride structure, and the zinc blend structure. The rock salt structure derives it name from common table salt, which exhibits this type of crystal structure (see Figure 4.15). The structure is formed by two interpenetrating FCC lattices—one composed of cations, the other composed of anions. Other examples of ceramic materials with the rock salt structure include MgO, MnS, LiF, and FeO. The cesium chloride structure is a combination of two simple cubic structures, one formed by cations, the other formed by anions (Figure 4.15). The zinc blend structure is a combination of two FCC structures. Some examples of ceramics with zinc blend structures are ZnS, ZnTe, and SiC (a medium used in grinding paper). These three ceramic crystal structures have in common the fact that to fulfill the conditions of neutrality, there is one cation and one anion per unit cell.
1600 Temperature (˚C)
hexagon, one atom in the center of the basal plane of the hexagon, and three atoms in the center of the cell, off-centered from the caxis. Some examples of elements with this structure are the metals zinc, cobalt, and titanium.
δ - iron 1200 γ - iron 800 400
α - iron 25
ε - iron 75 100 125 150 175
FIGURE 4.14 Pressure-temperature phase diagram for iron.
98 CHAPTER 4
Material Classes, Structure, and Properties
Zinc Cesium Sodium Chlorine (a)
FIGURE 4.15 (a) Rock salt structure for NaCl, (b) cesium chloride structure, and (c) a zinc blend.
However, there are other types of ceramic structure for which the charges of cations and anions are not the same. An example is the calcium fluorite structure (CaF2; see Figure 4.16). The unit cell is composed of eight cubes, for which the anions occupy the corner sites and the cations the center of the cubes. To achieve neutrality, there are half as many Ca2+ ions as F− ions. As a result, only half the cubes exhibit the presence of a cation.
FIGURE 4.16 Calcium Fluorite structure (CaF2). H
FIGURE 4.17 Mer unit of ethylene.
Normally, when we talk about metals or ceramics, we consider atoms or ions as single entities. However, in the case of polymers the situation is quite different; we normally think of molecules as the single entity. Polymer molecules consist of a repetition of a single unit called a mer, a term that derives from the Greek word meros, which means part. Therefore, poly + mer means many parts. The simplest type of polymer is called polyethylene, and the mer is ethylene. The ethylene molecule has the structure shown in Figure 4.17. The molecule is composed of carbon and hydrogen. As we have discussed, carbon has four valence electrons that can participate in bonding, whereas hydrogen has only one. Thus in the ethylene molecule, each carbon forms a single bond with each hydrogen atom (each atom is sharing one electron), whereas the two carbon atoms form a double bond between themselves (each atom is sharing two electrons). Now let’s imagine that we replace all hydrogen atoms with fluorine atoms. What will happen? The resulting polymer will be called polytetrafluroethylene (PTFE), or Teflon (see Figure 4.18). What about if we replace one hydrogen with one Cl atom? Then we obtain the polymer polyvinylchloride (PVC). What about doing the same thing but exchanging the hydrogen atom with a CH3 methyl group? Then we obtain the polymer polypropylene (PP). We can further
The Internal Structure of Materials 99
characterize the types of polymers by observing the repeating unit. Hence, when all the repeating units along a chain are of the same type, the resulting polymer is called a homopolymer. However, if chains are composed of two or more different units, the polymer is called a copolymer. In addition, if the different units are arranged in blocks, the polymer is called a block copolymer (see Figure 4.19). The molecular structure of polymers can be further categorized as linear polymers, branched polymers, cross-linked polymers, and network polymers. In the case of linear polymers, the mer units are joined together end to end in single chains. The molecules will be spaghetti-like and characterized by many Van der Waals bonds between the chains (see Figure 4.20). Some examples are the polymers polyethylene, polystyrene, and nylon. In the case of branched polymers, the main chains are connected through branches. As a result, the density of the polymer is lowered (Figure 4.20). In crosslinked polymers, adjacent linear chains are joined one to another at various positions by covalent bonds. This process is called crosslinking and is accomplished by including additives that form the covalent bonds (Figure 4.20). Examples of this type of polymer are rubber elastic materials. Finally, network polymers form when mer units can bond in three dimensions (Figure 4.20). An example of this type of polymer is epoxy.
Polyvinyl chloride (PVC)
FIGURE 4.18 Mer structures of the more common polymeric materials.
Defects In the previous chapters we have always assumed a pure material or a compound with no defects in it. Thus the structures we have talked about were in “some way” ideal situations. However, in fact, 100% pure materials and with no defects do not exist, although some materials can have small amounts of impurities and/or defects. The origin of these defects is very diverse, ranging from atomic packing problems during processing to the formation of interfaces with poor atomic registry or the generation of defects during deformation. On the basis of our discussion so far, you are probably thinking that the presence of defects is deleterious to materials. In some cases that’s true, but in many cases defects are extremely beneficial. Some examples include: ■
The presence of small amounts of carbon in iron (known as steel) makes possible the achievement of high strengths. The addition of 0.01% of arsenic can increase the conductivity of Si by 10,000 times. Some defects called dislocations are responsible for plastic deformation in materials.
FIGURE 4.19 Schematic representations of (a) random, (b) alternating, (c) block, and (d) graft copolymers.
100 CHAPTER 4
Material Classes, Structure, and Properties
FIGURE 4.20 Schematic representation of (a) linear, (b) branched, (c) cross-linked, and (d) network polymer molecular structures.
In general, we can classify the defects as point defects, linear defects, planar defects (interfacial defects), or volume defects (bulk defects), for which the scale of each class is shown in Figure 4.21. Let’s examine each class of defect in more detail. The simplest point defect is called a vacancy, which is a lattice point from which an atom is missing (see Figure 4.22). Vacancies are introduced into a material during solidification or heat treatments or by radiation of atomic particles. In fact, in a nuclear power plant, where radiation is continuously being produced, the monitoring of the formation of vacancies is crucial for the safety of the plant. The presence of vacancies in a crystal is a necessity because the presence of vacancies will increase the entropy (randomness) of the crystal. In addition, the presence of a vacancy changes the stress field of the crystal. As shown in Figure 4.22, the vacancy induces a tensile stress field around the neighboring atoms. In addition, the equilibrium number of vacancies increases exponentially with temperature. Typically, at room temperature, there is one vacancy per 1 million atoms, whereas at the melting temperature, there are 1000 vacancies per million atoms. A self-interstitial point defect can also form in materials. This occurs when an atom from the lattice goes into an interstitial position, a small space that is not usually occupied by any atom (see Figure 4.23). The self-interstitial atom creates large distortions in the lattice because the initial available space is smaller than the atom dimensions. In ionic structures, such as ceramic materials, because of neutrality, there are two types of point defects: (1) the Schottky defect, which is a pair of defects formed by a vacancy of one cation and a vacancy of one anion (see Figure 4.24), and (2) the Frenkel defect, which is formed by a vacancy of one cation and a self-interstitial cation (Figure 4.24) or a vacancy of one anion and a self-interstitial anion. So far we have only discussed defects in pure solids or compounds. However, as mentioned before, impurities must exist. Even if the metal is almost (99.9999%) pure, there are still 1023 impurities in 1 m3. Therefore the following question arises: Where do the impurities go? That all depends on the impurity and the host material. The final result will be a consequence of (1) the kind of impurity, (2) the impurity concentration, and (3) the temperature and pressure. However, in general, impurities can go to a substitutional site, that is, a site occupied by the host atom. In this case they will be called substitutional atoms. Or impurities can go to an interstitial site
The Internal Structure of Materials 101
and will be called interstitial atoms (different from self-interstitials). Whether the impurities go to a substitutional or interstitial site will depend on (1) atomic size, (2) crystal structure, (3) electronegativity, and (4) valence electrons. With respect to atomic size, interstitial atoms are small compared with host atoms. In covalent bonded materials, substitutional atoms can create a unique imperfection in the electronic structure if the impurity atom is from a group in the periodic table other than that of the host atoms. An example is the addition of As or P (Group V) in Si (Group IV; see Figure 4.25). Only four of five valence electrons of these impurities can participate in the bonding, because there are only four possible bonds with neighboring atoms. The extra nonbonding electron is loosely bound to the region around the impurity atom in a weak electrostatic interaction. Thus the binding energy of this electron is relatively small, in which case it becomes a free or conducting electron. In polymers, the addition of impurities can also have significant consequences. For example, natural rubber becomes cross-linked when small amounts of sulfur (5%) are added. As a result, the mechanical properties change dramatically. Natural rubber has a tensile strength of 300 psi, whereas vulcanized rubber (sulfur addition) has a tensile strength of 3000 psi. Now let’s discuss another class of defects called linear defects. These defects, also called dislocations, are the main mechanism in operation when a material is deformed plastically. Currently, several techniques are available for the direct observation of dislocations. The transmission electron microscope (TEM) is probably the most utilized in this respect. Let’s look at the simplest case, the edge dislocation. Imagine the following sequence of events: (1) take a perfect crystal, (2) make a cut in the crystal, (3) open the cut, and (4) insert an extra plane of atoms (see Figure 4.26). The end result is an edge dislocation. These dislocations are typically generated during processing or in service, if subjected to enough stress. The presence and motion of dislocations dictate whether materials are ductile or brittle. Because metals can easily generate and move dislocations, they are ductile. On the other hand, ceramic materials have a high difficulty in nucleating and moving dislocations due to the covalent/ionic character of the bonds, and they are therefore brittle. One of the important parameters related to dislocations is the knowledge of the amount of dislocation length per unit volume. This is called the dislocation density and is given by
Centimeters 10 10 10 10 10 Atomic point defects
Electronic point defects
Interfacial defects Line defects
FIGURE 4.21 Range of scales for the various classes of defects.
FIGURE 4.22 A vacancy defect.
FIGURE 4.23 A self-interstitial defect.
102 CHAPTER 4
Material Classes, Structure, and Properties
where LD is the total length of dislocations and V is the volume. Another class of defects is that of interfacial defects. Among these, we’ll first discuss the free surfaces. All solid materials have finite sizes. As a result, the atomic arrangement at the surface is different from within the bulk. Typically, surface atoms form the same crystal structure as in the bulk, but the unit cells have slightly larger lattice parameters. In addition, surface atoms have more freedom to move and thus have higher entropy. We can now understand that different crystal surfaces should have different energies, depending on the number of broken bonds.
FIGURE 4.24 A Schottky defect and a Frenkel defect.
Silicon (4+) Phosphorous (5+)
FIGURE 4.25 Addition of phosphorous, having five valence electrons, to silicon leads to an increase in electrical conductivity due to an extra bonding electron.
The second type of interfacial defect is the grain boundary. This boundary separates regions of different crystallographic orientation. The simplest form of a grain boundary is called a tilt boundary because the misorientation is in the form of a simple tilt about an axis (see Figure 4.27). We know that grain boundaries have also an interfacial energy due to the disruption of atomic periodicity. However, will they have higher or lower energies than free surfaces? The answer is lower energies. This is because grain boundaries exhibit some distortion in the type of bonds they form, but there are no absent bonds. Most of the materials utilized in our daily lives are polycrystalline materials. This means that the materials are composed of many crystals with different orientations, separated by grain boundaries (see Figure 4.28). It turns out that this network of grains significantly affects several of the material properties. The last type of interfacial defect is the interphase boundary. These are the boundaries that separate regions of materials with different structure and/or composition. An example is a dentist’s drill, which is a mixture of small crystals of tungsten carbide surrounded by a matrix of cobalt. The interfaces between the tungsten carbide and the cobalt matrix are interphase boundaries. Finally, we are left to discuss bulk defects. Most of the time these volume defects are introduced during the production of materials. In some cases, impurities in a material combine with each other and form inclusions. These are second-phase particles that can considerably affect the mechanical properties of materials. One other type of defect is the casting defect. These can be cavities and gas holes produced under certain conditions of temperature
Mechanical Behavior 103
and pressure. A different type of volume defect is the cracks formed during heating and cooling cycles or during formability processes. Finally, welding defects can be formed during welding procedures due to the fact that the heat generated during welding is not uniform. As a consequence, a region affected by the heat is produced, where the properties change gradually away from the heat source.
Edge dislocation line
Stress, Strain, Stiffness, and Strength Stress is something that is applied to a material by loading it. Strain—a change of shape—is the material’s response. It depends on the magnitude of the stress and the way it is applied—the mode of loading. Ties carry tension; often they are cables. Columns carry compression; tubes are more efficient as columns than are solid rods of similar areas because they don’t buckle as easily. Beams carry bending moments. Shafts carry torsion. Pressure vessels contain a pressure. Often they are shells: curved, thin-walled structures.
FIGURE 4.26 Sequence of events leading to the formation of an edge dislocation.
Stiffness is the resistance to change of shape that is elastic, meaning that the material returns to its original shape when the stress is removed. Strength is its resistance to permanent distortion or total failure. Stress and strain are not material properties; they describe a stimulus and a response. Stiffness (measured by the elastic modulus E, defined in a moment) and strength (measured by the yield strength σy or tensile strength σts) are material properties. Stiffness and strength are central to mechanical design. The elastic moduli reflect the stiffness of the bonds that hold atoms together. There is not much you can do to change any of this, so the moduli of pure materials cannot be manipulated at all. If you want to control them you must either mix materials together, making composites, or disperse space within them, making foams.
Axis of tilt
Modes of loading Most engineering components carry loads. Their elastic response depends on the way the loads are applied. Usually one mode dominates, and the component can be idealized as one of the simply loaded cases in Figure 4.29: tie, column, beam, shaft, or shell. Ties carry simple axial tension, shown in (a) in the figure; columns do the same in simple compression, as in (b). Bending of a beam (c) creates simple axial tension in elements above the neutral axis (the center line, for a beam with a symmetric cross-section) and simple
FIGURE 4.27 Tilt boundary.
104 CHAPTER 4
Material Classes, Structure, and Properties
compression in those below. Shafts carry twisting or torsion (d), which generates shear rather than axial load. Pressure difference applied to a shell, such as the cylindrical tube shown at (e), generates biaxial tension or compression.
Stress Consider a force F applied as normal to the face of an element of material, as in Figure 4.30 on the left of row (a) in the figure. The force is transmitted through the element and balanced by an equal but opposite force on the other side so that it is in equilibrium (it does not move). Every plane normal to F carries the force. If the area of such a plane is A, the tensile stress σ in the element (neglecting its self-weight) is FIGURE 4.28 Transmission electron microscopy image of polycrystalline copper. These grains are separated by grain boundaries. (Courtesy of R. Calinas, University of Coimbra; M. Vieira, University of Coimbra and P.J. Ferreira, University of Texas at Austin.)
If the sign of F is reversed, the stress is compressive and given a negative sign. Forces are measured in Newtons (N), so stress has the dimensions of N/m2. But a stress of 1 N/m2 is tiny—atmospheric pressure is 105 N/m2—so the usual unit is MN/m2 (106 N/m2), called megapascals, symbol MPa. If, instead, the force lies parallel to the face of the element, three other forces are needed to maintain equilibrium (Figure 4.30b). They create a state of shear in the element. The shaded plane, for instance, carries the shear stress τ of
The units, as before, are MPa. One further state of multiaxial stress is useful in defining the elastic response of materials: that produced by applying equal tensile or compressive forces to all six faces of a cubic element, as in Figure 4.30c. Any plane in the cube now carries the same state of stress; it is equal to the force on a cube face divided by its area. The state of stress is one of hydrostatic pressure, symbol p, again with the units of MPa. There is an unfortunate convention here. Pressures are positive when they push—the reverse of the convention for simple tension and compression. Engineering components can have complex shapes and can be loaded in many ways, creating complex distributions of stress. But no matter how complex, the stresses in any small element within the
Mechanical Behavior 105
component can always be described by a combination of tension, compression, and shear.
Strain Strain is the response of materials to stress (second column of Figure 4.30). A tensile stress σ applied to an element causes the element to stretch. If the element in Figure 4.30a, originally of side Lo, stretches by δL = L − Lo, the nominal tensile strain is
A compressive stress shortens the element; the nominal compressive strain (negative) is defined in the same way. Since strain is the ratio of two lengths, it is dimensionless.
tan (γ ) =
w ≈γ Lo
In practice tanγ ≈ γ because strains are almost always small. Finally, a hydrostatic pressure p causes an element of volume V to change in volume by δV. The volumetric strain, or dilatation (Figure 4.30c), is ∆=
A shear stress causes a shear strain γ (Figure 4.30b). If the element shears by a distance w, the shear strain
Stress-strain curves and moduli Figures 4.31, 4.32, and 4.33 show typical tensile stress-strain curves for a metal, a polymer, and a ceramic, respectively; that for the polymer is shown at four different temperatures relative to its glass temperature, Tg. The initial part, up to the elastic limit σel, is approximately linear (Hooke’s law), and it is elastic, meaning that the strain is recoverable; the material returns to its original shape when the stress is removed. Stresses above the elastic limit cause permanent deformation (ductile behavior) or brittle fracture. Within the linear elastic regime, strain is proportional to stress (Figure 4.30, third column). The tensile strain is proportional to the tensile stress:
σ = Eε
FIGURE 4.29 Modes of loading and states of stress: (a) tie, (b) column, (c) beam, (d) shaft, and (e) shell.
106 CHAPTER 4
Material Classes, Structure, and Properties
Tensile stress σ = F/A usual units MPa
Tensile strain ε = (L - Lo)/Lo
E = Young's modulus
Shear stress τ = Fs/A usual units MPa
τ=Gγ G = Shear modulus
Shear strain γ = w/Lo Volume Vo
Volume V p
p p p
FIGURE 4.30 The definitions of stress, strain, and elastic moduli.
Pressure p usual units MPa
Volume strain (dilatation) ∆= (V - Vo)/Vo
p=K∆ K = Bulk modulus
Stress σ = F/Ao
Tensile strength σts
and the same is true in compression. The constant of proportionality, E, is called Young’s modulus. Similarly, the shear strain γ is proportional to the shear stress τ
τ = Gγ 0.2% proof stress σy
and the dilatation ∆ is proportional to the pressure p:
Slope E Elongation εf Strain ε = δL/L
FIGURE 4.31 Stress-strain curve for a metal.
p = K∆
where G is the shear modulus and K the bulk modulus, as illustrated in the third column of Figure 4.30. All three of these moduli have the same dimensions as stress, that of force per unit area (N/m2 or Pa). As with stress it is convenient to use a larger unit, this time an even bigger one, that of 109 N/m2, giga pascals, or GPa.
Mechanical Behavior 107
Strength and ductility
Ductility is a measure of how much plastic strain a material can tolerate. It is measured in standard tensile tests by the elongation εf (the tensile strain at break) expressed as a percent (Figures 4.31 and 4.32). Strictly speaking, εf is not a material property, because it depends on the sample dimensions—the values that are listed in handbooks and in the CES software are for a standard test geometry—but it remains useful as an indicator of a material’s ability to be deformed. Ceramics do not deform plastically in the way that metals and polymers do. It is still possible to speak of a strength or elastic limit, σel (Figure 4.33). Its value is larger in compression than in tension by a factor of about 12.
Stress s = F/Ao
Limited plasticity: T = 0.8 Tg Ao
Cold drawing: T = Tg
L Viscous flow: T >> Tg 1% Elongation εf Strain Strain e = dL/L
FIGURE 4.32 Stress-strain curve for a polymer.
Compressive strength σel Compression Stress σ = F/Ao
For polymers, σy is identified as the stress at which the stress-strain curve becomes markedly nonlinear—typically, a strain of 1% (see Figure 4.32). The behavior beyond yield depends on the temperature relative to the glass temperature Tg. Well below Tg, most polymers are brittle. As Tg is approached, plasticity becomes possible until, at about Tg, thermoplastics exhibit cold drawing: large plastic extension at almost constant stress during which the molecules are pulled into alignment with the direction of straining, followed by hardening and fracture when alignment is complete. At still higher temperatures, thermoplastics become viscous and can be molded; thermosets become rubbery and finally decompose.
X Brittle: T 10 GPa and relative cost 40,000
p to 150 kW
Transportation, PC, laptops
Distributed generation, marine
membranes are quite thick, to prevent fuel crossover. However, for applications in transportation, thinner membranes with higher power density are preferred. In addition, typical membranes for PEMFCs require hydration, which limits the operating temperature of the fuel cell to around 80°C. To address the problem of cost associated with the use of platinum (Pt) nanoparticles, less expensive platinum alloy nanoparticles have been investigated, in particular binary alloys, such as Pt3Ni and Pt3Co. Theoretical calculations as well as experimental results seem to show much higher catalyst activities for Pt-alloy nanoparticles than pure platinum (Pt) nanoparticles (see Figure 9.58). However, the mechanism behind this enhanced activity is still controversial. Several hypotheses describing this behavior have been suggested: (1) a Pt skin develops during heat treatment, (2) a Pt skeleton is produced during an acid-leaching treatment, (3) a Pt-X (X denotes another metal) skin sputters onto the metal M, and (4) Pt-M solid solutions form (see Figure 9.59). With respect to particle agglomeration, one problem seems to be the mobility of Pt nanoparticles along the carbon support, the dissociation of Pt, and the leakage of hydrogen fuel through the membrane. Finally, to increase the operating temperature of PEMFCs, nanocomposite membranes capable of retaining the water content at
(Annealed) skeleton (Sputtered) skeleton
Specific activity* (mA/cm 2)
Table 9.1 Comparison Between Polymer Membrane Fuel Cells (PEMFCs) and Solid Oxide Fuel Cells (SOFCs) (Adapted from R. Lashway, MRS Bulletin, Vol. 30, No.8, August 2005)
FIGURE 9.58 Platinum (Pt)-alloy nanoparticles show greater catalytic activity than pristine Pt nanoparticles. (Stamenkovic, et al., JACS 128 (2006), 88138819.)
FIGURE 9.59 Mechanisms proposed to explain the enhanced activity in Pt-alloy nanoparticles. (Courtesy of Y. Shao-Horn, MIT.)
384 CHAPTER 9
Design Environments and Systems
Electron flow Hydrogen
Cathode Electrolyte Oxygen ions
FIGURE 9.60 Operation of a solid-oxide fuel cell. (Courtesy of Earnest Garrison, Illinois Institute of Technology.)
high temperatures are being developed. PEMFCs are very good candidates for transportation, personal electronics, and relatively small stationary and portable power generation. For large-scale stationary applications, SOFCs are preferred (see Figure 9.60). This is because SOFCs operate at high temperatures (800–1000°C) and thus are difficult to use in intermittent applications where on-off cycles are frequent. SOFCs are typically composed of a solid-oxide membrane electrolyte, an anode, and a cathode. The most common materials used for the solid-oxide membrane are ceramic-based materials, such as zirconia doped with yttria and scandia. The type and concentration of dopant determine the operating temperature and the ionic conductivity of the membrane. In SOFCs, the mobile species are O2- ions, which travel from the cathode to the anode, to react with H+ ions to produce water (see Figure 9.60). Conventional SOFCs use a La1-xSrxMnO3 metallic perovskite as the cathode and a porous Ni/YSZ cermet as the anode. SOFCs bring some advantages compared to other fuel cells, such as the use of inexpensive metal oxides or composites of metal oxides and metals, as cathode and anode catalysts, instead of Pt, which is expensive and scarce. Higher temperatures also permit, in principle, the direct use of hydrocarbon fuels. However, conventional SOFCs operating at temperatures around 1000oC suffer from various limitations, namely a restricted selection of materials that can be used as cathode and anode, interfacial reactions between the various layers, and a mismatch in thermal expansion between the electrolyte and the electrodes, with consequences for the mechanical properties. These challenges can be minimized while still maintaining the use of hydrocarbon fuels by operating at temperatures around 500–800oC. However, at these temperatures, novel electrolytes with high oxygen ionic conductivities and efficient catalysts for oxygen reduction and hydrogen oxidations are required. As a result, alternative materials such as La1-xSrxCoO3 and La1-xSrxFeO3 for the cathode, Sr2Mn1-xMgxMoO6-δ and rare-earth doped ceria (SmxCe1-xO2-δ) for the anode and Ce1-xMxO2-δ (M = Gd, Sm and Ca) for the electrolyte have shown, so far, promising results. In summary, fuel cells offer significant advantages as an alternative energy technology, particularly high efficiency, quieter power generation, and clean exhaust products. Explorations are under way for the storage of energy-rich gases via the use of nanoporous metal organic frameworks, or MOFs. These are
Enabling Environments and Systems: Energy 385
highly porous organic matrix substances that can store hydrogen and other gases (see Figure 11.3 in Chapter 11). Batteries, as fuel cells, are also electrochemical power sources. However, in contrast to fuel cells, which produce electricity continuously as long as a fuel and an oxidant are delivered, batteries convert chemical energy into electrical energy by electrochemical reactions occurring between the already existing constituents. A battery is composed of one or more electrochemical cells, which can be connected in parallel or series to deliver power. A typical electrochemical cell consists of three main elements (see Figure 9.61): an anode, which generates electrons to an external circuit and is oxidized during discharge; a cathode, which collects the electrons from the external circuit and is reduced during discharge; and an electrolyte, which allows the transport of ions between the anode and the cathode but not the transport of electrons. The electrolyte is typically a liquid solution in which a salt is dissolved in a solvent. In addition to these three main components, an electrochemical cell also contains current collectors to allow the flow of electrons to and from the electrodes. These materials are normally metals but should not react with the electrodes. There are two types of batteries, primary and secondary, based on their ability to recharge. In the former the chemical reactions are irreversible, whereas in the latter the electrode material exhibits reversible chemical reactions. Since they are not rechargeable, primary batteries are normally used for applications that demand long shelf life and minimum replacement. On the other hand, secondary or rechargeable batteries are usually used in applications that require transient amounts of high energy. Currently, rechargeable batteries are the most common method of storing electrical energy, particularly because they are very efficient (90% energy conversion) and relatively inexpensive. The first rechargeable batteries were lead-acid, eventually evolving to nickel-cadmium and nickel-metal hydride (Ni-MH), and more recently to lithium-ion batteries (see Table 9.2). The Ni-MH batteries were widely used for portable electronic devices, but due to the implementation of Li-ion batteries with high energy density and design flexibility, they have been almost out of circulation for this type of application. Ni-MH batteries are still used in hybrid vehicles, although in the near future Li-ion batteries are also likely to dominate this market. The development of Li-ion batteries started in the early 1970s, driven by the fact that lithium is both the lightest metal and highly
Electron flow Load Electrolyte
FIGURE 9.61 Basic components of an electrochemical cell. (Encyclopedia Britannica.)
386 CHAPTER 9
Design Environments and Systems
Table 9.2 Performance of Secondary Battery Systems (Adapted from MRS Bulletin, August 2002)
Layered cathode insertion
Layered anode insertion
FIGURE 9.62 Operation of a Li-ion battery during discharge.
Organic solvent + Li salt
Cell voltage (V)
Energy density (Wh/Kg)
electropositive. In batteries, Li is usually present at the anode as a compound material, typically LiC6. During discharge, lithium acts as electron donor to the external circuit, whereas the positive Li ions are transported through the electrolyte (Figure 9.62). At the cathode, the lithium ions react with the incoming electrons from the circuit and the cathode material, such as LiCoO2. Since the battery is rechargeable, the reversible reaction must be possible. To facilitate the insertion and extraction of lithium ions from the cathode and anode, respectively, both the LiCoO2 and the LiC6 compounds have layered structures (Figure 9.63). Despite the success achieved so far with the development of Liion batteries, there are still several factors that limit the performance of these devices, in particular material problems with the anode, cathode, electrolyte, and separator. Carbon-lithium anodes have low energy densities (a factor of 10 lower) compared to pure lithium anodes. However, pure lithium anodes have been shown to cause cell short-circuiting. Further experiments with lithium compounds, such as Li4.4Sn and Li4Si, resulted in high specific capacities, but the materials suffer from very large volume expansion-contraction (up to 300%) during the charge-discharge process, leading to cracking of the anode. More recently, nanoscale materials have been proposed for the anode—in particular, Si nanowires and an amorphous nanostructured tin-cobalt-carbon material. These materials provide large surface areas and reduced volume expansion-contraction, but many other nanoscale-related
Enabling Environments and Systems: Energy 387
properties are still unknown. In addition, these materials are still very expensive. Aside from the anode, the cathode is a key factor in developing high-performance lithium-ion batteries. Typically, the cathode contains a transition metal, which can be easily reduced and oxidized, must interact with lithium rapidly and without inducing a structural change, should be a good electronic conductor, and should be cheap and nontoxic. Finally, it must react with lithium and produce a high voltage. The most used cathode material is the layered LiCoO2. This compound is easy to process and has a long shelf life. However, it does not exceed a reversible capacity of 140 mAh/g (half the theoretical capacity) and contains toxic and expensive cobalt. The layered LiNiO2 is less expensive and less toxic than LiCoO2, showing also higher capacity, but it is difficult to synthesize, may release oxygen at high temperature, and is likely to exhibit a drastic fade in capacity during cycling. More recently, LiFePO4 has been suggested as a cathode material for Li-ion batteries. Because Fe is also a transition metal, is more available than Co and Ni, and is less toxic, this compound seems to be a good choice. In addition, it has a good capacity of 170 mAh/g at a cell voltage of 3.4 V, while the phosphate group is very stable. However, this material has a quite low electronic conductivity at room temperature and poor lithium conductivity. As a result, this material is now being studied in great detail, particularly because it is being thought of for use in electric vehicles. In this regard, reducing the size of LiFePO4 particles to the nanoscale and coating them with carbon seem to be very effective in improving the electronic and ionic conductivities. Another route that has been thought to improve the energy and power of Li-ion batteries is to use layered Li2MnO3 and LiMO2 (M = Co, Cr, Ni, Mn). These materials exhibit high capacities of around 250 mAh/g, although they are still in the early stages of development. Finally, some words about the electrolyte. For lithium-ion batteries, a good electrolyte must exhibit high ionic conductivity, good electrochemical and thermal stability and low reactivity with the other elements of the battery and be cheap and environmentally friendly. Typically, the electrolytes used so far tend to be liquid solutions. However, recently there has been a great interest in replacing liquid electrolytes with gel polymer electrolytes, which are membranes formed by containing a liquid solution in a polymer matrix. Shifting away from the Li-ion system, there
Li+ Co O
FIGURE 9.63 Layered anode and cathode materials for Li-ion fuel cells. (Courtesy of Electronics-lab.)
388 CHAPTER 9
Design Environments and Systems
has been some work in developing batteries based on sodium. However, the low melting temperature of sodium has generated several practical concerns.
+ - + -+ + - ++- - + + -- + ++ + + - + -- + + + +-- + + - -++ + -- -+ + + -+ -- +- -+ + + -- - - + - + -- ++ + + + - + -+ + -
+ + + + + -
+ + + + + +
Electrolyte ions Electric double layer construction
FIGURE 9.64 Electrochemical capacitor.
Current collector Electrolyte Porous electrode Separator
Individual ultracapacitor cell
FIGURE 9.65 Double-layer electrochemical supercapacitors. (Courtesy of Maxwell Technologies, Wikipedia.)
Energy density (Wh/kg)
Fuel cells 100
1 hour 1 second
10 10 hours
1 0.03 second
Electrochemical capacitors are also a viable alternative technology for storing energy. However, unlike batteries that store energy by means of a chemical reaction, capacitors store energy as electrical charge on the surface of electrodes. This happens through electrostatic interactions that occur in the electrode and solution interface region by which electric charges of equal magnitude, but opposite sign, accumulate on each electrode (see Figure 9.64). Because the electrodes are not deteriorated by this process, capacitors exhibit good performance over long periods of time. In addition, capacitors are rapidly charged and discharged, making them attractive for applications requiring quick responses. On the other hand, because the energy-storing mechanism is basically a surface process, the energy capacity of typical electrochemical capacitors is very dependent on surface area. Normally, electrochemical capacitors are subdivided into supercapacitors and pseudocapacitors. Supercapacitors are based on a structure involving an electrical double layer separated by a very thin dielectric wall (see Figure 9.65). Each layer contains a highly porous electrode suspended within an electrolyte. An applied potential on the positive electrode attracts the negative ions in the electrolyte, whereas the potential on the negative electrode attracts the positive ions. A dielectric material between the two electrodes prevents the charges from crossing between the two electrodes. In general, supercapacitors enhance the storage density through the use of activated carbon. This material is composed of nanopores to increase the surface area, allowing a greater number of electrons to be stored in any given volume. Typically, supercapacitors exhibit storage capabilities of less than 10Wh/kg. In addition, because the double layer can withstand only a low voltage, higher voltages are normally achieved by connecting individual supercapacitors in series. Supercapacitors are often used as backups to avoid short power failures and as a supplementary power boost for highenergy demands. Supercapacitors are also ideal for applications that require rapid charging.
Power density (W/kg)
FIGURE 9.66 Comparison of energy density and power density for fuel cells, batteries, and supercapacitors. (Courtesy of Maxwell Technologies, Wikipedia.)
In summary, fuel cells exhibit high energy storage but limited power density. Batteries deliver somewhat less energy density, but the power output is improved. On the other hand, supercapacitors, also known as ultracapacitors, are high-power devices with low energy storage capability (see Figure 9.66).
Interactive, Smart, and Intelligent Systems and Environments 389
9.8 INTERACTIVE, SMART, AND INTELLIGENT SYSTEMS AND ENVIRONMENTS Responsive Environments The environments previously discussed in this chapter have all related to fundamental conditions of spatial or surrounding environments (mechanical, thermal, lighting, and so on). There are, however, many other, more behaviorally based ways designers use to characterize environments that are useful to briefly address here. They typically involve the environments already described but go beyond them and focus on interactive, smart, or intelligent behaviors. In the 1920s the well-known architect Le Corbusier described the house of the future as a “Machine for Living,” with its connotations of automation. Subsequently, the 1953 “All Electric House” enabled an occupant in a bedroom to turn on a kitchen coffeemaker at the right time in the morning. These general areas have since evolved into intense and popular areas of study in relation to what are now commonly described as interactive, smart, or intelligent environments. Typically these environments seek to improve our experiences in living and work environments in both buildings and vehicles by providing information, aiding in task performance, or more generally improving lifestyle quality. Many “smart environments” in recent years have consisted of spaces with multiple sensors that control lighting and thermal environments and provide ubiquitous communications. Simple commercial systems do many other things, such as informing homeowners whether the pet dog has strayed from the area of the house. Far more sophisticated approaches now seek to have automated systems for detecting and identifying specific human users within a space (e.g., via facial detection) and adjusting the living or work environment characteristics in response to the needs of that specific individual. Before looking at nano-based applications in this domain, we should lay some background. The three key descriptive phrases— interactive, smart, and intelligent environments—typically mean quite different things to different people. Do the phrases imply equivalent concepts? Can something be interactive without being smart? We already have thermostats for controlling temperature levels and other sensors for light levels. Is a sensor-equipped automated house that automatically shuts lights off or on, depending on whether a room is occupied, truly a smart or intelligent environment? Do common sensor-driven actuation and communication
390 CHAPTER 9
Design Environments and Systems
systems alone define “smart” or “intelligent” environments? There is a considerable degree of controversy over terminology here, even though common dictionary definitions suggest clear distinctions that largely hinge around the level of cognition involved. At one time in the past, a sensor-controlled lighting system would surely have been thought of as “smart,” but the definition bar has now been generally heightened, although involved groups cannot really agree on definitions that really capture the essence of smartness or intelligence. All generally agree on the importance of enabling sensor-based actuation and communication systems, but these may be directly responsive only and not involve any kind of cognitive action that one would somehow think necessary in something called an “intelligent” environment. These are not easy concepts to untangle, but it is clear that their very fuzziness has engendered a great deal of confusion in what has blossomed into an absolutely enormous area of study that draws from many diverse fields, including materials science, electromechanical engineering, computer science (including expert systems and artificial intelligence), product design, and architecture. Here we seek to only briefly summarize this field. We start by briefly summarizing aspects of interactive, smart, and intelligent environments, as the terms are commonly now used and understood (see Figure 9.67). Impacts of developments in nanomaterial and nanotechnology will then be examined.
Increasing cognition levels
FIGURE 9.67 Terms used to describe systems or environments that are designed to have responsive or cognitive behaviors.
Interactivity can assume many forms but is usually considered to involve some type of physical, sound, light, or other response to a directed action on the part of an occupant. Actual applications vary widely. Figure 9.68 shows an interesting and delightful interactive display called Tulipomania. The installation is in one of Torino’s shopping galleries. When visitors come close, the animations projected onto the sandblasted glass panels move gently, as though in a breeze. Other kinds of interactive display systems in buildings are becoming more and more common for many purposes: general information and way-finding, entertainment, information about products in the space, and so forth. A common application in a retail setting is for product point-of-sales information to be displayed as a user approaches the product. Proximity or other kinds of sensors are used. Aspirations can be higher as well. In the American Museum of Natural History in New York City, for example, an interactive display wall helped give visitors a sense of Einstein’s theories by responding to the motions of visitors moving relative to the wall. Via displays
Interactive, Smart, and Intelligent Systems and Environments 391
FIGURE 9.68 Tulipomania, an interactive installation in Torino, Italy. (Courtesy of Ivividia.)
that opened up or closed down, visitors were encouraged to feel gravity as a mass-warping time space. Many sensor-based systems of this type involve complex display and sound and audio systems. So-called smart systems have even more of a basis in complex sensorbased electronic and computational systems but frequently involve “smart materials” as well. Again, many different approaches are evolving here. Many of the materials that we have already described have an apparent ability to change one or more of their properties in response to changes in their surrounding thermal, radiant, electrical, mechanical, or chemical environments. Thermochromics, for example, change their apparent color as the temperature of their surrounding environment increases and there is an input of thermal energy into the material. Magnetorheological materials change their viscosity when subjected to varying levels of magnetic fields. As we will discuss in Section 10.2, these and other materials of this type are often called smart materials because they exhibit useful changes in properties in the presence of varying external stimuli. Examples of smart systems based on these kinds of materials abound. For example, there are many self-damping systems used for vibration control, including skis that have self-damping mechanisms for reducing the troublesome “chatter” that can be experienced by advanced skiers in difficult terrains. In the automotive industry, there are “smart tires” or “smart suspension systems” that enhance driving performance (see Section 12.2). In the aerospace industry
392 CHAPTER 9
Design Environments and Systems
there has been considerable attention directed toward the development of “smart skins” that incorporate a series of sensors and actuation devices based on smart materials, including shape memory alloys, to enhance wing performance. Nanomaterials and nanotechnologies offer great potential as both tiny sensors and actuators and thus have the potential to be integrated into surface structures quite easily. Section 10.2 addresses smart materials and systems in more detail. There are many types of intelligent systems and environments. Among the most popular are systems that first detect and identify specific human users within a space and then tailor aspects of the living or work environment in response to the needs or tasks of those specific individuals. More advanced systems use facial and gesture recognition systems that seek to enable users to control specific aspects of their living or work environments, without any kind of manual or even voice inputs. These systems invariably involve complex computational infrastructures as well as a host of different kinds of sensory and actuation devices. Characteristics of intelligent systems are examined in more detail in the following section.
Characterizing Interactive, Smart, and Intelligent Environments Figure 9.69 suggests how intelligent environments can be broadly characterized in terms of their functional descriptions, the way smart behaviors are embedded in the environment or the ways that they are controlled, and the general cognition levels associated with various behaviors. Following this diagram, we broadly use characterizations of smart or intelligent environments that reflect different primary streams of meaning and description. The first is in relation to definitions of systems and environments (use and surrounding). In addition to performance-specific systems that are constituents of larger products, vehicles, or buildings, this area encompasses human occupation and use needs and issues vis-à-vis lifestyle, health, and work. Included are physical comfort and health issues vis-à-vis the surrounding environment. Use issues focus on lifestyle considerations or task performances (e.g., what would an optimal environment for a stockbroker look like?). The level of component, subsystem, system, or environment to be considered is important here. Many simple components involve only single behaviors, such as a light that goes off or on, whereas other highly complex systems or environments involve multiple
Interactive, Smart, and Intelligent Systems and Environments 393
Systems and environments Types
Enabling systems and environments Air Thermal Lighting Sound Structural Electromechanical Other
Multiple Metaphor models
Increasing behaviors addressed
Embedment/ Control Strategy
Direct smart materials
Use/interpetation of information
Discrete component control
Guided responses Artificial intelligence
Use environments Living Entertainment Work Health Ergonomic Other
Reasoning/ evaluation Reflection
Increasing cognition levels
and often interactive behaviors that need to be considered. Specific performance or use goals need to be stipulated for each level considered. A second area is in relation to levels of assisted cognition within the computational world for various system or environment goals. At a low level in this category are the many attempts to provide information-rich environments that support systems or environments, including human physical and intellectual needs. At a higher level, expert systems have been devised to interpret information and provide guided responses. Artificial intelligence approaches seek to provide further cognitive capabilities and even perform reasoning. The third broad area deals with technological implementation strategies, materials, and devices. It is here that characteristics of sensors and sensor-driven actuators, materials with propertyvarying characteristics, and various logic control systems, including nanomaterials and nanotechnologies, come into play. Various kinds of technologies could be used to capture more sophisticated information about user states and context awareness via gesture or facial recognition systems.
Basic and enhanced constituitive models (systems + materials)
Metaphor models (biological)
Embedded system controls
Tangible and other interfaces
Increasingly transparent interfaces
FIGURE 9.69 Smart and intelligent environments can be broadly characterized in terms of their functional descriptions and numbers of behaviors, the general cognition levels imparted by the computational environment, and the embedded materials and technologies used for implementation.
394 CHAPTER 9
Design Environments and Systems
Consider a first example involving relatively simple cognition levels. Biosensors could be placed within an environment to detect biohazards that might result from a terrorist action. Within an integrated electronic system, information from the sensors could be analyzed and interpreted in relation to human tolerance levels, and various alerts or warnings would be communicated, even direct mitigation systems called into action. In terms of Figure 9.69, this scenario would be illustrative of “single-behavior” sensory detection, coupled with a very simple expert system (a basic “if-then” formulation) and implemented through a direct mechatronic model (discrete component and system control). A more complex example is an “intelligent room” environment designed for individuals with special medical needs or who are recovering from an operation. These rooms might have a whole host of means for monitoring personal vital signs, event recovery measures, general mental and physical condition states (e.g., awareness, ability to function), indicators of whether medicines have been taken regularly, whether the patient has had visits, whether the patient has moved around and how (mobility assessments), and a whole host of information concerning surrounding physical and environmental states, such as temperature levels. Facial characterization and gesture recognition systems might be needed for further assessments or as a way for nonverbal patients to communicate. The initial sensing goal in the above example is to detect and measure everything needed for an externally located medical group to access a patient’s state and progress. If fully automated, expert or artificial intelligence systems would analyze and interpret information and, if necessary, cause specific actions to be evoked (e.g., at a low level this might be a voice communication to a patient to “Take your 11:00 a.m. medicine,” or, at a higher level, could cause a medical team to be dispatched). In this scenario, not only are large numbers of sensors involved, but the interactions of multiple behaviors must be analyzed and specific actions evoked. This same room might make use of self-cleaning and antimicrobial surfaces (see Section 10.2). Though some basic ideas and aspirations are fairly straightforward, not all these kinds of interactions and responses can be achieved at the moment. Limitations exist throughout, including in sensory and computational components that are more the focus of this book than are related cognition algorithms, which remain extremely troublesome. As we move from specific applications, such as the medically oriented room we’ve described, and more into general intelligent environments, there is less than clarity on what we really
Interactive, Smart, and Intelligent Systems and Environments 395
want intelligent environments to ultimately do. This latter topic is fascinating but largely beyond the scope of this book. (See Further Reading for a more extensive list of sources on smart or intelligent environments.) Here we focus more on material/technology-related concerns and opportunities.
Nanomaterials and Nanotechnology Applications Developments in these areas can potentially be greatly enhanced by nano-based approaches. We have already seen several examples of applications, including self-damping systems used for vibration control in cable-supported bridges or buildings, that are based on magnetorheological fluids that can in turn be enhanced via nanoparticles with improved magnetic properties (Section 9.2) and transparency-changing windows (Section 9.5). Behaviors such as these are the basis for many larger approaches to smartness when they are coupled with sensor/control systems that activate them during appropriate conditions. Other approaches that need not include sensor/controls systems include self-healing surfaces or the self-cleaning or antimicrobial surfaces noted previously that are based on nanosized titanium dioxide particles. (These surfaces are discussed in Section 10.2.) Surfaces such as these would be an important component in any kind of smart or intelligent room directed toward health or medical applications or even for everyday cleanliness in kitchens, bathrooms, and other common spaces. Many interactive, smart, or intelligent environments already use a variety of sensory technologies; nonetheless, it remains surprising how few sensor, control, and actuation devices are actually used in most current applications. Difficulties in precisely locating a few sensors in relation to the measurand remain problematic. More are invariably needed to capture necessary information. Devices that are used are also often quite visibly intrusive due to their size and often appear as “add-ons” to wall, ceiling, or floor surfaces in a room—a fact known to cause occupant behaviors to change (who has not acted at least a bit differently when in front of a Webcam?). An immediate stated desire of designers of these kinds of environments is to have perfectly seamless integration of involved sensors and actuators with the surfaces of products in the space or within surfaces of the surrounding room. Even more speculative approaches that question the very surfaces themselves are discussed in the literature (see Further Reading).
396 CHAPTER 9
Design Environments and Systems
As discussed in Section 9.4, directions for many future nano-based electronic systems are characterized by improved performance, decreasing size, increased multifunctionality, and decreased costs. Many research efforts are explicitly directed toward making improved sensors for a variety of applications, and many are expected to find a ready application area in interactive, smart, and intelligent systems. Expected benefits include not only improved performances but also ever smaller and cheaper sensors. Nanoelectromechanical Systems (NEMS) are on the immediate horizon as well. These trends intersect very well with technological needs in interactive, smart, and intelligent systems. The idea of being able to have large numbers of inexpensive sensors distributed throughout a spatial environment that are designed to capture specific kinds of information (about users, processes, or conditions within a space) has great appeal with designers involved with conceptualizing not only smart buildings, but smart cities as well. A future can be imagined where distributed sensors (perhaps the “swarms” discussed in Section 9.4, but more likely multitudes of still tiny but more sophisticated inter-connected nanoscale sensors, actuators and other devices) aid in our every living and work activities within buildings and cities. It is here that trends toward smallness, high performance, and multifunctionality in enabling electronic systems intersect with goals of interactivity, smartness, and intelligence. At the moment, this area remains rather speculative, but the potential is clearly there.
The enormous potential for widespread nanomaterial applications to occur inherently depends on the availability of large quantities of nanomaterials at reasonable costs. In the current emerging state of the field, not all nanomaterial forms found in the laboratory are widely available, fewer still as commercialized products. Costs for nanomaterial products are also high. The importance of costs in any application or design context hardly needs explanation. Costs are invariably a driving factor, one often cited as an inhibiting factor in the development of applications involving nanomaterials—and not without good reason. In the early days of nanomaterial exploration, a gram of nanotubes could cost several thousand dollars; even recently, 500 or so dollars per gram was a common price. Even if the amounts used in applications were relatively small, say, 5% by weight in a nanocomposite, final product costs were so high as to prohibit all but the most specialized applications. Costs have since dropped dramatically but nonetheless remain a significant factor.
Nanomaterials Costs 397
In the current context, many groups that commercially produce nanomaterials (such as various kinds of nanoparticles or nanotubes) are just now transitioning from their roles as suppliers to the research sector to that of becoming producers of commodity products. This transition, in turn, is being driven by the development of more and more real applications that demand larger quantities, or by real product prospects just on the horizon (see Figure 9.70). The actual number of producers, however, is still relatively few in comparison to the multitude of businesses that produce conventional materials, and outputs remain relatively small. Several claim to be able to scale up to larger volumes quickly. Nonetheless, the industry remains in an emergent state. A sign that further transitions will occur is the increased number of major chemical and traditional material suppliers starting to produce nanomaterials. There is every expectation that increasing demand will in turn lead to increases in production volumes. In the following discussion, the range of currently available nanomaterials is briefly reviewed, as are their general characteristics. Various parameters that affect unit costs—particularly type, treatments, and quantities—are also identified.
Types Nanoparticles for applications are already commercially available in a wide range of forms that can support a host of applications. Fundamental types include basic elements, compounds, and oxides. Various alloys, carbides, sulfides, and other forms can also be obtained. Materials such as silver (Ag), gold (Au), aluminum (Al), and iron (Fe) are commonly available, as are many fundamental forms. A wide array of compounds (such as tungsten carbide, TiC) and oxides (such as titanium dioxide, TiO2) are also available. These materials are available in nanoparticle form and some in nanopowder form (a term sometimes used to describe nanoparticles less than 30 nm in diameter). Actual diameters can vary considerably. Common silver nanoparticles, for example, are readily available in diameters ranging from 10 nm all the way up to the micron size (2 um or 2000 nm). Some other materials are currently available only in smaller or larger sizes, depending on their makeup. Titanium dioxide (TiO2), widely used in its anatase form for photocatalytic applications (self-cleaning, antimicrobial), typically ranges from 5 to 20 nm, whereas in another of its forms (rutile) diameters are often larger (40–50 nm). Many polymeric nanocomposites are based on dispersed clay nanoparticles (often called nanofillers). Montmorillonite is often used.
FIGURE 9.70 The control room of the new Baytubes® production facility in Laufenburg, showing the top of the fluidized bed reactor. The facility has a capacity of 30 metric tons annually. Market potential estimates for carbon nanotubes (CNTs) in the coming years are several thousand metric tons per year. (Courtesy of Baytubes.)
398 CHAPTER 9
Design Environments and Systems
It is a layered smectite clay mineral that has a platelet structure. Platelets are very thin—for example, 1–2 nm—but have very large surface dimensions, perhaps over 500 nm, that make them highly effective providers of surface areas. These kinds of nanoparticles are relatively inexpensive compared to other types of nanoparticles and can be easily manufactured in bulk quantities. Section 8.8 describes nanocomposites based on smectite materials in greater detail. Nanoparticles can also come in varying levels of treatments. Various nanoparticles can be obtained that, for example, already have hydrophobic or hydrophilic properties (see Chapter 8) useful in a wide range of applications. Typically, when obtained from a manufacturer, nanoparticle batches may need to be further processed via application of surfactant coatings, ultrasonification, milling, or other processes because of their inherent tendency to agglomerate or attract moisture. Carbon nanotubes for applications are available in a wide variety of single-walled (SWNT) and multiwalled (MWNT) forms, including different lengths, diameters, and purities. A primary quality and cost issue is purity. Depending on the synthesis process used, purified forms are characterized by descriptions such as “95 wt%” or “60 wt%,” which simply refers to the actual percentage by weight of nanotube content within a unit weight of a gram of nanotube material. Other constituents might include ash, amorphous carbon, residual catalyst, or other materials. Some SWNT formulations can also include some percentage of MWNTs. Obviously, higher purity forms have more effective properties. Cost-per-gram values, however, are invariably higher than lower purity forms. Lower purity and lower-cost forms, however, can be suitable for many bulk applications. Most commercialization has been with MWNTs. SWNTs are available but often at higher unit prices. Typical diameters for available SWNTs are on the order of 1–2 nm, and common lengths are on the order of 10–50 um, although there is variation in these numbers as well. Special short nanotube forms are also available that are on the order of 0.3–5 um. Outer diameters of common MWNTs are on the order of 5–15 nm, with inside diameters on the order of 2–8 nm. Several walls are common. Short-form MWNTs often have larger outer diameters (20–50 nm or so) and somewhat larger inner diameters than longer forms. Incorporating carbon nanotubes into other matrix materials to form nanocomposites has often proven difficult because of the surface chemistry of the carbon. Problems include achieving uniform dispersions and poor adhesion with the primary matrix. Many highly
Nanomaterials Costs 399
Various kinds of surface treatments have been developed to reduce some of these problems. In particular, many nanotube products are now available in what are called “functionalized” form. Normally these functionalized carbon nanotubes processes involve chemically attaching different molecules or functional groups to the sides of nanotubes that allow various kinds of bonding. Processes vary depending on the need but can include using a variety of oxidation methods or polymeric wrappings. Functionalized nanotubes can develop better bonding in mechanically directed nanocomposites (via covalent rather than Van der Waals bonding). In other cases, noncovalent bonding is preferred. In the biological or chemical areas, nanotubes can be functionalized to be able to play diverse roles, including as biosensors. Attachment of certain kinds of molecular groups can allow protein adsorption or bindings, which in turn enables drug delivery or other application potentials. Functionalized nanotubes are invariably more expensive than normal types. Not unexpectedly, costs for functional nanotubes used in specialized biological or medical applications can be extremely high. Figure 9.71 illustrates some general pricing characteristics for carbon nanotubes. Unit costs for high-purity materials are greater than lower-purity materials. Functionalized or treated versions are more costly than basic types. Costs also vary with quantities. In the diagram, the steep curves to the left reflect costs for very small quantities similar to those used in a laboratory or development context. For any real application, quantities acquired would necessarily be quite large, and costs would correspondingly decrease. Figure 9.72 illustrates how basic unit cost ranges for common nanomaterial products broadly compare to other materials. As with other high-performance materials that are used in composites, however, one should keep in mind that direct comparisons with truly bulk materials, such as steel, should be viewed in the light that quite small quantities of nanomaterials may normally be actually used. Many actual products based on nanocomposites, for example, have only relatively low percentages (for example, 2% to 5%) of nanomaterials by weight. Many nano-based thin films or paints involve only small amounts as well and consequently can be competitively priced. On the other hand, the gross unit costs of
Costs decrease with volume
Cost per gram
useful polymeric, inorganic, and organic composite forms involving the use of dispersed carbon nanotubes in common liquids, including polymer resins, water, or various solvents, are inherently difficult to make due to the insolubility of carbon nanotubes.
F - 90% wt Costs increase with increasing purity and functionalization
90% wt 60% Wt 0
Number of grams
FIGURE 9.71 General cost variables for carbon nanotubes.
400 CHAPTER 9
Design Environments and Systems
Price per kg of engineering materials
Highly functionalized Diamond
Nanomaterials SWNTs MWNTs
Material price per unit mass ($/kg)
Al nitride PEEK
Stainless steels Mg alloys
Metals Al alloys
Glass Structural steel Oil
Nylons PMMA EVA, PS PP, PE
W carbide Boron carbide Silicon carbide
Technical ceramics and glasses
Structural composites GFRP
Alumina Pyrex Glass
C-steels Cast irons
Construction materials Timber Brick Concrete
FIGURE 9.72 Material price in US$/kg for common engineering materials and for typical nanomaterials. Costs for nanomaterials vary dramatically with the type of material, the degree of functionalization, and special processing needs for inclusion in products.
many technologically sophisticated and high-value products currently involving the use of nanomaterial or nanotechnologies are normally quite high. Interestingly, the current price of a very highend hearing aid that has a nanotechnology component is currently just under $1,000,000 per kilogram (mass: 2 grams, cost: $1800), and the price of a cobalt-chrome denture involving nanomateri-
Further Reading 401
als is $90,000 per kg, based on a similar calculation (mass: 20 grams)—thus the latter has costs similar to those of the hearing aid. Certainly this is suggestive of where many nanomaterials are most likely to find markets.
FURTHER READING General M. Addington and D. Schodek, Smart materials and technologies for the architecture and design professions, The Architectural Press, 2005. Michael F. Ashby, Materials Selection in mechanical design, 3rd ed., Elsevier Butterworth-Heinemann, 2005. Michael F. Ashby, Materials: Engineering, science, processing, and design, Elsevier, 2007. George Elvin, Nanotechnology for green building, Green Technology Forum, 2007 Charles Harper, Handbook of materials for product design, McGraw-Hill, 2001. Daniel Schodek and Martin Bechthold, Structures, 6th ed., Prentice-Hall, 2007. Benjamin Stein and John S. Reynolds, Mechanical and electrical equipment for buildings, 9th ed., John Wiley and Sons, 2000. Ben Walsh, Environmentally beneficial nanotechnologies: Barriers and technologies, Report to Food Department of Environment, Food and Rural Affairs, Oakdene Hollins, UK, 2007.
Environments and Systems L. Beranek and Istavan Ver, Noise and vibration control engineering, John Wiley & Sons, 1992. Advanced fenestration technology - Nanogel, Cabot Corporation, 2007. A.S. Edelstein and R.C. Cammarata (eds.), Nanomaterials: Synthesis, properties and applications, Institute of Physics Publishing, 2002. A European roadmap for photonics and nanotechnologies, MONA (Merging Optics and Nanotechnologies), 2007. Paolo Gardini, Sailing with the ITRS into nanotechnology, International Technology Roadmap for Semiconductors, 2006. Earnest Garrison, Solid oxide fuel cells, Science and Mathematics with Application of Relevant Technology (SMART) program, Illinois Institute of Technology, 2007. Hideo Hosono, Yoshinao Mishima, Hideo Takezoe, and Kenneth MacKenzie, Nanomaterials: Research towards applications, Elsevier, 2006. A. Inoue, Acta Mater 2000;48:279. W. L. Johnson, Material research bulletin 1999;24(10):42. Michael Moser, Engineering acoustics: An introduction to noise control, Springer-Verlag, 2004. Microstructured Materials Group, Silica aerogels, Lawrence Berkeley Laboratories, 2004. A European roadmap for photonics and nanotechnologies, MONA (Merging Optics and Nanotechnologies), 2007.
402 CHAPTER 9
Design Environments and Systems
William Lam and Christopher Ripman (eds.), Perception and lighting as formgivers for architecture, Van Nostrand Reinholt, 1992. Michel, Lou, Light: The shape of space: Designing with space and light, John Wiley and Sons, 1995 Nanogel—Cabot’s Nanogel technology, Cabot Corporation, 2007. A. Ortega, The engineering of small-scale systems: An NSF perspective, ITherm, San Diego, CA, 2006. C. H. Smith. In: H. H. Liebermann (ed.), Rapidly solidified alloys, processes, structures, properties, applications, Marcel Dekker, 1993. Marc G. Stanley, Competing for the future: Unlocking small wonders for tomorrow’s nanoelectronic uses, Advanced Technology Program, NIST, 2007. K. Sobolev, How nanotechnology can change the concrete world, American Ceramic Society Bulletin, Vol. 84, No. 11, November 2005. Harnessing materials for energy, MRS Bulletin, Vol. 33, No.4, April 2008. Fuel cells: Advanced rechargeable lithium batteries, MRS Bulletin, Vol. 27, No. 8, August 2002. Organic-based photovoltaics, MRS Bulletin, Vol. 30, No.1, January, 2005. Hydrogen storage, MRS Bulletin, Vol. 27, No. 9, September 2002.
CH A PTER 10
Nanomaterial Product Forms and Functions
10.1 CHARACTERIZING FORMS AND FUNCTIONS This chapter looks at many kinds of nanomaterials or nanotechnologies as they are commonly identified by product type, such as nanopaints, or by their function, such as antimicrobial. Many individuals and firms seek to characterize their research or products for either scientific or marketing purposes in a focused way and naturally make use of everyday descriptions that capture their essence. Indeed, they are often highly useful descriptors that bring alive the exciting intent of a product, such as a self-healing nanopaint, as well as being descriptive of general product form and application arena. These characterizations are thus usually related to highly specific nanoproduct types and applications and much less so to underlying physical or chemical phenomena. As we will see, however, there is considerable overlapping as well as simple confusion in the kinds of terminology used here. Do we really mean nanopaint, for example, or something like polymeric paints containing nanoparticles? Presumably the latter is a more correct description of what is actually meant—we certainly don’t mean “tiny paint”— but the language is surely more cumbersome. In this chapter, we describe research and products by the commonplace, if not always precise, language that is typically used. We draw a distinction between common types of nanomaterial properties and functional behaviors that might be the intention or application of a particular type of nanoproduct and the actual form of the nanoproduct itself. In the first instance, we have both property characteristics (e.g., mechanical, optical) and functional descriptors (e.g., self-cleaning or antimicrobial). In the second instance of product form, we have descriptors such as nanocoatings, Nanomaterials, Nanotechnologies and Design Copyright 2009 Elsevier Ltd. All rights of reproduction in any form reserved.
404 CHAPTER 10
Nanomaterial Product Forms and Functions
nanofilms, nanopaints, nanotextiles, and others. Obviously, different product forms can be described in terms of basic properties as well as possess one or more of the functional behaviors noted. Many nanoproduct forms, such as nanotextiles, possess multiple functional qualities—for example, antistaining and antimicrobial.
Functions in relation to primary properties
There is considerable difficulty and redundancy in describing various nanoproducts and functions in this way because of their overlapping and often ambiguous nature—for example, one person’s coating is another’s thin film. Figure 10.1 accepts these over-
Optical/light Sound Thermal Electromagnetic Chemical Self-healing Self-cleaning Antistaining
Antimicrobial Antibacterial Antifungal Antimold Antireflection Bonding/adhesion
FIGURE 10.1 Typical relationships among common nanoforms and nanoproducts and properties and functionalities that are important to designers and engineers.
The chart is not exhaustive; other product forms or functions could be listed as well, e.g., nanopowders, antistatic behavior, air or water purification.
Application relation Low
Characterizing Forms and Functions 405
laps and ambiguities and is simply a device for organizing the discussion in this chapter. The figure illustrates common characteristics and functionalities in relation to typical product forms. The vertical axis shows normal attribute or property characteristics of nanomaterials, that is, mechanical (strength, stiffness, etc.), thermal, optical, sound, chemical, and electromagnetic, and various functionalities (antibacterial and other). There has already been considerable discussion of property characteristics of nanomaterials in Chapters 6–9 and their role in product applications. There are also characteristics that are directly related to property attributes that involve words such as color changing or shape changing or other so-called “smart” actions. This chapter only briefly touches on these characteristics. Rather, we focus more on the kinds of functional behaviors listed in Figure 10.1. In the field there is considerable excitement about how nanomaterials can contribute to imparting different functional qualities of the type shown to various bulk materials. Our list of desired functionalities is abbreviated and could be easily extended to include many others—for example, antistatic, anticorrosive, and seemingly anti-anything. Other applications such as air or water purification could possibly be put here as well. Only selected functionalities, however, are examined in this chapter. The horizontal axis of Figure 10.1 shows various common product forms that can be obtained in bulk sizes and that can be used in various engineering, architecture, and product design applications. At left on the horizontal axis are primary forms of nanocomposites, in the middle are surface-oriented films and coatings, and on the right are special product forms. Not all product forms are shown. In particular, forms of nanoparticles or nanotubes that are fundamental constituents of other nanocomposite types, such as nanopowders or nanoclays, are not shown. These are indeed product forms, but they are essentially ingredients in more complex bulk forms that have immediate applications and are not treated here. The chart suggests that different product forms, such as nanopaints, can be described in terms of both their primary properties and intended functionalities. The color intensities on the chart do nothing more than broadly suggest common relationships as a guide for thinking about relationships. Thus, we have self-cleaning nanopaints or antimicrobial nanotextiles. The color variations on the chart are meant to be suggestive of the intensity of relationships only. Thus we see that the exploitation of optical properties and
406 CHAPTER 10
Nanomaterial Product Forms and Functions
phenomena are naturally done with nanoproducts that are primarily surface oriented, such as nanofilms; or, alternatively phrased, the purpose of many surface-oriented nanoproducts has to do with optical properties—self-cleaning, antimicrobial, and so forth. We also see that primary strength properties are normally a less important consideration in nanocoatings than are other properties. In the following sections, various functionalities and product types—selfcleaning, antimicrobial, and so forth—are explored. Specific forms are then discussed.
10.2 FUNCTIONAL CHARACTERISTICS The fundamental properties and related applications of nanomaterials and nanocomposites have already been discussed extensively in Chapters 6–9. The first part of this section initially looks at functional characteristics that are primarily, albeit not exclusively, related to surface behaviors. In designing or selecting materials, surface properties are of fundamental importance. Surfaces can now be designed to have many specific properties that are fundamentally important in the design and use of buildings and products. The general need and desire to keep surfaces clean and free of dirt has long been with us. Needs can stem from particular use applications. In medical facilities, the need to keep surfaces from contributing to the spread of bacteria is obvious—hence the need for surfaces that are easy to clean or that have antibacterial or antimicrobial properties. The very act of keeping surfaces clean continues to occupy enormous amounts of human energy; hence the need for selfcleaning surfaces. The need for antistaining surfaces on everything from walls and automotive seat covers to clothing hardly needs explanation. Problems of fungi or mold growth on surfaces, particularly in buildings, may not initially seem very high on any list of important problems, but many serious and recurrent health problems experienced by building occupants are known to be related to the presence of mold (the “sick building” syndrome) as well as other factors. Antifungal and antimold material characteristics are needed. Other functional needs related to surfaces include abrasion and scratch resistance. A successful quest for self-healing or self-repairing surfaces that recall similar behaviors in the skins of humans and animals would provide an enormous benefit to all. Materials with special behaviors related to light and color also have widespread applicability.
Functional Characteristics 407
Fundamental Approaches for Cleaning and Antimicrobial Actions Needs for achieving clean and hygienic surfaces have been with us for a long time, and many conventional material responses to them have achieved varying degrees of success. The use of nanomaterials for self-cleaning, antimicrobial, fungicidal, and related applications for various types of surfaces is more recent but has quickly become widespread. Most nano-based products intended for these applications use coatings, paints, or films that contain nanoparticles and that are applied or bonded to conventional materials. Some applications, however, have surface layers in which nanoparticles have been directly intermixed into the base material. Though many needs, such as cleaning or antifungal, may initially seem quite different, technological responses are often quite similar. Three primary technologies drive applications in these areas: the ability to make hydrophobic (water-repelling) surfaces, hydrophilic (water-attracting) surfaces, and photocatalytic surfaces. Nano-based approaches that invoke hydrophilic (water-repelling) action to spread water or hydrophobic action to bead water are widely used in achieving clean surfaces (see Figure 10.2). Nanomaterials with special photocatalytic properties that absorb ultraviolet (UV) energy that in turn causes dirt or other foreign particles on the surface to slowly loosen or break down via oxidation can aid in self-cleaning and can provide antimicrobial action. As we will see, actions such as self-cleaning can be accomplished in several ways and can be based on hydrophobic, hydrophilic, or photocatalytic means; these primary approaches can be combined in a variety of ways. Antimicrobial action can also be achieved via photocatalytic action or by making direct use of embedded nanomaterials such as copper that have intrinsic anti-microbial action, as we’ll discuss later. Prior to looking at specific applications in detail, it is useful to look at a common referent in nature to understand how certain types of cleaning actions can naturally occur. The lotus flower has long been a symbol of purity in Asian countries (see Figure 10.3). In the 1970s, two botanical researchers (Barthlott and Neinhuis, from the University of Bonn) noticed that the surfaces of the flower are rarely soiled, even as they arise from muddy lands, and that this effect could be observed in many plants that are covered in tiny wax structures that appeared to make the surfaces unwettable. Interestingly, using a scanning electron microscope (SEM) they found that the surfaces were not smooth. Conventional wisdom suggested that the smoother the surface, the less likely dirt was to adhere to it,
Hydrophobic (water repelling; drops form beads)
Hydrophilic (water attracting; drops flatten out)
Photocatalytic (UV-induced reactions that cause decomposition of dirt molecules) (a) Basic actions
(b) Water drop on hydrophobic surface
FIGURE 10.2 Basic approaches for self-cleaning, easy-cleaning, and antimicrobial functions. Some nanomaterials, e.g., copper, have intrinsic antimicrobial actions as well.
408 CHAPTER 10
Nanomaterial Product Forms and Functions
FIGURE 10.3 The lotus flower has long symbolized purity because of its self-cleaning activity, now known to be a result of hydrophobic action. Many plants exhibit this action. FIGURE 10.4 On superhydrophobic leaf surfaces, water droplets form spherical droplets that roll off easily, removing dirt particles as well. This is happening on the leaves of the Asiatic crop plant Colocasia esculenta, shown here. The papillae that are evident are about 5 to 10 micrometers high and are coated with a nanostructure of wax crystals. The photo was originally taken by Wilhelm’s Barthlott’s research group. (Courtesy of BASF.)
ct Ef fe
FIGURE 10.5 Self-cleaning action due to the Lotus Effect®. The rolling drops pick up dirt particles.
but, in the case of the lotus leaves, the surfaces had fairly rough micro- and nanostructures that imparted roughness to the surface. Several other plant leaves exhibit similar characteristics (see Figure 10.4). The roughness minimizes contact between a water drop and the leaf itself, and surface tension causes drops to form into beads while reducing the wetting of the surface itself. In the lotus flower leaf, the surface was found to be defined by cells of some 20 to 50 µm in size, with crystals of about 0.5–3 µm (500 to 3000 nm) in size. Barthlott and Neinhuis named this combination of effects the Lotus Effect.® The result of this effect is that water droplets bead up into spheres rather than spread. This characteristic is common in hydrophobic (water-repellant) surfaces (see the following discussion) or in oleophilic (oil-repellent) surfaces. These droplets then roll off the surface easily. As they roll, dirt particles cling to the beads and are removed with them as the beads roll off; hence a natural “self-cleaning” action occurs (see Figure 10.5). The hydrophobic (water repellent) action we’ve mentioned can be contrasted with a hydrophilic (water-attracting) action. The amount of wetting that occurs on a surface depends on what action is present, which is in turn dependent on the various interfacial energies between the water droplet, the solid surface, and the surround-
Functional Characteristics 409
ing environment. As suggested in Figure 10.6, three primary surface tension factors influence the shape of a water droplet. The relative magnitude of these tensions influence the value of the “contact angle” (θ). If the value of this angle is 90° or more, the surface is generally termed hydrophobic. Smaller angles of less than 90° are hydrophilic.
Liquid-to-solid surface tension
Liquid drop IV
90° > q > 0° IS
High wetting of surface
q >90° q
Reduced wetting of surface
q ≥150° SV
Superhydrophobic surfaces (a)
Another important variable in a self-cleaning surface is the contact angle (θ) between the water drop and the surface. The lotus flower surface has a localized contact angle of about 160°. Keep in mind FIGURE 10.6 Factors affecting how much a liquid wets a surface. (Photo courtesy of BASF.)
Liquid-to-vapor surface tension
SV : Solid-to-vapor surface tension
Generally, if the surface tension of the solid surface is greater than that of the liquid, drops will spread and surface wetting will occur; if the critical surface tension of the solid is less than that of the liquid, the water droplet will be repelled. Note that the contact area between the water droplet and surface is minimized in hydrophobic surfaces. Relative surface tensions can in turn be influenced by the presence of surface bumps or roughness, which in turn opens the way for using nanomaterials to affect whether the surfaces of a material are hydrophobic or hydrophilic. Surfaces with a contact angle of greater than 150° are called superhydrophobic (180° is obviously the upper bound). Making surfaces either superhydrophobic or superhydrophillic are goals of nanomaterial research in this area. A first basic approach to making surfaces self-cleaning is to use nanosurfaces designed with roughness characteristics that serve similar functions to those in self-cleaning plants associated with the Lotus Effect®, which is in turn based on hydrophobic (waterrepellant) action. Dirt or other foreign particles are picked up by a water droplet if the force that picks up the particle is greater than the electrostatic force between the particle and the surface. One important variable is the surface roughness. With particular surface roughnesses, the contact area between the particle and the surface is minimized, thus minimizing the force needed to remove the particle. With some roughness patterns, tiny air bubbles can become trapped between the water drops and the surface that can, in turn, enhance the water-repellant properties of the surface and the related cleaning action (see Figure 10.7). This occurs when the energy needed to wet a hydrophobic surface with water exceeds that needed to “wet” the solid surface with air. In this case the liquid drop will try to minimize its contact area with the solid, which in turn can leave air pockets beneath the drop.
410 CHAPTER 10
Nanomaterial Product Forms and Functions
FIGURE 10.7 Hydrophobic (water-repelling) action due to surface roughness. Nanopatterns can reduce the contact area and increase hydrophobic behavior.
Oxidized Unpaired electron UV Light
Titanium dioxide coating
that though our discussion has constantly referred to the lotus flower surface, many materials can be engineered to produce equivalent surface structures. Teflon, for example, intrinsically has a relatively high localized contact angle (115°) for water, which intrinsically gives it some of these properties and can be altered to have even higher contact angle values. Note that though references have been made to water droplets only, the actual contact angles vary depending on what liquid is used as well as what solid surface is present. This dependency is significant when liquids other than water are important. Oleophylic surfaces, for example, repel oil. A second approach involving water-repellant actions involves extremely smooth, surfaces (not rough), which is fundamentally quite different from the Lotus Effect® cleaning action. With highly smooth surfaces, there is a decrease in the surface energy of the surface and consequently a lower force of surface attraction, which again causes water beads to form. Surfaces based specifically on this action are easy to clean and resistant to dirt buildup. They are not intrinsically self-cleaning in the sense we’ve described, albeit natural actions such as rain can aid in washing away dirt particles from sloped or vertical surfaces. Surfaces of this type are widely used in locations where easy cleaning is important, such as bathroom fixtures. In these approaches, the objective is to use the waterattraction characteristic to develop a thin sheetlike film of water that can be largely transparent and that aids in surface washing and cleaning. Hydrophilic surfaces also form the basis for some “antifogging” applications. The third major action of interest here is photocatalysis, a naturally occurring process that happens when certain materials are exposed to ultraviolet (UV) UV light. It is one of the most fundamental approaches used to enable many functional behaviors, including self-cleaning and antimicrobial actions. Later we will see that photocatalytic approaches are also used for many other applications, such as air purification.
Freed electron Loosened / decomposed material
FIGURE 10.8 Photocatalytic action. Photocatalysis can aid in self-cleaning and antibacterial activity and in the reduction of pollutants in the air.
The photocatalysis process can be initiated by UV light present in normal sunlight or from any other kind of UV light source. The process causes oxidizing reagents to form that in turn cause the decomposition of many organic substances that are deposited on or that form on surfaces (see Figure 10.8). Titanium dioxide (TiO2) or zinc oxides are often used as photocatalytic materials. They are relatively inexpensive and respond well to UV light. For many self-
Functional Characteristics 411
cleaning applications, titanium oxide (TiO2) nanoparticles that are in their anatase form (one of the three forms of titanium oxide) are used due to their photocatalytic properties. Exposure to UV radiation produces electron-hole pairs in the material. The free radicals or electrons that result react with foreign substances on the surface and produce chemical reactions that ultimately decompose the foreign substances through oxidation. Organic matter can be quickly decomposed. The loosened and decomposed material can then be washed away by normal rainfall or other means. Since bacteria formation is associated with organic matter, the washing away of this matter also causes the surfaces to have antibacterial qualities. As we discuss more later, the same photocatalytic effect can also reduce pollutants in the air. Most photocatalytic processes are activated by UV wavelengths that are commonly present in sunlight. Wavelengths in the UV range, however, constitute only a narrow portion of the sunlight spectrum. Increased photocatalytic efficiencies can be envisioned if activated by other wavelengths as well. Considerable research is under way to find nanosubstances that exhibit photocatalytic properties when subjected to a broader range of wavelengths. The three major actions discussed—hydrophobicity, hydrophilicity, and photocatalysis—form the basis of current easy-cleaning, self-cleaning, and antimicrobial surfaces. The surfaces can form on glasses, tiles, enameled panels, and other hosts (see the following discussion). They also can have overlapping actions. Of particular interest here are photocatalytic surfaces made using titanium dioxide (TiO2). These same surfaces have high surface energies and hence have been found to exhibit hydrophilic behaviors where water forms into thin films rather than beading. This combined behavior is very useful and has been exploited in many products, including the so-called self-cleaning glasses we’ll discuss in a moment. Specific applications in glasses, tiles, paints, textiles, and other product forms will be discussed shortly. It is important to observe that the use circumstance can dictate which approach is used. Photocatalytic processes now based only on UV light are obviously primarily suitable for exterior, not interior, surfaces where sunlight is present. Products based on the Lotus Effect® are best used where there is frequent general washing from rain or other sources; otherwise streaks can develop. Many surfaces are particularly sensitive to degradation when exposed to the kinds of disinfectants commonly used in cleaning. (This is a particular problem in
412 CHAPTER 10
Nanomaterial Product Forms and Functions
medical settings.) Abrasions can also occur that destroy surface characteristics.
Self-Cleaning and Easy-Cleaning Materials Self-cleaning and easy-cleaning glasses and tiles In architecture, the primary intended cleaning action is the removal of everyday dirt, dust, or other things that naturally appear on windows or other surfaces in buildings. So-called self-cleaning glasses for use in windows in buildings or vehicles as shown in Figures 10.9 and 10.10 are now made by a number of major glass-producing companies (e.g., Pilkington, Saint Gobain, and others). Similar glasses are made for vehicles and other applications. In most products, related objectives include killing bacteria or fungi that develop on surfaces and breaking down pollutants or compounds that can cause discolorations.
FIGURE 10.9 The Beach House, by Malcolm Carver. (Courtesy of Pilkington.)
FIGURE 10.10 A self-cleaning glass that exhibits both photocatalytic and hydrophilic actions is used in the Beach House. (Courtesy of Pilkington.)
In glasses, the self-cleaning action normally comes from coatings with thicknesses at the nanoscale that have particular photocatalytic and hydrophilic (water-attracting) properties. In several applications, the glass is first coated with a photocatalytic material, normally titanium dioxide (TiO2). The photocatalytic coatings produce chemical reactions (described previously) when subjected to ultraviolet (UV) light that help in oxidizing foreign substances and decomposing them. Coating thicknesses are on the order of 15 nm—and are transparent. Titanium dioxide is normally white, and thicknesses need to be restricted to obtain the needed transparency for glass. When the surface is subjected to rain or simple washing, hydrophilic action then causes the water to form into thin, flat sheets (without large droplets). In hydrophilic action, water droplets hitting the surface of the coated glass attract each other, thus forming thin sheets. Surface drainage is enhanced (as is subsequent surface drying). The water sheet carries off the loosened dirt particles (see Figure 10.11). Since organic matter is decomposed, these same coatings also have positive antistaining and antibacterial properties. Coatings of the type described have been aggressively developed by a number of major glass product manufacturers and have begun to be widely utilized in real applications. The application to glass shown in Figure 10.9 uses a glass produced by Pilkington. This product is often noted as an application of “nanomaterials.” For this product, the company is quite clear about whether or not its product should be described as a nanomaterial or nanotechnology—it should not. This positioning is interesting and worth
Functional Characteristics 413
looking into in light of the definitional and nomenclature problems first noted in Chapter 6. According to a quote provided by Dr. Kevin Sanderson, principal project manager from the On-Line Coatings Technology Group, Pilkington Activ has been described as an example of nanotechnology. Due to the coatings’ thickness, Pilkington Activ does fall under certain nanotechnology definitions, e.g., IUPAC. It is critical to understand, however, that the reason we fall under this description of nanotechnology is that the thickness of the coating is